Upcoming SlideShare
×

Thanks for flagging this SlideShare!

Oops! An error has occurred.

×
Saving this for later? Get the SlideShare app to save on your phone or tablet. Read anywhere, anytime – even offline.
Standard text messaging rates apply

# Fundamentals modern-manufacturing-4th-solution-manual

3,892

Published on

Selling this solutions …

Selling this solutions
Thank you

1 Comment
7 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No

Are you sure you want to  Yes  No
Views
Total Views
3,892
On Slideshare
0
From Embeds
0
Number of Embeds
0
Actions
Shares
0
0
1
Likes
7
Embeds 0
No embeds

No notes for slide

### Transcript

• 1. SOLUTION MANUAL
• 12. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 Flow Curve 3.4 In Problem 3.3, determine the strength coefficient and the strain-hardening exponent in the flow curve equation. Be sure not to use data after the point at which necking occurred. Solution: Starting volume of test specimen V = 125(62.5) = 7812.5 mm3 . Select two data points: (1) F = 23042 N and L = 131.25 mm; (2) F = 28913 N and L = 147.01 mm. (1) A = V/L = 7812.5/131.25 = 59.524 mm2 . Stress σ = 23042/59.524 = 387.1 MPa. Strain ε = ln(131.25/125) = 0.0488 (2) A = 7812.5/147.01 = 53.143 mm2 . Stress σ = 28913/53.143 = 544.1 MPa. Strain ε = ln(147.01/125) = 0.1622 Substituting these values into the flow curve equation, we have (1) 387.1 = K(0.0488)n and (2) 544.1 = K(0.1622)n 544.1/387.1 = (0.1622/0.0488)n 1.4056 = (3.3238)n ln(1.4056) = n ln(3.3238) 0.3405 = 1.2011 n n = 0.283 Substituting this value with the data back into the flow curve equation, we obtain the value of the strength coefficient K: K = 387.1/(0.0488).283 = 909.9 MPa K = 544.1/(0.1622).283 = 910.4 MPa Use average K = 910.2 MPa The flow curve equation is: σ = 910.2 ε0.283 3.5 In a tensile test on a metal specimen, true strain = 0.08 at a stress = 265 MPa. When true stress = 325 MPa, true strain = 0.27. Determine the strength coefficient and the strain-hardening exponent in the flow curve equation. Solution: (1) 265 = K(0.08)n and (2) 325 = K(0.27)n 325/265 = (0.27/0.08)n 1.2264 = (3.375)n n ln(3.375) = ln(1.2264) 1.2164 n = 0.2041 n = 0.1678 Substituting this value with the data back into the flow curve equation, we obtain the value of the strength coefficient K: (1) K = 265/(0.08).1678 = 404.85 MPa (2) K = 325/(0.27).1678 = 404.85 MPa The flow curve equation is: σ = 404.85 ε0.1678 3.6 During a tensile test, a metal has a true strain = 0.10 at a true stress = 37,000 lb/in2 . Later, at a true stress = 55,000 lb/in2 , true strain = 0.25. Determine the strength coefficient and strain-hardening exponent in the flow curve equation. Solution: (1) 37,000 = K(0.10)n and (2) 55,000 = K(0.25)n 55,000/37,000 = (0.25/0.10)n 1.4865 = (2.5)n n ln(2.5) = ln(1.4865) 0.9163 n = 0.3964 n = 0.4326 Substituting this value with the data back into the flow curve equation, we obtain the value of the strength coefficient K: (1) K = 37,000/(0.10)0.4326 = 100,191 lb/in2 (2) K = 55,000/(0.25)0.4326 = 100,191 lb/in2 The flow curve equation is: σ = 100,191 ε0.4326
• 13. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 3.7 In a tensile test a metal begins to neck at a true strain = 0.28 with a corresponding true stress = 345.0 MPa. Without knowing any more about the test, can you estimate the strength coefficient and the strain-hardening exponent in the flow curve equation? Solution: If we assume that n = ε when necking starts, then n = 0.28. Using this value in the flow curve equation, we have K = 345/(0.28).28 = 492.7 MPa The flow curve equation is: σ = 492.7 ε0.28 3.8 A tensile test for a certain metal provides flow curve parameters: strain-hardening exponent is 0.3 and strength coefficient is 600 MPa. Determine (a) the flow stress at a true strain = 1.0 and (b) true strain at a flow stress = 600 MPa. Solution: (a) Yf = 600(1.0).3 = 600 MPa (b) ε = (600/600)1/.3 = (1.0)3.33 = 1.00 3.9 The flow curve for a certain metal has a strain-hardening exponent of 0.22 and strength coefficient of 54,000 lb/in2 . Determine (a) the flow stress at a true strain = 0.45 and (b) the true strain at a flow stress = 40,000 lb/in2 . Solution: (a) Yf = 54,000(0.45).22 = 45,300 lb/in2 (b) ε = (40,000/54,000)1/.22 = (0.7407)4.545 = 0.256 3.10 A metal is deformed in a tension test into its plastic region. The starting specimen had a gage length = 2.0 in and an area = 0.50 in2 . At one point in the tensile test, the gage length = 2.5 in, and the corresponding engineering stress = 24,000 lb/in2 ; at another point in the test prior to necking, the gage length = 3.2 in, and the corresponding engineering stress = 28,000 lb/in2 . Determine the strength coefficient and the strain-hardening exponent for this metal. Solution: Starting volume V = LoAo = 2.0(0.5) = 1.0 in3 (1) A = V/L = 1.0/2.5 = 0.4 in2 So, true stress σ = 24,000(0.5)/0.4 = 31,250 lb/in2 and ε = ln(2.5/2.0) = 0.223 (2) A = 1.0/3.2 = 0.3125 in2 So, true stress σ = 28,000(0.5)/0.3125 = 44,800 lb/in2 and ε = ln(3.2/2.0) = 0.470 These are two data points with which to determine the parameters of the flow curve equation. (1) 31,250 = K(0.223)n and (2) 44,800 = K(0.470)n 44,800/31,250 = (0.470/0.223)n 1.4336 = (2.1076)n ln(1.4336) = n ln(2.1076) 0.3602 = .7455 n n = 0.483 (1) K = 31,250/(0.223).483 = 64,513 lb/in2 (2) K = 44,800/(0.470).483 = 64,516 lb/in2 Use average K = 64,515 lb/in2 The flow curve equation is: σ = 64,515 ε0.483 3.11 A tensile test specimen has a starting gage length = 75.0 mm. It is elongated during the test to a length = 110.0 mm before necking occurs. Determine (a) the engineering strain and (b) the true strain. (c) Compute and sum the engineering strains as the specimen elongates from: (1) 75.0 to 80.0 mm, (2) 80.0 to 85.0 mm, (3) 85.0 to 90.0 mm, (4) 90.0 to 95.0 mm, (5) 95.0 to 100.0 mm, (6) 100.0 to 105.0 mm, and (7) 105.0 to 110.0 mm. (d) Is the result closer to the answer to part (a) or part (b)? Does this help to show what is meant by the term true strain? Solution: (a) Engineering strain e = (110 - 75)/75 = 35/75 = 0.4667
• 14. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 (b) True strain ε = ln(110/75) = ln(1.4667) = 0.383 (c) (1) L = 75 to 80 mm: e = (80 - 75)/75 = 5/75 = 0.0667 (2) L = 80 to 85 mm: e = (85 - 80)/80 = 5/80 = 0.0625 (3) L = 85 to 90 mm: e = (90 - 85)/85 = 5/85 = 0.0588 (4) L = 90 to 95 mm: e = (95 - 90)/90 = 5/90 = 0.0556 (5) L = 95 to 100 mm: e = (100 - 95)/95 = 5/95 = 0.0526 (6) L = 100 to 105 mm: e = (105 - 100)/100 = 5/100 = 0.0500 (7) L = 105 to 110 mm: e = (110 - 105)/105 = 5/105 = 0.0476 _____________________________________________ Sum of incremental engineering strain values = 0.3938 (d) The resulting sum in (c) is close to the true strain value in (b). The summation process is an approximation of the integration over the range from 75 to 110 mm in (b). As the interval size is reduced, the summation becomes closer to the integration value. 3.12 A tensile specimen is elongated to twice its original length. Determine the engineering strain and true strain for this test. If the metal had been strained in compression, determine the final compressed length of the specimen such that (a) the engineering strain is equal to the same value as in tension (it will be negative value because of compression), and (b) the true strain would be equal to the same value as in tension (again, it will be negative value because of compression). Note that the answer to part (a) is an impossible result. True strain is therefore a better measure of strain during plastic deformation. Solution: Engineering strain e = (2.0 - 1.0)/1.0 = 1.0 True strain ε = ln(2.0/1.0) = ln(2.0) = 0.693 (a) To be compressed to the same engineering strain (e = -1.0) the final height of the compression specimen would have to be zero, which is impossible. (b) To be compressed to the same true strain value (e = -0.693) the final height of the compression specimen can be determined as follows: ε = -.693 = ln(Lf/Lo) Lf/Lo = exp.(-0.693) = 0.500 Therefore, Lf = 0.5 Lo 3.13 Derive an expression for true strain as a function of D and Do for a tensile test specimen of round cross section, where D = the instantaneous diameter of the specimen and Do is its original diameter. Solution: Starting with the definition of true strain as ε = ln(L/Lo) and assuming constant volume, we have V = AoLo = AL Therefore, L/Lo = Ao/A A = πD2 and Ao = πDo 2 Ao/A = πDo 2 /πD2 = (Do/D)2 ε = ln(Do/D)2 = 2 ln(Do/D) 3.14 Show that true strain = ln(1 + e), where e = engineering strain. Solution: Starting definitions: (1) ε = ln(L/Lo) and (2) e = (L - Lo)/Lo Consider definition (2): e = L/Lo - Lo/Lo = L/Lo - 1 Rearranging, 1 + e = L/Lo Substituting this into definition (1), ε = ln(1 + e) 3.15 Based on results of a tensile test, the flow curve strain-hardening exponent = 0.40 and strength coefficient = 551.6 MPa. Based on this information, calculate the (engineering) tensile strength for the metal.
• 15. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 Solution: Tensile strength occurs at maximum value of load. Necking begins immediately thereafter. At necking, n = ε. Therefore, σ = 551.6(0.4)0.4 = 382.3 MPa. This is a true stress. TS is defined as an engineering stress. From Problem 3.15, we know that ε = 2 ln(Do/D). Therefore, 0.4 = 2 ln(Do/D) ln(Do/D) = .4/2 = 0.2 Do/D = exp(0.2) = 1.221 Area ratio = (Do/D)2 = (1.221)2 = 1.4918 The ratio between true stress and engineering stress would be the same ratio. Therefore, TS = 1.4918(382.3) = 570.3 MPa 3.16 A copper wire of diameter 0.80 mm fails at an engineering stress = 248.2 MPa. Its ductility is measured as 75% reduction of area. Determine the true stress and true strain at failure. Solution: Area reduction AR = (Ao - Af)/Ao = 0.75 Ao - Af = 0.75 Ao Ao - 0.75Ao = 0.25 Ao = Af If engineering stress = 248.2 MPa, then true stress σ = 248.2/0.25 = 992.8 MPa True strain ε = ln(Lf/Lo) = ln(Ao/Af) = ln(4) = 1.386. However, it should be noted that these values are associated with the necked portion of the test specimen. 3.17 A steel tensile specimen with starting gage length = 2.0 in and cross-sectional area = 0.5 in2 reaches a maximum load of 37,000 lb. Its elongation at this point is 24%. Determine the true stress and true strain at this maximum load. Solution: Elongation = (L - Lo)/Lo = 0.24 L - Lo = 0.24 Lo L = 1.24 Lo A = Ao/1.24 = 0.8065 Ao True stress σ = 37,000/0.8065(0.5) = 91,754 lb/in2 True strain ε = ln(1.24) = 0.215 Compression 3.18 A metal alloy has been tested in a tensile test with the following results for the flow curve parameters: strength coefficient = 620.5 MPa and strain-hardening exponent = 0.26. The same metal is now tested in a compression test in which the starting height of the specimen = 62.5 mm and its diameter = 25 mm. Assuming that the cross section increases uniformly, determine the load required to compress the specimen to a height of (a) 50 mm and (b) 37.5 mm. Solution: Starting volume of test specimen V = πhDo 2 /4 = 62.5π(25)2 /4 = 30679.6 mm3 . (a) At h = 50 mm, ε = ln(62.5/50) = ln(1.25) = 0.223 Yf = 620.5(.223).26 = 420.1 MPa A = V/L = 30679.6/50 = 613.6 mm2 F = 420.1(613.6) = 257,770 N (b) At h = 37.5 mm, ε = ln(62.5/37.5) = ln(1.667) = 0.511 Yf = 620.5(0.511).26 = 521.1 MPa A = V/L = 30679.6 /37.5 = 818.1 mm2 F = 521.1(818.1) = 426,312 N 3.19 The flow curve parameters for a certain stainless steel are strength coefficient = 1100 MPa and strain- hardening exponent = 0.35. A cylindrical specimen of starting cross-sectional area = 1000 mm2 and height = 75 mm is compressed to a height of 58 mm. Determine the force required to achieve this compression, assuming that the cross section increases uniformly.
• 18. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 11 Viscosity of Fluids 3.28 Two flat plates, separated by a space of 4 mm, are moving relative to each other at a velocity of 5 m/sec. The space between them is occupied by a fluid of unknown viscosity. The motion of the plates is resisted by a shear stress of 10 Pa due to the viscosity of the fluid. Assuming that the velocity gradient of the fluid is constant, determine the coefficient of viscosity of the fluid. Solution: Shear rate = (5 m/s x 1000 mm/m)/(4 mm) = 1250 s-1 η = (10N/m2 )/(1250 s-1 ) = 0.008 N-s/m2 = 0.008 Pa-s 3.29 Two parallel surfaces, separated by a space of 0.5 in that is occupied by a fluid, are moving relative to each other at a velocity of 25 in/sec. The motion is resisted by a shear stress of 0.3 lb/in2 due to the viscosity of the fluid. If the velocity gradient in the space between the surfaces is constant, determine the viscosity of the fluid. Solution: Shear rate = (25 in/sec)/(0.5 in) = 50 sec-1 η = (0.3 lb/in2 )/(50 sec-1 ) = 0.0006 lb-sec/in2 . 3.30 A 125.0-mm-diameter shaft rotates inside a stationary bushing whose inside diameter = 125.6 mm and length = 50.0 mm. In the clearance between the shaft and the bushing is a lubricating oil whose viscosity = 0.14 Pa-s. The shaft rotates at a velocity of 400 rev/min; this speed and the action of the oil are sufficient to keep the shaft centered inside the bushing. Determine the magnitude of the torque due to viscosity that acts to resist the rotation of the shaft. Solution: Bushing internal bearing area A = π(125.6)2 x 50/4 = 19729.6 mm2 = 19729.2(10-6 ) m2 d = (125.6 - 125)/2 = 0.3 mm v = (125π mm/rev)(400 rev/min)(1 min/60 sec) = 2618.0 mm/s Shear rate = 2618/0.3 = 8726.6 s-1 τ = (0.14)(8726.6) = 1221.7 Pa = 1221.7 N/mm2 Force on surface between shaft and bushing = (1221.7 N/mm2 )(19729.2(10-6 )) = 24.1 N Torque T = 24.1 N x 125/2 mm = 1506.4 N-mm = 1.506 N-m
• 21. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-03-09, 03-03-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3 Problems 4.1 The starting diameter of a shaft is 25.00 mm. This shaft is to be inserted into a hole in an expansion fit assembly operation. To be readily inserted, the shaft must be reduced in diameter by cooling. Determine the temperature to which the shaft must be reduced from room temperature (20°C) in order to reduce its diameter to 24.98 mm. Refer to Table 4.1. Solution: For steel, α = 12(10-6 ) mm/mm/°C according to Table 4.1. Revise Eq. (4.1) to D2 - D1 = αD1 (T2 - T1). 24.98 - 25.00 = 12(10-6 )(25.00)(T2 - 20) -0.02 = 300(10-6 )(T2 - 20) -0.02 = 0.0003(T2 - 20) = 0.0003T2 - 0.006 -.02 + 0.006 = 0.0003T2 -0.014 = 0.0003T2 T2 = -46.67°C 4.2 A bridge built with steel girders is 500 m in length and 12 m in width. Expansion joints are provided to compensate for the change in length in the support girders as the temperature fluctuates. Each expansion joint can compensate for a maximum of 40 mm of change in length. From historical records it is estimated that the minimum and maximum temperatures in the region will be -35°C and 38°C, respectively. What is the minimum number of expansion joints required? Solution: Assume L1 =500 m at -35 C, α=12x10-6 /C L2 – L1 = αL1(T2 – T1) L2 – L1 = 12x10-6 (500)(38 – (-35)) L2 – L1 = 0.42 m Each expansion joint will control 40 mm = 0.04 m of expansion. 10 joints will provide 0.40 m of expansion. 11 joints will provide 0.45 m of expansion. Therefore, a minimum of 11 joints are needed for coverage of the total length. Each bridge section will be 500/11 = 45.5 m long. 4.3 Aluminum has a density of 2.70 g/cm3 at room temperature (20°C). Determine its density at 650°C, using data in Table 4.1 as a reference. Solution: Assume a 1 cm3 cube, 1 cm on each side. From Table 4.1, α = 24(10-6 ) mm/mm/°C L2 - L1 = αL1 (T2 - T2). L2 = 1.0 + 24(10-6 )(1.0)(650 - 20) = 1.01512 cm (L2 )3 = (1.01512)3 = 1.04605 cm3 Assume weight remains the same; thus ρ at 650°C = 2.70/1.04605 = 2.581 g/cm3 4.4 With reference to Table 4.1, determine the increase in length of a steel bar whose length = 10.0 in, if the bar is heated from room temperature of 70°F to 500°F. Solution: Increase = (6.7 x 10-6 in/in/F)(10.0 in)(500°F - 70°F) = 0.0288 in. 4.5 With reference to Table 4.2, determine the quantity of heat required to increase the temperature of an aluminum block that is 10 cm x 10 cm x 10 cm from room temperature (21°C) to 300°C. Solution. Heat = (0.21 cal/g-°C)(103 cm3 )(2.70 g/cm3 )(300°C - 21°C) = 158,193 cal. Conversion: 1.0 cal = 4.184J, so heat = 662,196 J. 4.6 What is the resistance R of a length of copper wire whose length = 10 m and whose diameter = 0.10 mm? Use Table 4.3 as a reference. Solution: R = rL/A, A = π(0.1)2 /4 = 0.007854 mm2 = 0.007854(10-6 ) m2 From Table 4.3, r = 1.7 x 10-8 Ω-m2 /m
• 22. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-03-09, 03-03-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 4 R = (1.7 x 10-8 Ω-m2 /m)(10 m)/( 0.007854(10-6 ) m2 ) = 2164.5(10-2 ) Ω = 21.65 Ω 4.7 A 16 gage nickel wire (0.0508-in diameter) connects a solenoid to a control circuit that is 32.8 ft away. (a) What is the resistance of the wire? Use Table 4.3 as a reference. (b) If a current was passed through the wire, it would heat up. How does this affect the resistance? Solution: (a) L = 32.8 ft = 393.6 in Area A = π(0.0508)2 /4 = 0.00203 in2 R = r (L/A) = 6.8 x 10-8 (39.4)(393.6/0.00203) = 0.520 ohm (b) If a current is passed through the wire causing the wire to heat up, the resistivity of the wire would change. Since nickel is a metal, the resistivity would increase, causing the resistance to increase. This, in turn, would cause slightly more heat to be generated. 4.8 Aluminum wiring was used in many homes in the 1960s due to the high cost of copper at the time. Aluminum wire that was 12 gauge (a measure of cross-sectional area) was rated at 15 A of current. If copper wire of the same gauge were used to replace the aluminum wire, what current should the wire be capable of carrying if all factors except resistivity are considered equal? Assume that the resistance of the wire is the primary factor that determines the current it can carry and the cross- sectional area and length are the same for the aluminum and copper wires. Solution: The area and length are constant between the types of wires. The overall change in resistance is due to the change in resistivity of the materials. From Table 4.3: For Aluminum r = 2.8 x 10-8 For Copper r = 1.7 x 10-8 The resistance will reduce by 1.7x10-8 /2.8x10-8 = 0.61 Since I = E/R and Rcu=0.61(Ral), then Icu = 1/0.61*Ial = 15/0.61= 25 A Note that the code value is actually 20 A due to several factors including heat dissipation and rounding down to the nearest 5 amp value.
• 27. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 11-11-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 5.5 A sine bar is used to determine the angle of a part feature. The length of the sine bar is 6.000 in. The rolls have a diameter of 1.000 in. All inspection is performed on a surface plate. In order for the sine bar to match the angle of the part, the following gage blocks must be stacked: 2.0000, 0.5000, 0.3550. Determine the angle of the part feature. Solution: H = 2.0000+0.5000 + 0.3550 = 2.8550 in A = sin-1 (H/L) = sin-1 (2.8550/6.000 ) = sin-1 ( 0.4758 ) = 28.41° 5.6 A 200.00 mm sine bar is used to inspect an angle on a part. The angle has a dimension of 35.0 ± 1.8°. The sine bar rolls have a diameter of 30.0 mm. A set of gage blocks is available that can form any height from 10.0000 to 199.9975 mm in increments of 0.0025 mm. Determine (a) the height of the gage block stack to inspect the minimum angle, (b) height of the gage block stack to inspect the maximum angle, and (c) smallest increment of angle that can be setup at the nominal angle size. All inspection is performed on a surface plate. Solution: (a) sin A = (H/L); H = L sin A = 200.00 Sin (35.0-1.8) = 200.00 sin 33.2 = 109.51264 = 109.5150 mm (must round up to insure angle is in tolerance. (b) H = L sin A = 200.00 sin (35.0 + 1.8) = 200.00 sin (36.8) = 119.80472 = 119.8025 mm (must round down to insure angle within dimensions) (c) H at nominal angle = L sin A = 200.00 Sin (35.0) = 114.7152 mm Closest angle to nominal is at H=114.7150; A = sin-1 (H/L) = sin-1 (114.7150/200.000) A = sin-1 (0.573575) = 34.99989953° At one increment above, H=114.7175; A = sin-1 (H/L) = sin-1 (114.7175/200.000 ) = A = sin-1 (0.5735875) = 35.00077385° Change in A = 35.00077385 – 34.9989953 = 0.0008743°
• 32. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 01-03-09, 01-03-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 6.2 For the preceding problem, use the inverse lever rule to determine the proportions of liquid and solid phases present in the alloy. Solution: From Fig 6.2, measured values of CL and CS are: CL = 5 mm, CS = 12 mm. Liquid phase proportion = 12/(12 + 5) = 12/17 = 0.71 Solid phase proportion = 5/17 = 0.29 6.3 Using the lead-tin phase diagram in Figure 6.3, determine the liquid and solid phase compositions for a nominal composition of 40% Sn and 60% Pb at 204°C (400°F). Solution: From Fig 6.3, the compositions are observed as follows: Liquid phase composition = 56% Sn - 44% Pb. α phase composition = 18% Sn - 82% Pb. 6.4 For the preceding problem, use the inverse lever rule to determine the proportions of liquid and solid phases present in the alloy. Solution: From Fig 6.3, measured values of CL and CS are: CL = 10.5 mm, CS = 15 mm. Liquid phase proportion = 15/(15 + 10.5) = 15/25.5 = 0.59 α phase proportion = 10.5/25.5 = 0.41 6.5 Using the lead-tin phase diagram in Figure 6.3, determine the liquid and solid phase compositions for a nominal composition of 90% Sn and 10% Pb at 204°C (400°F). Solution: From Fig 6.3, the compositions are observed as follows: Liquid phase composition = 78% Sn - 22% Pb. β phase composition = 98% Sn - 2% Pb. 6.6 For the preceding problem, use the inverse lever rule to determine the proportions of liquid and solid phases present in the alloy. Solution: From Fig 6.3, measured values of CL and CS are: CL = 7.8 mm, CS = 4.2 mm. Liquid phase proportion = 4.2/(13) = 0.32 α phase proportion = 7.8/13 = 0.68 6.7 In the iron-iron carbide phase diagram of Figure 6.4, identify the phase or phases present at the following temperatures and nominal compositions: (a) 650°C (1200°F) and 2% Fe3C, (b) 760°C (1400°F) and 2% Fe3C, and (c) 1095°C (2000°F) and 1% Fe3C. Solution: (a) Alpha + iron carbide, (b) gamma + iron carbide, and (c) gamma.
• 43. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-12-09, 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 4 are no voids in the composite. Determine the (a) mass of vinyl ester in the section, (b) mass of E- glass fibers in the section, and (c) the density of the composite. Solution: Volume V = (1.00 cm)(50.00 cm)(200.00 cm) = 10,000 cm3 (a) Vm = fm (Vc) = 0.650(10,000 cm3 ) = 6,500 cm3 mm = 6500 cm3 (0.882 g/cm3 ) = 5733 g (b) Vr = fr (Vc) = 0.350(10,000 cm3 ) = 3,500 cm3 mr = 3500 cm3 (2.60 g/cm3 ) = 9100 g (c) ρc = = fm ρm + fr ρr = 0.650(0.882) + 0.350(2.60) = 1.48 g/cm3 9.2 For problem 9.1, determine the modulus of elasticity in (a) the longitudinal direction of the glass fibers and (b) the perpendicular direction to the glass fibers. Solution: fm = 0.650, fr = 0.350, Em = 3.60 GPa, and Er = 76.0 GPa (a) Ec = fmEm + frEr Ec = 0.650(3.60) + 0.350(76.0) = 28.9 GPa (b) Ec’ = EmEr/(fmEr + frEm) Ec’ = 3.60(76.0)/(0.650(76.0) + 0.350(3.60)) = 5.40 GPa 9.3 A composite sample of carbon reinforced epoxy has dimensions of 12 in by 12 in by 0.25 in and mass of 1.8 lb. The carbon fibers have a modulus of elasticity of 50(106 ) lb/in2 and a density of 0.069 lb/in3 . The epoxy matrix has modulus of elasticity of 0.61(106 ) lb/in2 and a density of 0.042 lb/in3 . What is the volume fraction of (a) the carbon fibers and (b) the epoxy matrix in the sample? Assume there are no voids in the sample. Solution: Vc = 12(12)(0.25) = 36 in3 ρc = mc/Vc = 1.8/36 = 0.050 lb/in3 (a) fm = 1 – fr ρc = fmρm + frρr ρc = (1-fr)ρm + frρr ρc = ρm - frρm + frρr = ρm - fr(ρm - ρr) fr = (ρm - ρc)/(ρm - ρr) = (0.042 – 0.050)/(0.042 – 0.069) = 0.30 = 30% (b) fm = 1 – fr fm = 1- 0.30 = 0.70 = 70% 9.4 In problem 9.3, what is the predicted value for the modulus of elasticity (a) in the longitudinal direction and (b) the perpendicular to the carbon fibers? Solution: fm = 0.70, fr = 0.30, Em = 0.61x106 lb/in2 , and Er = 50.0x106 lb/in2 (a) Ec = fmEm + frEr Ec = 0.70(0.61x106 ) + 0.30(50.0x106 ) = 15 x 106 lb/in2 (b) Ec’ = EmEr/(fmEr + frEm) Ec’ = 0.61(106 )(50.0(106 )/(0.70(50.0x106 ) + 0.30(0.61x106 )) = 0.87 x 106 lb/in2 9.5 A composite has a matrix of polyester with Kevlar-29 fibers. The volume fractions of polyester and Kevlar are 60% and 40%, respectively. The Kevlar fibers have a modulus of elasticity of 60 GPa in the longitudinal direction and 3 GPa in the transverse direction. The polyester matrix has a modulus of elasticity of 5.6 GPa in both directions. (a) Determine the modulus of elasticity for the composite in the longitudinal direction. (b) Determine the modulus of elasticity in the transverse direction. Solution: fm = 0.60, fr = 0.40, Em = 5.6 GPa, and Er = 60 GPa (a) Ec = fmEm + frEr Ec = 0.60(5.6) + 0.40(60) = 27.4 GPa
• 44. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-12-09, 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 (b) Ec’ = EmEr/(fmEr + frEm) Ec’ = 5.6(60)/(0.60(60) + 0.40(5.6)) = 8.79 GPa
• 48. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 4 Heat required = 2.70(6597.3){0.88(660-25) + 389.3 + 0.88(800-660)} = 17,812.71{558.8 + 389.3 + 123.2} = 19,082,756 J 10.2 A sufficient amount of pure copper is to be heated for casting a large plate in an open mold. The plate has dimensions: length = 20 in, width = 10 in, and thickness = 3 in. Compute the amount of heat that must be added to the metal to heat it to a temperature of 2150°F for pouring. Assume that the amount of metal heated will be 10% more than what is needed to fill the mold cavity. Properties of the metal are: density = 0.324 lbm/in3 , melting point = 1981°F, specific heat of the metal = 0.093 Btu/lbm-F in the solid state and 0.090 Btu/lbm-F in the liquid state, and heat of fusion = 80 Btu/lbm. Solution: Volume V = (20 x 10 x 3)(1 + 10%) = 600(1.1) = 660.0 in3 Assuming To = 75 °F and using Eq. (10.1), H = 0.324 x 660{0.093(1981 - 75) + 80 + 0.090(2150 - 1981)} = 213.84{177.26 + 80 + 15.21} H = 58,265 Btu 10.3 The downsprue leading into the runner of a certain mold has a length = 175 mm. The cross-sectional area at the base of the sprue is 400 mm2 . The mold cavity has a volume = 0.001 m3 . Determine (a) the velocity of the molten metal flowing through the base of the downsprue, (b) the volume rate of flow, and (c) the time required to fill the mold cavity. Solution: (a) Velocity v = (2 x 9815 x 175)0.5 = (3,435,096)0.5 = 1853 mm/s (b) Volume flow rate Q = vA = 1853 x 400 = 741,200 mm3 /s (c) Time to fill cavity TMF = V/Q = 1,000,000/741,200 = 1.35 s 10.4 A mold has a downsprue of length = 6.0 in. The cross-sectional area at the bottom of the sprue is 0.5 in2 . The sprue leads into a horizontal runner which feeds the mold cavity, whose volume = 75 in3 . Determine (a) the velocity of the molten metal flowing through the base of the downsprue, (b) the volume rate of flow, and (c) the time required to fill the mold cavity. Solution: (a) Velocity v = (2 x 32.2 x 12 x 6.0)0.5 = (4636.8)0.5 = 68.1 in/sec (b) Volume flow rate Q = vA = 68.1 x 0.5 = 34.05 in3 /sec (c) Time to fill cavity TMF = V/Q = 75.0/34.05 = 2.2 sec. 10.5 The flow rate of liquid metal into the downsprue of a mold = 1 liter/sec. The cross-sectional area at the top of the sprue = 800 mm2 , and its length = 175 mm. What area should be used at the base of the sprue to avoid aspiration of the molten metal? Solution: Flow rate Q = 1.0 l/s = 1,000,000 mm3 /s Velocity v = (2 x 9815 x 175)0.5 = 1854 mm/s Area at base A = 1,000,000/1854 = 540 mm2 10.6 The volume rate of flow of molten metal into the downsprue from the pouring cup is 50 in3 /sec. At the top where the pouring cup leads into the downsprue, the cross-sectional area = 1.0 in2 . Determine what the area should be at the bottom of the sprue if its length = 8.0 in. It is desired to maintain a constant flow rate, top and bottom, in order to avoid aspiration of the liquid metal. Solution: Velocity at base v = (2gh)0.5 = (2 x 32.2 x 12 x 8)0.5 = 78.6 in/sec Assuming volumetric continuity, area at base A = (50 in/sec)/(78.6 in/sec) = 0.636 in2 10.7 Molten metal can be poured into the pouring cup of a sand mold at a steady rate of 1000 cm3 /s. The molten metal overflows the pouring cup and flows into the downsprue. The cross section of the sprue is round, with a diameter at the top = 3.4 cm. If the sprue is 25 cm long, determine the proper diameter at its base so as to maintain the same volume flow rate. Solution: Velocity at base v = (2gh)0.5 = (2 x 981 x 25)0.5 = 221.5 cm/s Assuming volumetric continuity, area at base A = (1000 cm/s)/(221.5 cm/s) = 4.51 cm2 Area of sprue A = πD2 /4; rearranging, D2 = 4A/π = 4(4.51)/π = 5.74 cm2
• 50. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 Solution: The initial volume of liquid metal = 1,000,000 mm3 . When poured into the mold it takes the shape of the open mold, which is 200 mm by 200 mm square, or 40,000 mm2 . The starting height of the molten metal is 1,000,000 / 40,000 = 25 mm. Volumetric solidification shrinkage is 6%, so when the aluminum has solidified its volume = 1,000,000(0.94) = 940,000 mm3 . Because its base still measures 200 mm by 200 mm due to the flow of liquid metal before solidification, its height has been reduced to 940,000 / 40,000 = 23.5 mm. Thermal contraction causes a further shrinkage of 1.6%. Thus the final dimensions of the plate are 200(0.984) by 200(0.984) by 23.5(0.984) = 196.8 mm by 196.8 mm by 23.124 mm. Solidification Time and Riser Design 10.12 In the casting of steel under certain mold conditions, the mold constant in Chvorinov's rule is known to be 4.0 min/cm2 , based on previous experience. The casting is a flat plate whose length = 30 cm, width = 10 cm, and thickness = 20 mm. Determine how long it will take for the casting to solidify. Solution: Volume V = 30 x 10 x 2 = 600 cm3 Area A = 2(30 x 10 + 30 x 2 + 10 x 2) = 760 cm2 Chvorinov’s rule: TTS = Cm (V/A)2 = 4(600/760)2 = 2.49 min 10.13 Solve for total solidification time in the previous problem only using an exponent value of 1.9 in Chvorinov's rule instead of 2.0. What adjustment must be made in the units of the mold constant? Solution: Chvorinov’s rule: TTS = Cm (V/A)1.9 = 4(600/760)1.9 = 2.55 min The units for Cm become min/in1.9 - strange units but consistent with Chvorinov’s empirical rule. 10.14 A disk-shaped part is to be cast out of aluminum. The diameter of the disk = 500 mm and its thickness = 20 mm. If the mold constant = 2.0 sec/mm2 in Chvorinov's rule, how long will it take the casting to solidify? Solution: Volume V = πD2 t/4 = π(500)2 (20)/4 = 3,926,991 mm3 Area A = 2πD2 /4 + πDt = π(500)2 /2 + π(500)(20) = 424,115 mm2 Chvorinov’s rule: TTS = Cm (V/A)2 = 2.0(3,926,991/424,115)2 = 171.5 s = 2.86 min 10.15 In casting experiments performed using a certain alloy and type of sand mold, it took 155 sec for a cube-shaped casting to solidify. The cube was 50 mm on a side. (a) Determine the value of the mold constant in Chvorinov's rule. (b) If the same alloy and mold type were used, find the total solidification time for a cylindrical casting in which the diameter = 30 mm and length = 50 mm. Solution: (a) Volume V = (50)3 = 125,000 mm3 Area A = 6 x (50)2 = 15,000 mm2 (V/A) = 125,000/15,000 = 8.333 mm Cm = TTS /(V/A)2 = 155/(8.333)2 = 2.232 s/mm2 (b) Cylindrical casting with D = 30 mm and L = 50 mm. Volume V = πD2 L/4 = π(30)2 (50)/4 = 35,343 mm3 Area A = 2πD2 /4 + πDL = π(30)2 /2 + π(30)(50) = 6126 mm2 V/A = 35,343/6126 = 5.77 TTS = 2.232 (5.77)2 = 74.3 s = 1.24 min. 10.16 A steel casting has a cylindrical geometry with 4.0 in diameter and weighs 20 lb. This casting takes 6.0 min to completely solidify. Another cylindrical-shaped casting with the same diameter-to-length ratio weighs 12 lb. This casting is made of the same steel, and the same conditions of mold and pouring were used. Determine: (a) the mold constant in Chvorinov's rule, (b) the dimensions, and (c) the total solidification time of the lighter casting. The density of steel = 490 lb/ft3 . Solution: (a) For steel, ρ = 490 lb/ft3 = 0.2836 lb/in3 Weight W = ρV, V = W/ρ = 20/0.2836 = 70.53 in3
• 51. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 Volume V = πD2 L/4 = π(4)2 L/4 = 4πL = 70.53 in3 Length L = 70.53/4π = 5.61 in Area A = 2πD2 /4 + πDL = 2π(4)2 /4 + π(4)(5.61) = 95.63 in2 (V/A) = 70.53/95.63 = 0.7375 Cm = 6.0/(0.7353)2 = 11.03 min/in2 (b) Find dimensions of smaller cylindrical casting with same D/L ratio and w = 12 lb. Weight is proportional to volume: V = (12/20)(70.53) = 42.32 in3 D/L ratio = 4.0/5.61 = 0.713; thus L = 1.4025D Volume V = πD2 L/4 = π(D)2 (1.4025D)/4 = 1.1015D3 D3 = (42.32 in3 )/1.1015 = 38.42 in3 D = (38.42)0.333 = 3.374 in L = 1.4025(3.374) = 4.732 in (c) V = πD2 L/4 = π(3.374)2 (4.732)/4 = 42.32 in3 A = 2πD2 /4 + πDL = 0.5π(3.374)2 + π(3.374)(4.732) = 68.04 in2 V/A = 42.32/68.04 = 0.622 in. TTS = 11.03(.622)2 = 4.27 min. 10.17 The total solidification times of three casting shapes are to be compared: (1) a sphere with diameter = 10 cm, (2) a cylinder with diameter and length both = 10 cm, and (3) a cube with each side = 10 cm. The same casting alloy is used in the three cases. (a) Determine the relative solidification times for each geometry. (b) Based on the results of part (a), which geometric element would make the best riser? (c) If the mold constant = 3.5 min/cm2 in Chvorinov's rule, compute the total solidification time for each casting. Solution: For ease of computation, make the substitution 10 cm = 1 decimeter (1 dm) (a) Chvorinov’s rule: TTS = Cm(V/A)2 (1) Sphere volume V = πD3 /6 = π(1)3 /6 = π/6 dm3 Sphere surface area A = πD2 = π(1)2 = π dm2 V/A = (π/6)/π = 1/6 = 0.1667 dm Chvorinov’s rule TTS = (0.1667)2 Cm = 0.02778Cm (2) Cylinder volume V = πD2 H/4 = π(1)2 (1)/4 = π/4 = 0.25π dm3 Cylinder area A = 2πD2 /4 + πDL = 2π(1)2 /4 + π(1)(1) = π/2 + π = 1.5π dm2 V/A = 0.25π/1.5π = 0.1667 dm Chvorinov’s rule TTS = (0.1667)2 Cm = 0.02778Cm (3) Cube: V = L3 = (1)3 = 1.0 dm3 Cube area = 6L2 = 6(1)2 = 6.0 dm2 V/A = 1.0/6.0 = 0.1667 dm Chvorinov’s rule TTS = (0.1667)2 Cm = 0.02778Cm (b) All three shapes are equivalent as risers. (c) If Cm = 3.5 min/cm2 = 350 min/dm2 , then TTS = 0.02778(350) = 9.723 min. Note, however, that the volumes of the three geometries are different: (1) sphere V = 0.524 dm3 = 524 cm3 , cylinder V = 0.25π = 0.7854 dm3 = 785.4 cm3 , and (3) cube V = 1.0 dm3 = 1000cm3 . Accordingly, we might revise our answer to part (b) and choose the sphere on the basis that it wastes less metal than the other shapes. 10.18 The total solidification times of three casting shapes are to be compared: (1) a sphere, (2) a cylinder, in which the length-to-diameter ratio = 1.0, and (3) a cube. For all three geometries, the volume = 1000 cm3 . The same casting alloy is used in the three cases. (a) Determine the relative solidification times for each geometry. (b) Based on the results of part (a), which geometric element would make
• 52. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 the best riser? (c) If the mold constant = 3.5 min/cm2 in Chvorinov's rule, compute the total solidification time for each casting. Solution: For ease of computation, make the substitution 10 cm = 1 decimeter (1 dm). Thus 1000 cm3 = 1.0 dm3 . (1) Sphere volume V = πD3 /6 = 1.0 dm3 . D3 = 6/π = 1.910 dm3 . D = (1.910)0.333 = 1.241 dm Sphere area A = πD2 = π(1.241)2 = 4.836 dm2 V/A = 1.0/4.836 = 0.2067 dm Chvorinov’s rule TTS = (0.2067)2 Cm = 0.0428Cm (2) Cylinder volume V = πD2 H/4 = πD3 /4 = 1.0 dm3 . D3 = 4/π = 1.273 dm3 Therefore, D = H = (1.273)0.333 = 1.084 dm Cylinder area A = 2πD2 /4 + πDL = 2π(1.084)2 /4 + π(1.084)(1.084) = 5.536 dm2 V/A = 1.0/5.536 = 0.1806 dm Chvorinov’s rule TTS = (0.1806)2 Cm = 0.0326Cm (3) Cube: V = L3 =1.0 dm3 . L = 1.0 dm Cube area = 6L2 = 6(1)2 = 6.0 dm2 V/A = 1.0/6.0 = 0.1667 dm Chvorinov’s rule TTS = (0.1667)2 Cm = 0.02778Cm (b) Sphere would be the best riser, since V/A ratio is greatest. (c) Given that Cm = 3.5 min/cm2 = 350 min/dm3 Sphere: TTS = 0.0428(350) = 14.98 min Cylinder: TTS = 0.0326(350) = 11.41 min Cube: TTS = 0.02778(350) = 9.72 min 10.19 A cylindrical riser is to be used for a sand-casting mold. For a given cylinder volume, determine the diameter-to-length ratio that will maximize the time to solidify. Solution: To maximize TTS, the V/A ratio must be maximized. Cylinder volume V = πD2 L/4. L = 4V/πD2 Cylinder area A = 2πD2 /4 + πDL Substitute the expression for L from the volume equation in the area equation: A = πD2 /2 + πDL = πD2 /2 + πD(4V/πD2 ) = πD2 /2 + 4 V/D Differentiate the area equation with respect to D: dA/dD = πD – 4 V/D2 = 0 Rearranging, πD = 4V/D2 D3 = 4 V/π D = (4 V/π)0.333 From the previous expression for L, substituting in the equation for D that we have developed, L = 4V/πD2 = 4V/π(4V/π)0.667 = (4V/π)0.333 Thus, optimal values are D = L = (4V/π)0.333 , and therefore the optimal D/L ratio = 1.0 10.20 A riser in the shape of a sphere is to be designed for a sand casting mold. The casting is a rectangular plate, with length = 200 mm, width = 100 mm, and thickness = 18 mm. If the total solidification time of the casting itself is known to be 3.5 min, determine the diameter of the riser so that it will take 25% longer for the riser to solidify. Solution: Casting volume V = LWt = 200(100)(18) = 360,000 mm3 Casting area A = 2(200 x 100 + 200 x 18 + 100 x 18) = 50,800 mm2 V/A = 360,000/50,800 = 7.0866 Casting TTS = Cm(7.0866)2 = 3.50 min Cm = 3.5/(7.0866)2 = 0.0697 min/mm2 Riser volume V = πD3 /6 = 0.5236D3
• 53. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 9 Riser area A = πD2 = 3.1416D2 V/A = 0.5236D3 /3.1416D2 = 0.1667D TTS = 1.25(3.5) = 4.375 min = 0.0697(0.1667D)2 = 0.001936D2 D2 = 4.375/0.001936 = 2259.7 mm2 D = 47.5 mm 10.21 A cylindrical riser is to be designed for a sand casting mold. The length of the cylinder is to be 1.25 times its diameter. The casting is a square plate, each side = 10 in and thickness = 0.75 in. If the metal is cast iron, and the mold constant = 16.0 min/in2 in Chvorinov's rule, determine the dimensions of the riser so that it will take 30% longer for the riser to solidify. Solution: Casting volume V = tL2 = 0.75(10.0)2 = 75 in3 Casting area A = 2L2 + 4Lt = 2(10.0)2 + 4(10.0)(0.75) = 230.0 in2 V/A = 75/230 = 0.3261 Casting TTS = 16(0.3261)2 = 1.70 min Riser TTS = 1.30(1.70) = 2.21 min Riser volume V = πD2 H/4 = 0.25πD2 (1.25D) = 0.3125πD3 Riser area A = 2πD2 /4 + πDH = 0.5πD2 + 1.25πD2 = 1.75πD2 V/A = 0.3125πD3 /1.75πD2 = 0.1786D Riser TTS = 16.0(0.1786D)2 = 16.0(0.03189)D2 = 0.5102D2 = 2.21 min D2 = 2.21/0.5102 = 4.3316 D = (4.3316)0.5 = 2.081 in H = 1.25(2.081) = 2.602 in. 10.22 A cylindrical riser with diameter-to-length ratio = 1.0 is to be designed for a sand casting mold. The casting geometry is illustrated in Figure P10.25, in which the units are inches. If the mold constant in Chvorinov's rule = 19.5 min/in2 , determine the dimensions of the riser so that the riser will take 0.5 min longer to freeze than the casting itself. Solution: Casting volume V = V(5 in x 10 in rectangular plate) + V(5 in. half disk) + V(upright tube) - V(3 in x 6 in rectangular cutout). V(5 in x 10 in rectangular plate) = 5 x 12.5 x 1.0 = 62.5 in3 V(5 in. half disk) = 0.5π(5)2 (1)/4 = 9.817 in3 V(upright tube) = 3.0π(2.5)2 /4 - 4π(1.5)2 /4) = 7.657 in3 V(3 in x 6 in rectangular cutout) = 3 x 6 x 1 = 18.0 in3 Total V = 62.5 + 9.817 + 7.657 - 18.0 = 61.974 in3 Total A = 1 x 5 + 1(12.5 + 2.5π + 12.5) + 2(6+3) + 2(5 x 12.5 - 3 x 6) + 2(.5π(5)2 /4) - 2(1.5)2 π/4 + 2.5π(3) + 1.5π(3+1) = 203.36 in2 V/A = 61.974/203.36 = 0.305 in Casting TTS = 19.5(0.305)2 = 1.81 min Riser design: specified TTS = 1.81 + 0.5 = 2.31 min Riser volume V = πD2 L/4 = πD3 /4 = 0.25πD3 Riser area A = πDL + 2πD2 /4 = πD2 + 0.5πD2 = 1.5πD2 V/A = 0.25πD3 /1.5πD2 = D/6 TTS = Cm(V/A)2 2.31 = 19.5(D/6)2 = 0.5417D2 D2 = 2.31/0.5417 = 4.266 in2 D = 2.065 in and L = 2.065 in
• 58. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-19-09, 03-22-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 (a) Wc = 325(0.058) = 18.85 lb At least 2 caplets are required beneath to support the weight of the core. Probably 3 or 4 caplets would be better to achieve stability. (b) Wm = 325(.313) = 101.73 lb Fb = 101.73 - 18.85 = 82.88 lb A total of 9 caplets are required above the core to resist the buoyancy force. 11.4 A sand core used to form the internal surfaces of a steel casting experiences a buoyancy force of 23 kg. The volume of the mold cavity forming the outside surface of the casting = 5000 cm3 . What is the weight of the final casting? Ignore considerations of shrinkage. Solution: Sand density = 1.6 g/cm3 , steel casting density ρ = 7.82 g/cm3 Fb = Wm - Wc = 7.82V - 1.6V = 6.22V = 23 kg = 23,000 g V = 3698 cm3 . Cavity volume V = 5000 cm3 Volume of casting V = 5000 - 3698 = 1302 cm3 . Weight of the final casting W = 1302(7.82) = 10,184 g = 10.184 kg Centrifugal Casting 11.5 A horizontal true centrifugal casting operation will be used to make copper tubing. The lengths will be 1.5 m with outside diameter = 15.0 cm, and inside diameter = 12.5 cm. If the rotational speed of the pipe = 1000 rev/min, determine the G-factor. Solution: From Eq. (11.4), GF = R(πN/30)2 /g = 7.5(π(1000)/30)2 /981 = 83.8 11.6 A true centrifugal casting operation is to be performed in a horizontal configuration to make cast iron pipe sections. The sections will have a length = 42.0 in, outside diameter = 8.0 in, and wall thickness = 0.50 in. If the rotational speed of the pipe = 500 rev/min, determine the G-factor. Is the operation likely to be successful? Solution: Using outside wall of casting, R = 0.5(8)/12 = 0.333 ft. v = πRN/30 = π(0.333)(500)/30 = 17.45 ft/sec. GF = v2 /Rg = (17.45)2 /(0.333 x 32.2) = 28.38 Since the G-factor is less than 60, the rotational speed is not sufficient, and the operation is likely to be unsuccessful. 11.7 A horizontal true centrifugal casting process is used to make brass bushings with the following dimensions: length = 10 cm, outside diameter = 15 cm, and inside diameter = 12 cm. (a) Determine the required rotational speed in order to obtain a G-factor of 70. (b) When operating at this speed, what is the centrifugal force per square meter (Pa) imposed by the molten metal on the inside wall of the mold? Solution: (a) Using the outside wall diameter of the casting, which is equal to the inside wall diameter of the mold, D = 15 cm N = (30/π)(2g x 70/15).5 = 913.7 rev/min. (b) Use 1.0 cm of mold wall length as basis of area calculations. Area of this length of mold wall A = πDoL = π(15 cm)(1 cm) = 15π cm2 = 15π(10-4 ) m2 Volume of cast metal V = π(Ro 2 - Ri 2 )(1.0) = π((7.5)2 - (6)2 )(1.0) = 63.62 cm3 Mass m = (8.62g/cm3 )(63.62 cm3 ) = 548.4 g = 0.5484 kg v = πRN/30 Use mean radius R = (7.5 + 6.0)/2 = 6.75 cm v = π(6.75)(913.7)/30 = 645.86 cm/s = 6.4585 m/s Centrifugal force per square meter on mold wall = Fc/A where Fc = mv2 /R Fc = (0.5484 kg)(6.4586 m/s)2 /(6.75 x 10-2 m) = 338.9 kg-m/s2 Given that 1 N = 9.81 kg-m/s2 , Fc = 338.9/9.81 = 34.55 N
• 59. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-19-09, 03-22-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 Fc/A = (34.55 N)/(15π x 10-4 m2 ) = 0.7331(104 ) N/m2 = 7331 Pa 11.8 True centrifugal casting is performed horizontally to make large diameter copper tube sections. The tubes have a length = 1.0 m, diameter = 0.25 m, and wall thickness = 15 mm. (a) If the rotational speed of the pipe = 700 rev/min, determine the G-factor on the molten metal. (b) Is the rotational speed sufficient to avoid "rain?" (c) What volume of molten metal must be poured into the mold to make the casting if solidification shrinkage and contraction after solidification are considered? Solidification shrinkage for copper = 4.5%, and solid thermal contraction = 7.5%. Solution: (a) GF = v2 /Rg g = 9.8 m/s2 v = πRN/30 = π(.125)(700)/30 = 9.163 m/s GF = (9.163)2 /(0.125 x 9.8) = 68.54 (b) G-factor is sufficient for a successful casting operation. (c) Volume of final product after solidification and cooling is V = (0.252 - (0.25-.03)2 )π x 1.0/4 = 0.25π(0.252 - 0.222 ) = 0.011074 m3 Given: solidification shrinkage = 4.5% and solid thermal contraction = 7.5% for copper. Taking these factors into account, Volume of molten metal V = 0.011074/(1 - 0.045)(1 - 0.075) = 0.01254 m3 11.9 If a true centrifugal casting operation were to be performed in a space station circling the Earth, how would weightlessness affect the process? Solution: The mass of molten metal would be unaffected by the absence of gravity, but its weight would be zero. Thus, in the G-factor equation (GF = v2 /Rg), GF would theoretically go to infinity if g = 0. Thus, it should be possible to force the metal against the walls of the mold in centrifugal casting without the nuisance of “raining” inside the cavity. However, this all assumes that the metal is inside the mold and rotating with it. In the absence of gravity, there would be a problem in pouring the molten metal into the mold cavity and getting it to adhere to the mold wall as the mold begins to rotate. With no gravity the liquid metal would not be forced against the lower surface of the mold to initiate the centrifugal action. 11.10 A horizontal true centrifugal casting process is used to make aluminum rings with the following dimensions: length = 5 cm, outside diameter = 65 cm, and inside diameter = 60 cm. (a) Determine the rotational speed that will provide a G-factor = 60. (b) Suppose that the ring were made out of steel instead of aluminum. If the rotational speed computed in part (a) were used in the steel casting operation, determine the G-factor and (c) centrifugal force per square meter (Pa) on the mold wall. (d) Would this rotational speed result in a successful operation? Solution: (a) Use inside diameter of mold in Eq. (11.5), D = Do = 65 cm. Use g = 981 cm/s2 , N = 30(2g x GF/D).5 /π = 30(2 x 981 x 60/65).5 /π = 406.4 rev/min. (b) Rotational speed would be the same as in part (a) because mass does not enter the computation of rotational speed. N = 406.4 rev/min (c) Use 5 cm ring length as basis of area calculations. Area of this length of mold wall A = πDoL = π(65 cm)(5 cm) = 1021 cm2 = 0.1021 m2 Volume of cast metal V = π(Ro 2 - Ri 2 )(L) = π((65/2)2 - (60/2)2 )(5.0) = 2454.4 cm3 Density of steel ρ = 7.87 g/cm3 Mass m = (7.87g/cm3 )(2454.4 cm3 ) = 19,315.9 g = 19.316 kg v = πRN/30 Use mean radius R = (65 + 60)/4 = 31.25 cm = 0.3125 m v = π(31.25)(406.4)/30 = 1329.9 cm/s = 13.299 m/s Centrifugal force per square meter on mold wall = Fc/A where Fc = mv2 /R Fc = (19.316 kg)(13.299 m/s)2 /(0.3125 m) = 10,932.1 kg-m/s2 Given that 1 N = 9.81 kg-m/s2 , Fc = 10,932.1/9.81 = 1114.4 N
• 60. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-19-09, 03-22-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 Fc/A = (1114.4 N)/(0.1021 m2 ) = 10,914.7 N/m2 = 10,914.7 Pa (d) The G-factor of 60 would probably result in a successful casting operation. 11.11 For the steel ring of preceding Problem 11.10(b), determine the volume of molten metal that must be poured into the mold, given that the liquid shrinkage is 0.5%, solidification shrinkage = 3%, and solid contraction after freezing = 7.2%. Solution: Volume of final casting V = π(Ro 2 - Ri 2 )L = π(32.52 - 302 )(5) = 2454.4 cm3 Given that the molten metal shrinkage = 0.5%, and from Table 10.1, the solidification shrinkage for steel = 3% and the solid contraction during cooling = 7.2%, the total volumetric contraction is (1-0.005)(1-0.03)(1-0.072) = 0.8957 The required starting volume of molten metal V = 2454.4/(0.8957) = 2740.2 cm3 11.12 A horizontal true centrifugal casting process is used to make lead pipe for chemical plants. The pipe has length = 0.5 m, outside diameter = 70 mm, and wall thickness = 6.0 mm. Determine the rotational speed that will provide a G-factor = 60. Solution: D = 70 mm = 0.07 m. g = 9.8 m/s2 N = 30(2g x GF/D).5 /π = 30(2 x 9.8 x 60/.07).5 /π = 1237.7 rev/min. 11.13 A vertical true centrifugal casting process is used to make tube sections with length = 10.0 in and outside diameter = 6.0 in. The inside diameter of the tube = 5.5 in at the top and 5.0 in at the bottom. At what speed must the tube be rotated during the operation in order to achieve these specifications? Solution: Use Eq. (11.6) to make the computation of N: N = (30/π)(2gL/(Rt 2 -Rb 2 ).5 L = 10 in = 0.8333 ft Rt = 5.5/2 = 2.75 in = 0.22917 ft Rb = 5.0/2 = 2.50 in = 0.20833 ft N = (30/π)(2 x 32.2 x .8333/(0.229172 - 0.208332 ).5 = 9.5493(5888).5 = 732.7 rev/min 11.14 A vertical true centrifugal casting process is used to produce bushings that are 200 mm long and 200 mm in outside diameter. If the rotational speed during solidification is 500 rev/min, determine the inside diameter at the top of the bushing if the inside diameter at the bottom is 150 mm. Solution: L = 200 mm = 0.2 m. Rb = 150/2 = 75 mm = 0.075 m. N = (30/π)(2gL/(Rt 2 -Rb 2 ).5 = (30/π)(2 x 9.8 x 0.2/(Rt 2 - 0.0752 )).5 N = (30/π)(3.92/(Rt 2 - 0.005625)).5 = 500 rev/min (3.92/(Rt 2 - 0.005625)).5 = 500π/30 = 52.36 3.92/(Rt 2 -.005625) = (52.36)2 = 2741.56 Rt 2 -.005625 = 3.92/2741.56 = 0.00143 Rt 2 = .005625 + 0.001430 = 0.007055 Rt = (0.007055).5 = .08399 m = 83.99 mm. Dt = 2(83.99) = 167.98 mm. 11.15 A vertical true centrifugal casting process is used to cast brass tubing that is 15.0 in long and whose outside diameter = 8.0 in. If the speed of rotation during solidification is 1000 rev/min, determine the inside diameters at the top and bottom of the tubing if the total weight of the final casting = 75.0 lbs. Solution: For brass, density ρ = 0.313 lb/in3 (Table 11.1). Volume of casting V = 75.0/.313 = 239.6 in3 Assume the inside wall of the casting is straight from top to bottom (an approximation of the parabolic shape). The average inside radius Ri = (Rt + Rb)/2 Volume V = π(Ro 2 - Ri 2 )L = π(4.02 - Ri 2 )(15.0) = 239.6 in3 (4.02 - Ri 2 ) = 239.6/15π = 5.085 Ri 2 = 16.0 - 5.085 = 10.915 in2 Ri = 3.304 in
• 61. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-19-09, 03-22-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 Let Rt = Ri + y = 3.304 + y and Rb = Ri - y = 3.304 - y, where y = one-half the difference between Rt and Rb. N = (30/π)(2gL/(Rt 2 -Rb 2 ).5 = (30/π)(2 x 32.2 x 12 x 15/((3.304+y)2 -(3.304-y)2 )).5 Given N = 1000 rev/min, thus 1000π/30 = (11592/((3.304+y)2 -(3.304-y)2 )).5 ((3.304+y)2 -(3.304-y)2 ).5 = 30(11592).5 /1000π = 1.02814 (3.3042 + 6.608y + y2 - (3.3042 - 6.608y + y2 )).5 = 1.02814 (3.3042 + 6.608y + y2 - 3.3042 + 6.608y - y2 ).5 = 1.02814 (2 x 6.608y).5 = (13.216y).5 = 1.02814 3.635 (y).5 = 1.02814 y = .080 in. Rt = 3.304 + 0.080 = 3.384 in. Dt = 6.768 in. Rb = 3.304 - 0.080 = 3.224 in. Db = 6.448 in. Defects and Design Considerations 11.16 The housing for a certain machinery product is made of two components, both aluminum castings. The larger component has the shape of a dish sink, and the second component is a flat cover that is attached to the first component to create an enclosed space for the machinery parts. Sand casting is used to produce the two castings, both of which are plagued by defects in the form of misruns and cold shuts. The foreman complains that the parts are too thin, and that is the reason for the defects. However, it is known that the same components are cast successfully in other foundries. What other explanation can be given for the defects? Solution: Misruns and cold shuts result from low fluidity. One possible reason for the defects in this case is that the thickness of the casting cross sections is too small. However, given that the casting of these parts is successfully accomplished at other foundries, two other possible explanations are (1) the pouring temperature is too low, and (2) the pouring operation is performed too slowly. 11.17 A large steel sand casting shows the characteristic signs of penetration defect: a surface consisting of a mixture of sand and metal. (a) What steps can be taken to correct the defect? (b) What other possible defects might result from taking each of these steps? Solution: (a) What are the possible corrective steps? (1) Reduce pouring temperature. (2) Increase the packing of the mold sand to resist penetration. (3) Treat the mold cavity surface to make it harder. (b) What possible defects might result from each of these steps? In the case of step (1), the risk is for cold shuts and misruns. Steps (2) and (3) would reduce permeability of the sand, thus increasing the risk of sand blows and pin holes.
• 64. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-20-09, 03-27-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 61 12.7 The press-and-blow process is best suited to the production of (narrow-necked) beverage bottles, while the blow-and-blow process is more appropriate for producing (wide-mouthed) jars: (a) true, or (b) false? Answer. (b). It's the reverse. 12.8 Which one of the following processes is used to produce glass tubing: (a) Danner process, (b) pressing, (c) rolling, or (d) spinning? Answer. (a). 12.9 If a glass part with a wall thickness of 5 mm (0.20 in) takes 10 minutes to anneal, how much time would a glass part of similar geometry but with a wall thickness of 7.5 mm (0.30 in) take to anneal (choose the one closest answer): (a) 10 minutes, (b) 15 minutes, (c) 20 minutes, or (c) 30 minutes? Answer. (c). The rule is that annealing time varies as the square of the wall thickness. That would indicate an annealing time of (0.30/0.20)2 = 2.25 times 10 minutes or 22.5 minutes. 20 minutes is closest. 12.10 A lehr is which of the following: (a) a lion's den, (b) a melting furnace, (c) a sintering furnace, (d) an annealing furnace, or (e) none of the above? Answer. (d).
• 71. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-27-09, 04-28-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 13.3 An extruder barrel has a diameter of 110 mm and a length of 3.0 m. The screw channel depth = 7.0 mm, and its pitch = 95 mm. The viscosity of the polymer melt is 105 Pa-s, and the head pressure in the barrel is 4.0 MPa. What rotational speed of the screw is required to achieve a volumetric flow rate of 90 cm3 /s? Solution: A = tan-1 (p/(πD)) = tan-1 (95/110π) = 15.37° Qd = 0.5π2 D2 N dc sinAcosA = 0.5π2 (0.110)2 (N)(7.0x10-3 )sin 15.37 cos 15.37 = 106.8 N x 10-6 m3 /s Qb = π(4x106 )(0.110)(7x10-3 )3 (sin 15.37)2 /12(105)(3.0) = 8.81 x 10-6 m3 /s Qx = Qd - Qb = 106.8 N x 10-6 – 8.81 x 10-6 = 90 x 10-6 m3 /s 106.8 N = 90.0 + 8.81 = 98.81 N = 98.81/106.8 = 0.9252 rev/s = 55.51 rev/min. 13.4 An extruder has a barrel diameter of 2.5 in and a length of 6.0 ft. The screw has a channel depth of 0.25 in, a flight angle of 20°, and rotates at 55 rev/min. The material being extruded is polypropylene. At the present settings, the volumetric flow rate of the polymer melt is 1.50 in3 /sec and the head pressure is 500 lb/in2 . (a) Under these operating characteristics, what is the viscosity of the polypropylene? (b) Using Figure 13.2, approximate the temperature in °F of the polypropylene. Solution: (a) Qd = 0.5π2 D2 Ndc sinA cosA = 0.5π2 (2.52 )(55/60)(0.25)sin 20 cos 20 Qd = 2.27 in3 /sec Qb = Qd – Qx = 2.27 – 1.50 = 0.78 in3 /sec η = pπDdc 3 in2 A/(12 QbL) = 500π(2.5)(0.253 )sin2 (20)/(12(0.78)(6)(12)) = 0.011 lb-s/in2 (b) X-axis is Log scale. Therefore LOG(0.011) = -1.96 This is very close to –2, which is at the 10-2 hash mark on the y-axis. This yields about 410°F. 13.5 An extruder has diameter = 80 mm and length = 2.0 m. Its screw has a channel depth = 5 mm, flight angle = 18 degrees, and it rotates at 1 rev/sec. The plastic melt has a shear viscosity = 150 Pa-s. Determine the extruder characteristic by computing Qmax and pmax and then finding the equation of the straight line between them. Solution: Qmax = Qd = 0.5π2 (0.08)2 (1)(5x10-3 )sin 18 cos 18 = 0.158 x 10-3 (0.3090)(0.9510) = 46.4 x 10-6 m3 /s pmax = 6π(0.08)(1)(2)(150)(cot 18)/(5x10-3 )2 = 452.4(3.077)/25x10-6 = 55 x 106 Pa = 55 MPa Qx = 46.4 x 10-6 - (46.4x10-6 /55)p Qx = 46.4 x 10-6 - 0.8436 x 10-6 p, where p has units of MPa 13.6 Determine the helix angle A such that the screw pitch p is equal to the screw diameter D. This is called the "square" angle in plastics extrusion - the angle that provides a flight advance equal to one diameter for each rotation of the screw. Solution: Assume flight land = zero. From Eq. (15.4), tan A = pitch/πD If pitch = D, then A = tan-1 (1/π) = 17.66° 13.7 An extruder barrel has a diameter of 2.5 in. The screw rotates at 60 rev/min; its channel depth = 0.20 in, and its flight angle = 17.5°. The head pressure at the die end of the barrel is 800 lb/in2 and the length of the barrel is 50 in. The viscosity of the polymer melt is 122 x 10-4 lb-sec/in2 . Determine the volume flow rate of the plastic in the barrel. Solution: Qd = 0.5π2 (2.5)2 (1)(.2)sin 17.5 cos 17.5 = 0.5(12.337)(0.3007)(0.9537) = 1.769 in3 /sec Qb = π(800)(2.5)(.2)3 (sin 17.5)2 /12(122x10-4 )(50) = 0.621 in3 /sec Qx = 1.769 - 0.621 = 1.148 in3 /sec.
• 72. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-27-09, 04-28-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 13.8 An extruder barrel has a diameter of 4.0 in and an L/D ratio of 28. The screw channel depth = 0.25 in, and its pitch = 4.8 in. It rotates at 60 rev/min. The viscosity of the polymer melt is 100 x 10-4 lb-sec/in2 . What head pressure is required to obtain a volume flow rate = 150 in3 /min? Solution: A = tan-1 (pitch/πD) = tan-1 (4.8/4π) = 20.9° Qd = 0.5π2 (4)2 (1)(0.25)sin 20.9 cos 20.9 = 19.74(0.3567)(0.9342) = 6.578 in3 /sec = 394.66 in3 /min Qx = Qd - Qb = 394.66 - Qd = 150 Qb = 394.66 - 150 = 244.66 in3 /min = 4.078 in3 /sec L = 4(28) = 112 in. Qb = πp(4)(0.25)3 (sin 20.9)2 /(12(100x10-4 )(112)) = 4.078 0.0018592 p = 4.078 p = 2193.4 lb/in2 13.9 An extrusion operation produces continuous tubing with outside diameter = 2.0 in and inside diameter = 1.7 in. The extruder barrel has a diameter = 4.0 in and length = 10 ft. The screw rotates at 50 rev/min; it has a channel depth = 0.25 in and flight angle = 16°. The head pressure has a value of 350 lb/in2 and the viscosity of the polymer melt is 80 x 10-4 lb-sec/in2 . Under these conditions, what is the production rate in length of tube/min, assuming the extrudate is pulled at a rate that eliminates the effect of die swell (i.e., the tubing has the same OD and ID as the die profile)? Solution: Qd = 0.5π2 (4)2 (50/60)(.25)sin 16 cos 16 = 16.45(0.2756)(0.9613) = 4.358 in3 /sec Qb = π(350)(4)(.25)3 (sin 16)2 /(12(80x10-4 )(120)) = 0.453 in3 /sec Qx = 4.358 - 0.453 = 3.905 in3 /sec. Ax = 0.25π(22 - 1.72 ) = 0.872 in2 vx = 3.905/0.872 = 4.478 in/sec = 22.39 ft/min. 13.10 Continuous tubing is produced in a plastic extrusion operation through a die orifice whose outside diameter = 2.0 in and inside diameter = 1.5 in. The extruder barrel diameter = 5.0 in and length = 12 ft. The screw rotates at 50 rev/min; it has a channel depth = 0.30 in and flight angle = 16°. The head pressure has a value of 350 lb/in2 and the viscosity of the polymer melt is 90 x 10-4 lb-sec/in2 . Under these conditions, what is the production rate in length of tube/min, given that the die swell ratio is 1.25. Solution: Qd = 0.5π2 (5)2 (50/60)(.3)sin 16 cos 16 = 30.84(0.2756)(0.9613) = 8.171 in3 /sec Qb = π(350)(5)(.3)3 (sin 16)2 /(12(90x10-4 )(144)) = 0.725 in3 /sec Qx = 8.171 - 0.725 = 7.446 in3 /sec Die swell ratio applied to OD and ID: OD = 2(1.25) = 2.5, ID = 1.5(1.25) = 1.875 Ax = 0.25π(2.52 - 1.8752 ) = 2.1476 in2 vx = 7.446/2.1476 = 3.467 in/sec = 17.34 ft/min 13.11 An extruder has barrel diameter and length of 100 mm and 2.8 m, respectively. The screw rotational speed = 50 rev/min, channel depth = 7.5 mm, and flight angle = 17°. The plastic melt has a shear viscosity = 175 Pa-s. Determine: (a) the extruder characteristic, (b) the shape factor Ks for a circular die opening with diameter = 3.0 mm and length = 12.0 mm, and (c) the operating point (Q and p). Solution: Qmax = Qd = 0.5π2 (.1)2 (50/60)(7.5x10-3 ) sin 17 cos 17 = 308.4 x 10-6 (0.2924)(0.9563) = 86.2 x 10-6 m3 /s pmax = 6π(.1)(50/60)(2.8)(175)(cot 17)/(7.5x10-3 )2 = 44.75 x 106 Pa =44.75 MPa Qx = 86.2 x 10-6 - 1.926 x 10-12 p, where p has units of Pa (b) Given: Dd = 3 mm, Ld = 12 mm. Ks = π(3 x 10-3 )4 /(128(175)(12 x 10-3 )) = 0.9467 x 10-12 (c) 0.9467 x 10-12 p = 86.2 x 10-6 - 1.926 x 10-12 p 2.8727 x 10-12 p = 86.2 x 10-6
• 73. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-27-09, 04-28-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 9 p = 30.0 x 106 Pa = 30 MPa Qx = 0.9467 x 10-12 (30 x 106 ) = 28.4 x 10-6 m3 /s Check with extruder characteristic: Qx = 86.2 x 10-6 - 1.926 x 10-12 (30 x 106 ) = 28.4 x 10-6 m3 /s. 13.12 For Problem 13.11, assume the material is acrylic. (a) Using Figure 13.2, determine the temperature of the polymer melt. (b) If the temperature is lowered 20°C, estimate the resulting viscosity of the polymer melt. (Hint: the y-axis of Figure 13.2 is a log scale, not linear). Solution: (a) When viscosity = 175 Pa-s, Log(175) = 2.243, and temperature is approximately 260°C. (b) At 240°C, Log(viscosity) is approximately 2.7 and viscosity = 102.7 = 500 Pa-s. (Note: due to the log scale, small changes in the estimate will result in large changes in viscosity. 13.13 Consider an extruder in which the barrel diameter = 4.5 in and length = 11 ft. The extruder screw rotates at 60 rev/min; it has channel depth = 0.35 in and flight angle = 20°. The plastic melt has a shear viscosity = 125 x 10-4 lb-sec/in2 . Determine: (a) Qmax and pmax; (b) the shape factor Ks for a circular die opening in which Dd = 0.312 in and Ld = 0.75 in; and (c) the values of Q and p at the operating point. Solution: (a) Qmax = 0.5π2 (4.5)2 (1)(0.35)sin 20 cos 20 = 34.975(0.342)(0.9397) = 11.24 in3 /sec pmax = 6π(4.5)(1)(132)(0.0125)(cot 20)/(0.35)2 = 3139 lb/in2 (b) Given: Dd = 0.312 in., Ld = 0.75 in. Ks = π(0.312)4 /128(0.0125)(0.75) = 0.024808 (c) From (a), Qx = Qmax - (Qmax/pmax)p = 11.24 - 0.003581p From (b), Qx = 0.024808p Combining, .024808p = 11.24 - .003581p 0.02839p = 11.24 p = 395.9 lb/in2 Qx = 11.24 - 0.003581(395.9) = 9.82 in3 /sec 13.14 An extruder has a barrel diameter = 5.0 in and length = 12 ft. The extruder screw rotates at 50 rev/min; it has channel depth = 0.30 in and flight angle = 17.7°. The plastic melt has a shear viscosity = 100 x 10-4 lb-sec/in2 . Find: (a) the extruder characteristic, (b) the values of Q and p at the operating point, given that the die characteristic is Qx = 0.00150 p. Solution: (a) Qmax = 0.5π2 (5)2 (50/60)(0.3)sin 17.7 cos 17.7 = 30.84(0.3040)(0.9527) = 8.93 in3 /sec pmax = 6π(5)(50/60)(144)(0.01)(cot 17.7)/(0.3)2 = 3937.6 lb/in2 Qx = Qmax - (Qmax/pmax)p = 8.93 - 0.002268p (b) Given: die characteristic Qx = 0.0015p Qx = 8.93 - 0.002268p = 0.0015p 0.00377p = 8.93 p = 2370 lb/in2 Qx = 8.93 - 0.002268(2370) = 3.55 in3 /sec 13.15 Given the data in Problem 13.14, except that the flight angle of the extruder screw is a variable instead of a constant 17.7°. Use a spreadsheet calculator to determine the value of the flight angle that maximizes the volumetric flow rate Qx. Explore values of flight angle between 10° and 20°. Determine the optimum value to the nearest tenth of a degree. Solution: The author’s spreadsheet computations returned an optimum value of 13.5°. 13.16 An extruder has a barrel diameter of 3.5 in and a length of 5.0 ft. It has a screw channel depth of 0.16 in and a flight angle of 22°. The extruder screw rotates at 75 rev/min. The polymer melt has a shear viscosity = 65 x 10-4 lb-sec/in2 at the operating temperature of 525°F. The specific gravity of the polymer is 1.2 and its tensile strength is 8000 lb/in2 . A T-shaped cross section is extruded at a rate of
• 74. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-27-09, 04-28-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 10 0.11 lb/sec. The density of water is 62.5 lb/ft3 . (a) Find the equation for the extruder characteristic. (b) Find the operating point (Q and p), and (c) the die characteristic that is indicated by the operating point. Solution: (a) Qmax = 0.5π2 D2 Ndc sinA cosA = 0.5π2 (3.5)2 (75/60)(0.16)sin 22 cos 22 = 4.199 in3 /sec pmax = 6πDNLη cot A/dc 2 =6π(3.5)(75/60)(60)(0.0065)(cot 22)/(0.16)2 = 989.8 lb/in2 Qx = Qmax - (Qmax/pmax)p = 4.199 - 0.004242p (b) Given: T-shaped cross section extruded at 0.14 lb/sec. Density of polymer ρ = specific gravity of polymer x ρwater =1.2(62.4 lb/ft3 ) = 75 lb/ft3 Convert to lb/in3 : ρ= 75 lb/ft3 /(123 in3 /ft3 ) = 0.0433 lb/in3 Qx = 0.11/0.0433 = 2.540 in3 /sec. 2.540 = 4.199 - 0.004242p 0.004242p = 4.199 – 2.540 = 1.659 p = 391.1 lb/in2 (c) Qx = Ks p Ks = Qx/p = 2.540/391.1 = 0.00649 Qx = 0.00649 p Injection Molding 13.17 Compute the percentage volumetric contraction of a polyethylene molded part, based on the value of shrinkage given in Table 13.1. Solution: S = 0.025 for polyethylene from Table 13.1. Volumetric contraction = 1.0 - (1 - .025)3 = 1.0 - 0.92686 = 0.07314 = 7.314% Note that we are not using the parameter S from Table 13.1 in the way it was intended to be used. Its intended use is to compute the oversized dimension of a mold cavity in injection molding. Instead, we are using the shrinkage term to calculate the amount of (volumetric) reduction in size of the part after the polymer is injected into the cavity. In fact, a slightly different shrinkage parameter value may apply in this case. 13.18 The specified dimension = 225.00 mm for a certain injection molded part made of ABS. Compute the corresponding dimension to which the mold cavity should be machined, using the value of shrinkage given in Table 13.1. Solution: S = 0.006 for ABS from Table 13.1. Dc = 225.00 + 225.00(0.006) + 225.00(0.006)2 = 225.00 + 1.35 + 0.0081 = 226.36 mm. 13.19 The part dimension for a certain injection molded part made of polycarbonate is specified as 3.75 in. Compute the corresponding dimension to which the mold cavity should be machined, using the value of shrinkage given in Table 13.1. Solution: S = 0.007 for polycarbonate from Table 13.1. Dc = 3.75 + 3.75(0.007) + 3.75 (0.007)2 = 3.75 + 0.0263 + 0.0002 = 3.7765 in. 13.20 The foreman in the injection molding department says that a polyethylene part produced in one of the operations has greater shrinkage than the calculations indicate it should have. The important dimension of the part is specified as 112.5 ±0.25 mm. However, the actual molded part measures 112.02 mm. (a) As a first step, the corresponding mold cavity dimension should be checked. Compute the correct value of the mold dimension, given that the shrinkage value for polyethylene is 0.025 (from Table 13.1). (b) What adjustments in process parameters could be made to reduce the amount of shrinkage? Solution: (a) Given: S = 0.025, Dc = 112.5 + 112.5(.025) + 112.5(.025)2 = 115.383 mm
• 75. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-27-09, 04-28-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 11 (b) Adjustments to reduce shrinkage include: (1) increase injection pressure, (2) increase compaction time, and (3) increase molding temperatures. 13.21 An injection molded polyethylene part has a dimension of 2.500 in. A new material, polycarbonate, is used in the same mold. What is the expected corresponding dimension of the polycarbonate molding? Solution: For polyethylene the shrinkage is 0.025 in/in (from Table 13.1). Die Cavity = Dc = Dp + DpS + DpS2 = 2.500 + 2.500(0.025) + 2.500(0.025)2 = 2.564 in For polycarbonate, the shrinkage is 0.007 in/in Part dimension = Dc/(1 + S + S2 ) = 2.564/(1 + 0.007 + 0.0072 ) = 2.546 in Other Molding Operations and Thermoforming 13.22 The extrusion die for a polyethylene parison used in blow molding has a mean diameter of 18.0 mm. The size of the ring opening in the die is 2.0 mm. The mean diameter of the parison is observed to swell to a size of 21.5 mm after exiting the die orifice. If the diameter of the blow molded container is to be 150 mm, determine (a) the corresponding wall thickness of the container and (b) the wall thickness of the parison. Solution: (a) rs = Dp/Dd = 21.5/18.0 = 1.194 tm = tp Dp/Dm = rs td Dp/Dm = (1.194)(2.0)(21.5)/150.0 = 0.342 mm (b) tp = rs td = (1.194)(2.0) = 2.388 mm 13.23 A parison is extruded from a die with outside diameter = 11.5 mm and inside diameter = 7.5 mm. The observed die swell is 1.25. The parison is used to blow mold a beverage container whose outside diameter = 112 mm (a standard size 2-liter soda bottle). (a) What is the corresponding wall thickness of the container? (b) Obtain an empty 2-liter plastic soda bottle and (carefully) cut it across the diameter. Using a micrometer, measure the wall thickness to compare with your answer in (a). Solution: (a) Dd = (11.5 + 7.5)/2 = 9.5 mm, and td = (11.5 - 7.5)/2 = 2.0 mm tm = (1.25)2 (2.0)(9.5)/112 = 0.265 mm (= 0.010 in) (b) Measured value should be close to calculated value. Some wall thicknesses are less. 13.24 A blow-molding operation is used to produce a bottle with a diameter of 2.250 in and a wall thickness of 0.045 in. The parison has a thickness of 0.290 in. The observed die swell ratio is 1.30. (a) What is the required diameter of the parison? (b) What is the diameter of the die? Solution: (a) Dp = tmDm/tp = (0.045)(2.250)/0.290 = 0.349 in (b) Dd = Dp/rs = 0.349/1.30 = 0.268 in 13.25 An extrusion operation is used to produce a parison whose mean diameter = 27 mm. The inside and outside diameters of the die that produced the parison are 18 mm and 22 mm, respectively. If the minimum wall thickness of the blow-molded container is to be 0.40 mm, what is the maximum possible diameter of the blow mold? Solution: Dd = (22 + 18)/2 = 20 mm, and td = (22 - 18)/2 = 2 mm rs = 27/20 = 1.35 Rearranging Eq. (13.22) in text, Dm = rsd 3 tdDd/tm = (1.35)2 (2)(20)/(0.40) = 182.25 mm 13.26 A rotational molding operation is to be used to mold a hollow playing ball out of polypropylene. The ball will be 1.25 ft in diameter and its wall thickness should be 3/32 in. What weight of PP powder should be loaded into the mold in order to meet these specifications? The specific gravity of the PP grade is 0.90, and the density of water is 62.4 lb/ft3 . Solution: Density ρ = specific gravity of polymer x ρwater = 0.90(62.4 lb/ft3 ) = 56.2 lb/ft3
• 76. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-27-09, 04-28-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 12 Convert to lb/in3 : ρ = 56.2 lb/ft3 /(1728 in3 /ft3 ) = 0.0325 lb/in3 Volume = π(Do 3 - Di 3 )/6 = 0.16667π[(1.25x12)3 - (1.25x12 - 3/16)3 ] = 10.91 in3 Weight W = (10.91)(0.0325) = 0.355 lb. 13.27 The problem in a certain thermoforming operation is that there is too much thinning in the walls of the large cup-shaped part. The operation is conventional pressure thermoforming using a positive mold, and the plastic is an ABS sheet with an initial thickness of 3.2 mm. (a) Why is thinning occurring in the walls of the cup? (b) What changes could be made in the operation to correct the problem? Solution: (a) As the starting flat sheet is draped over the convex cup-shaped mold, the portion contacting the base of the cup experiences little stretching. However, the remaining portions of the sheet must be stretched significantly to conform to the sides of the cup. Hence, thinning in these sides results. (b) The problem could be solved by either: (1) fabricating a negative mold to replace the current positive mold, since a negative mold will distribute the material more uniformly and result in approximately equal thinning throughout the sheet; or (2) prestretch the sheet as in Figure 13.38 in the text.
• 82. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-01-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 4 15.10 Water jet cutting is one of several ways of cutting or trimming uncured or cured FRPs; in the case of cured FRPs, the process is noted for its reduction of dust and noise: (a) true or (b) false? Answer. (a).
• 87. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-01-09, 05-11-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 Find diameter D of a sphere of equivalent volume. V = πD3 /6 = 0.25πL3 D3 = 6(0.25πL3 )/π = 1.5L3 D = (1.5 L3 )0.333 = 1.1447 L Ks = AD/V = (1.5πL2 )(1.1447 L)/0.25πL3 = 6.868 (d) Cylinder with L/D = 2.0. For this cylinder shape, 0.5L = D. Thus, A = 2πD2 /4 + πDL = 0.5π(0.5L)2 + π(0.5L)L = 0.125πL2 + 0.5πL2 = 0.625πL2 , and V = (πD2 /4)L = 0.25π(0.5L)2 L = 0.0625πL3 Find diameter D of a sphere of equivalent volume. V = πD3 /6 = 0.0625πL3 D3 = 6(0.0625πL3 )/π = 0.375L3 D = (0.375 L3 )0.333 = 0.721 L Ks = A D/V = (0.625πL2 )(0.721 L)/0.0625πL3 = 7.211 (e) Disk with L/D = 0.10. For this shape, 10L = D. Thus, A = 2πD2 /4 + πDL = 0.5π(10L)2 + π(10L)L = 50πL2 + 10πL2 = 60πL2 , and V = (πD2 /4)L = 0.25π(10L)2 L = 25πL3 Find diameter D of a sphere of equivalent volume. V = πD3 /6 = 25πL3 D3 = 6(25πL3 )/ π = 150L3 D = (150 L3 )0.333 = 5.313 L Ks = A D/V = (60πL2 )(5.313 L)/25πL3 = 12.75 16.5 A pile of iron powder weighs 2 lb. The particles are spherical in shape and all have the same diameter of 0.002 in. (a) Determine the total surface area of all the particles in the pile. (b) If the packing factor = 0.6, determine the volume taken by the pile. Note: the density of iron = 0.284 lb/in3 . Solution: (a) For a spherical particle of D = 0.002 in, V = πD3 /6 = π(0.002)3 /6 = 0.00000000418 = 4.18 x 10-9 in3 /particle Weight per particle W = ρV = 0.284(4.18 x 10-9 in3 ) = 1.19 x 10-9 lb/particle Number of particles in 2 lb = 2.0/(1.19 x 10-9 ) = 1.681 x 109 A = πD2 = π(0.002)2 = 0.00001256 in2 = 12.56 x 10-6 in2 Total surface area = (1.681 x 109 )(12.56 x 10-6 ) = 21.116 x 103 in2 (b) With a packing factor of 0.6, the total volume taken up by the pile = (2.0/0.284)/0.6 = 11.74 in3 16.6 Solve Problem 16.5, except that the diameter of the particles is 0.004 in. Assume the same packing factor. Solution: (a) For a spherical particle of D = 0.004 in, V = πD3 /6 = π(0.004)3 /6 = 0.00000003351 = 33.51 x 10-9 in3 /particle Weight per particle W = ρV = 0.284(33.51 x 10-9 in3 ) = 9.516 x 10-9 lb/particle Number of particles in 2 lb = 2.0/(9.516 x 10-9 ) = 0.2102 x 109 A = πD2 = π(0.004)2 = 0.00005027 in2 = 50.27 x 10-6 in2 Total surface area = (0.2102 x 109 )(50.27 x 10-6 ) = 10.565 x 103 in2 (b) With a packing factor of 0.6, the total volume taken up by the pile = (2.0/0.284)/0.6 = 11.74 in3 16.7 Suppose in Problem 16.5 that the average particle diameter = 0.002 in; however, the sizes vary, forming a statistical distribution as follows: 25% of the particles by weight are 0.001 in, 50% are 0.002 in, and 25% are 0.003 in. Given this distribution, what is the total surface area of all the particles in the pile? Solution: For a spherical particle of D = 0.001 in, V = πD3 /6 = π(0.001)3 /6 = 0.5236 x 10-9 in3 /particle
• 88. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-01-09, 05-11-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 Weight per particle W = ρV = 0.284(0.5236 x 10-9 in3 ) = 0.1487 x 10-9 lb/particle Particles of size D = 0.001 in constitute 25% of total 2 lb. = 0.5 lb Number of particles in 0.5 lb = 0.5/(0.1487 x 10-9 ) = 3.362 x 109 A = πD2 = π(0.001)2 = 3.142 x 10-6 in2 /particle Total surface area of particles of D = 0.001 in = (3.362 x 109 )(3.142 x 10-6 ) = 10.563 x 103 in2 For a spherical particle of D = 0.002 in, V = π(0.002)3 /6 = 4.18 x 10-9 in3 /particle Weight per particle W = ρV = 0.284(4.18 x 10-9 in3 ) = 1.19 x 10-9 lb/particle Particles of size D = 0.002 in constitute 50% of total 2 lb. = 1.0 lb Number of particles in 1 lb = 1.0/(1.19 x 10-9 ) = 0.8406 x 109 A = πD2 = π(0.002)2 = 12.56 x 10-6 in2 Total surface area of particles of D = 0.002 in = (0.8406 x 109 )(12.566 x 10-6 ) = 10.563 x 103 in2 For a spherical particle of D = 0.003 in, V = π(0.003)3 /6 = 14.137 x 10-9 in3 /particle Weight per particle W = ρV = 0.284(14.137 x 10-9 in3 ) = 4.015 x 10-9 lb/particle Particles of size D = 0.003 in constitute 25% of total 2 lb. = 0.5 lb Number of particles in 0.5 lb = 0.5/(4.015 x 10-9 ) = 0.124 x 109 A = πD2 = π(0.003)2 = 28.274 x 10-6 in2 Total surface area of particles of D = 0.003 in = (0.124 x 109 )(28.274 x 10-6 ) = 3.506 x 103 in2 Total surface area of all particles = 10.563 x 103 + 10.563 x 103 + 3.506 x 103 = 24.632 x 103 in2 . 16.8 A solid cube of copper with each side = 1.0 ft is converted into metallic powders of spherical shape by gas atomization. What is the percentage increase in total surface area if the diameter of each particle is 0.004 in (assume that all particles are the same size)? Solution: Area of initial cube A = 6(1 ft)2 = 6 ft2 = 864 in2 Volume of cube V = (1 ft)3 = 1728 in3 Surface area of a spherical particle of D = 0.004 in is A = πD2 = π(0.004)2 = 50.265 x 10-6 in3 /particle Volume of a spherical particle of D = 0.004 in is V = πD3 /6 = π(0.004)3 /6 = 33.51 x 10-9 in3 /particle Number of particles in 1 ft3 = 1728/33.51 x 10-9 = 51.567 x 109 Total surface area = (51.567 x 109 )( 50.265 x 10-6 in3 ) = 2,592 x 103 = 2,592,000 in2 Percent increase = 100(2,592,000 - 864)/864 = 299,900% 16.9 A solid cube of aluminum with each side = 1.0 m is converted into metallic powders of spherical shape by gas atomization. How much total surface area is added by the process if the diameter of each particle is 100 microns (assume that all particles are the same size)? Solution: Area of starting cube A = 6(1 m)2 = 6 m2 Volume of starting cube V = (1 m)3 = 1 m3 D = 100 µm = 0.1 mm = 0.1 x 10-3 m Surface area of a sphere of D = 0.1 x 10-3 m is A = πD2 = π(0.1 x 10-3 )2 = 3.142 x 10-8 m3 /particle Volume of a sphere of D = 0.1 x 10-3 m is V = πD3 /6 = π(0.1 x 10-3 )3 /6 = 0.5236 x 10-12 m3 /particle Number of particles in 1 m3 = 1.0/0.5236 x 10-12 = 1.91 x 1012 Total surface area = (1.91 x 1012 )( 0.5236 x 10-12 m3 ) = 5.9958 x 104 = 59,958 m2 Added surface area = 59,958 - 6 = 59,952 m2 16.10 Given a large volume of metallic powders, all of which are perfectly spherical and having the same exact diameter, what is the maximum possible packing factor that the powders can take?
• 89. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-01-09, 05-11-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 Solution: The maximum packing factor is achieved when the spherical particles are arranged as a face-centered cubic unit cell, similar to the atomic structure of FCC metals; see Figure 2.8(b). The unit cell of the FCC structure contains 8 spheres at the corners of the cube and 6 spheres on each face. Our approach to determine the packing factor will consist of: (1) finding the volume of the spheres and portions thereof that are contained in the cell, and (2) finding the volume of the unit cell cube. The ratio of (1) over (2) is the packing factor. (1) Volume of whole and/or partial spheres contained in the unit cell. The unit cell contains 6 half spheres in the faces of the cube and 8 one-eighth spheres in corners. The equivalent number of whole spheres = 6(.5) + 8(.125) = 4 spheres. Volume of 4 spheres = 4πD3 /6 = 2.0944 D3 where D = diameter of a sphere. (2) Volume of the cube of one unit cell. Consider that the diagonal of any face of the unit cell contains one full diameter (the sphere in the center of the cube face) and two half diameters (the spheres at the corners of the face). Thus, the diagonal of the cube face = 2D. Accordingly, the face is a square with each edge = D√2 = 1.414D. The volume of the unit cell is therefore (1.414D)3 = 2.8284 D3 . The packing factor = 2.0944/2.8284 = 0.7405 = 74.05% Compaction and Design Considerations 16.11 In a certain pressing operation, the metallic powder fed into the open die has a packing factor of 0.5. The pressing operation reduces the powders to 2/3 of their starting volume. In the subsequent sintering operation, shrinkage amounts to 10% on a volume basis. Given that these are the only factors that affect the structure of the finished part, determine its final porosity. Solution: Packing factor = bulk density / true density Density = (specific volume)-1 Packing factor = true specific volume / bulk specific volume Pressing reduces bulk specific volume to 2/3 = 0.667 Sintering further reduces the bulk specific volume to 0.90 of value after pressing. Let true specific volume = 1.0 Thus for a packing factor of 0.5, bulk specific volume = 2.0. Packing factor after pressing and sintering = 1.0/(2.0 x .667 x .90) = 1.0/1.2 = 0.833 By Eq. (18.7), porosity = 1 - 0.833 = 0.167 16.12 A bearing of simple geometry is to be pressed out of bronze powders, using a compacting pressure of 207 MPa. The outside diameter = 44 mm, the inside diameter = 22 mm, and the length of the bearing = 25 mm. What is the required press tonnage to perform this operation? Solution: Projected area of part Ap = 0.25π(Do 2 - Di 2 ) = 0.25π(442 - 222 ) = 1140.4 mm2 F = Appc = 1140.4(207) = 236,062 N 16.13 The part shown in Figure P16.13 is to be pressed of iron powders using a compaction pressure of 75,000 lb/in2 . Dimensions are inches. Determine (a) the most appropriate pressing direction, (b) the required press tonnage to perform this operation, and (c) the final weight of the part if the porosity is 10%. Assume shrinkage during sintering can be neglected. Solution: (a) Most appropriate pressing direction is parallel to the part axis. (b) Press tonnage F = Appc Projected area of part Ap = 0.25π(Do 2 - Di 2 ) = 0.25π(2.82 - 0.8752 ) = 5.556 in2 F = Appc = 5.556(75,000) = 416,715 lb = 208 tons. (c) V = 0.25π(2.82 - 0.8752 )(0.5) + 0.25π(2.82 - 1.52 )(1.25 - 0.5) = 0.25π(3.5372 + 4.1925) = 6.071 in3
• 90. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-01-09, 05-11-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 From Table 4.1, density of iron ρ = 0.284 lb/in3 . At 10% porosity, part weight W = 6.071(0.284)(0.90) = 1.55 lb. 16.14 For each of the four part drawings in Figure P16.14, indicate which PM class the parts belong to, whether the part must be pressed from one or two directions, and how many levels of press control will be required? Dimensions are mm. Solution: (a) Class II, 2 directions because of axial thickness, one level of press control. (b) Class I, one direction part is relatively thin, one level of press control. (c) Class IV, 2 directions of pressing, 3 levels of press control required. (d) Class IV, 2 directions of pressing, 4 or 5 levels of press control due to multiple steps in part design.
• 96. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-12-09, 05-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3 Average flow stress fY = 550(0.85)0.22 /1.22 = 435 MPa. 18.2 A metal has a flow curve with strength coefficient = 850 MPa and strain-hardening exponent = 0.30. A tensile specimen of the metal with gage length = 100 mm is stretched to a length = 157 mm. Determine the flow stress at the new length and the average flow stress that the metal has been subjected to during the deformation. Solution: ε = ln (157/100) = ln 1.57 = 0.451 Flow stress Yf = 850(0.451)0.30 = 669.4 MPa. Average flow stress fY = 850(0.451)0.30 /1.30 = 514.9 MPa. 18.3 A particular metal has a flow curve with strength coefficient = 35,000 lb/in2 and strain-hardening exponent = 0.26. A tensile specimen of the metal with gage length = 2.0 in is stretched to a length = 3.3 in. Determine the flow stress at this new length and the average flow stress that the metal has been subjected to during deformation. Solution: ε = ln (3.3/2.0) = ln 1.65 = 0.501 Flow stress Yf = 35,000(0.501)0.26 = 29,240 lb/in2 . Average flow stress fY = 35,000(0.501)0.26 /1.26 = 23,206 lb/in2 . 18.4 The strength coefficient and strain-hardening exponent of a certain test metal are 40,000 lb/in2 and 0.19, respectively. A cylindrical specimen of the metal with starting diameter = 2.5 in and length = 3.0 in is compressed to a length of 1.5 in. Determine the flow stress at this compressed length and the average flow stress that the metal has experienced during deformation. Solution: ε = ln (1.5/3.0) = ln 0.5 = -0.69315 Flow stress Yf = 40,000(0.69315)0.19 = 37,309 lb/in2 . Average flow stress fY = 40,000(0.69315)0.19 /1.19 = 31,352 lb/in2 . 18.5 Derive the equation for average flow stress, Eq. (18.2) in the text. Solution: Flow stress equation [Eq. (18.1)]: Yf = Kεn fY over the range ε = 0 to ε = ε is given by ∫Kεn dε = K ∫εn dε = Kεn+1 /ε(n+1) = Kεn /(n+1) 18.6 For a certain metal, the strength coefficient = 700 MPa and strain-hardening exponent = 0.27. Determine the average flow stress that the metal experiences if it is subjected to a stress that is equal to its strength coefficient K. Solution: Yf = K = 700 = Kεn = 700ε.27 ε must be equal to 1.0. fY = 700(1.0).27 /1.27 = 700/1.27 = 551.2 MPa 18.7 Determine the value of the strain-hardening exponent for a metal that will cause the average flow stress to be 3/4 of the final flow stress after deformation. Solution: fY = 0.75 Yf Kεn /(1+n) = 0.75 Kεn 1/(1+n) = 0.75 1 = 0.75(1+n) = 0.75 + 0.75n 0.25 = 0.75n n = 0.333 18.8 The strength coefficient = 35,000 lb/in2 and strain-hardening exponent = 0.40 for a metal used in a forming operation in which the workpart is reduced in cross-sectional area by stretching. If the average flow stress on the part is 20,000 lb/in2 , determine the amount of reduction in cross-sectional area experienced by the part.
• 97. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-12-09, 05-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 4 Solution: fY = Kεn /(1+n) 20,000 = 35,000 ε.4 /(1.4) 1.4(20,000) = 35,000 ε.4 28,000/35,000 = 0.8 = ε.4 0.4 ln ε = ln (0.8) = -0.22314 ln ε = -0.22314/0.4 = -0.55786 ε = 0.5724 ε = ln(Ao/Af) = 0.5724 Ao/Af = 1.7726 Af = Ao/1.7726 = 0.564Ao 18.9 In a tensile test, two pairs of values of stress and strain were measured for the specimen metal after it had yielded: (1) true stress = 217 MPa and true strain = 0.35, and (2) true stress = 259 MPa and true strain = 0.68. Based on these data points, determine the strength coefficient and strain-hardening exponent. Solution: Solve two equations, two unknowns: ln K = ln σ - n ln ε (1) ln K = ln 217 – n ln 0.35 (2) ln K = ln 259 – n ln 0.68 (1) ln K = 5.3799 – (-1.0498)n = 5.3799 + 1.0498 n (2) ln K = 5.5568 – (-0.3857)n = 5.5568 + 0.3857 n 5.3799 + 1.0498 n = 5.5568 + 0.3857 n 1.0498 n – 0.3857 n = 5.5568 – 5.3799 0.6641 n = 0.1769 n = 0.2664 ln K = 5.3799 + 1.0498 (0.2664) = 5.6596 K = 287 MPa 18.10 The following stress and strain values were measured in the plastic region during a tensile test carried out on a new experimental metal: (1) true stress = 43,608 lb/in2 and true strain = 0.27 in/in, and (2) true stress = 52,048 lb/in2 and true strain = 0.85 in/in. Based on these data points, determine the strength coefficient and strain-hardening exponent. Solution: Solve two equations, two unknowns: ln K = ln σ - n ln ε (3) ln K = ln 43,608 – n ln 0.27 (4) ln K = ln 52,048 – n ln 0.85 (3) ln K = 10.6830 – (-1.3093)n = 10.6830 + 1.3093 n (4) ln K = 10.8600 – (-0.1625)n = 10.8600 + 0.1625 n (5) 10.6830 + 1.3093 n = 10.8600 + 0.1625 n 1.3093 n – 0.1625 n = 10.8600 – 10.6830 1.1468 n = 0.1769 n = 0.1543 ln K = 10.6830 + 1.3093 (0.1543) = 10.885 K = 53,374 lb/in2 Strain Rate 18.11 The gage length of a tensile test specimen = 150 mm. It is subjected to a tensile test in which the grips holding the end of the test specimen are moved with a relative velocity = 0.1 m/s. Construct a plot of the strain rate as a function of length as the specimen is pulled to a length = 200 mm. Solution: The following values are calculated for the plot: At L = 150 mm, strain rate ε = 0.1/0.15 = 0.667 s-1 At L = 160 mm, strain rate ε = 0.1/0.16 = 0.625 s-1 At L = 170 mm, strain rate ε = 0.1/0.17 = 0.588 s-1 At L = 180 mm, strain rate ε = 0.1/0.18 = 0.555 s-1 At L = 190 mm, strain rate ε = 0.1/0.19 = 0.526 s-1 At L = 200 mm, strain rate ε = 0.1/0.20 = 0.500 s-1
• 98. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-12-09, 05-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 18.12 A specimen with 6.0 in starting gage length is subjected to a tensile test in which the grips holding the end of the test specimen are moved with a relative velocity = 1.0 in/sec. Construct a plot of the strain rate as a function of length as the specimen is pulled to a length = 8.0 in. Solution: The following values are calculated for the plot: At L = 6.0 in, strain rate ε = 1/6.0 = 0.1667 sec-1 At L = 6.5 in, strain rate ε = 1/6.5 = 0.1538 sec-1 At L = 7.0 in, strain rate ε = 1/7.0 = 0.1429 sec-1 At L = 7.5 in, strain rate ε = 1/7.5 = 0.1333 sec-1 At L = 8.0 in, strain rate ε = 1/8.0 = 0.1250 sec-1 18.13 A workpart with starting height h = 100 mm is compressed to a final height of 50 mm. During the deformation, the relative speed of the plattens compressing the part = 200 mm/s. Determine the strain rate at (a) h = 100 mm, (b) h = 75 mm, and (c) h = 51 mm. Solution: (a) strain rate ε = 200/100 = 2.0 s-1 (b) strain rate ε = 200/75 = 2.667 s-1 (c) strain rate ε = 200/51 = 3.922 s-1 18.14 A hot working operation is carried out at various speeds. The strength constant = 30,000 lb/in2 and the strain-rate sensitivity exponent = 0.15. Determine the flow stress if the strain rate is (a) 0.01/sec (b) 1.0/sec, (c) 100/sec. Solution: (a) Yf = C(ε )m = 30,000(0.01).15 = 15,036 lb/in2 (b) Yf = 30,000(1.0)0.15 = 30,000 lb/in2 (c) Yf = 30,000(100)0.15 = 59,858 lb/in2 18.15 A tensile test is performed to determine the strength constant C and strain-rate sensitivity exponent m in Eq. (18.4) for a certain metal. The temperature at which the test is performed = 500°C. At a strain rate = 12/s, the stress is measured at 160 MPa; and at a strain rate = 250/s, the stress = 300 MPa. (a) Determine C and m. (b) If the temperature were 600°C, what changes would you expect in the values of C and m? Solution: (a) Two equations: (1) 160 = C(12)m and (2) 300 = C(250)m (1) ln 160 = ln C + m ln 12 or ln 160 - m ln 12 = ln C (2) ln 300 = ln C + m ln 250 or ln 300 - m ln 250 = ln C (1) and (2): ln 160 - m ln 12 = ln 300 - m ln 250 5.0752 – 2.4849 m = 5.7038 – 5.5215 m (5.5215 – 2.4849)m = 5.7038 – 5.0752 3.0366 m = 0.6286 m = 0.207 (1) C = 160/(12)0.207 = 160.1.6726 = 95.658 (2) C = 300/(250)0.207 = 300/3.1361 = 95.660 Averaging these values, C = 95.659 (b) If temperature were 600°C, the strength constant C would decrease and the strain-rate sensitivity exponent m would increase. 18.16 A tensile test is carried out to determine the strength constant C and strain-rate sensitivity exponent m for a certain metal at 1000°F. At a strain rate = 10/sec, the stress is measured at 23,000 lb/in2 ; and at a strain rate = 300/sec, the stress = 45,000 lb/in2 . (a) Determine C and m. (b) If the temperature were 900°F, what changes would you expect in the values of C and m? Solution: (a) Two equations: (1) 23,000 = C(10)m and (2) 45,000 = C(300)m 45,000/23,000 = 1.9565 = (300/10)m = (30)m
• 99. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 05-12-09, 05-13-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 ln 1.9656 = m ln 30 0.67117 = 3.4012 m m = 0.1973 (1) C = 23000/100.1973 = 23000/1.5752 = 14,601.4 (2) C = 45000/3000.1973 = 45000/3.0819 = 14,601.4 C = 14,601.4 (b) If temperature were decreased to 900°F, the strength constant C would increase and the strain- rate sensitivity exponent m would decrease.
• 105. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 102 Step 1: vf = (2.0)(10.0)(40)/(0.75 x 2.0)(1.03 x 10.0) = 51.78 ft/min Step 2: vf = (0.75 x 2.0)(1.03 x 10.0)(40)/(0.752 x 2.0)(1.032 x 10.0) = 51.78 ft/min Step 3: vf = (0.752 x 2.0)(1.032 x 10.0)(40)/(0.753 x 2.0)(1.033 x 10.0) = 51.78 ft/min 19.3 A series of cold rolling operations are to be used to reduce the thickness of a plate from 50 mm down to 25 mm in a reversing two-high mill. Roll diameter = 700 mm and coefficient of friction between rolls and work = 0.15. The specification is that the draft is to be equal on each pass. Determine (a) minimum number of passes required, and (b) draft for each pass? Solution: (a) Maximum draft dmax = µ2 R = (0.15)2 (350) = 7.875 mm Minimum number of passes = (to - tf)/dmax = (50 - 25)/7.875 = 3.17 → 4 passes (b) Draft per pass d = (50 - 25)/4 = 6.25 mm 19.4 In the previous problem, suppose that the percent reduction were specified to be equal for each pass, rather than the draft. (a) What is the minimum number of passes required? (b) What is the draft for each pass? Solution: (a) Maximum possible draft occurs on first pass: dmax = µ2 R = (0.15)2 (350) = 7.875 mm This converts into a maximum possible reduction x = 7.875/50 = 0.1575 Let x = fraction reduction per pass, and n = number of passes. The number of passes must be an integer. To reduce from to = 50 mm to to = 25 mm in n passes, the following relationship must be satisfied: 50(1 - x)n = 25 (1 - x)n = 25/50 = 0.5 (1 - x) = 0.51/n Try n = 4: (1 - x) = (0.5)1/4 = 0.8409 x = 1 - 0.8409 = 0.1591, which exceeds the maximum possible reduction of 0.1575. Try n = 5: (1 - x) = (0.5)1/5 = 0.87055 x = 1 - 0.87055 = 0.12945, which is within the maximum possible reduction of 0.1575. (b) Pass 1: d = 50(0.12945) = 6.47 mm, tf = 50 - 6.47 = 43.53 mm Pass 2: d = 43.53(0.12945) = 5.63 mm, tf = 43.53 - 5.63 = 37.89 mm Pass 3: d = 37.89(0.12945) = 4.91 mm, tf = 37.89 - 4.91 = 32.98 mm Pass 4: d = 32.98(0.12945) = 4.27 mm, tf = 32.98 - 4.27 = 28.71 mm Pass 5: d = 28.71(0.12945) = 3.71 mm, tf = 28.71 - 3.71 = 25.00 mm 19.5 A continuous hot rolling mill has two stands. Thickness of the starting plate = 25 mm and width = 300 mm. Final thickness is to be 13 mm. Roll radius at each stand = 250 mm. Rotational speed at the first stand = 20 rev/min. Equal drafts of 6 mm are to be taken at each stand. The plate is wide enough relative to its thickness that no increase in width occurs. Under the assumption that the forward slip is equal at each stand, determine (a) speed vr at each stand, and (b) forward slip s. (c) Also, determine the exiting speeds at each rolling stand, if the entering speed at the first stand = 26 m/min. Solution: (a) Let to = entering plate thickness at stand 1. to = 25 mm. Let t1 = exiting plate thickness at stand 1 and entering thickness at stand 2. t1 = 25 - 6 = 19 mm. Let t2 = exiting plate thickness at stand 2. t2 = 19 - 6 = 13 mm. Let vo = entering plate speed at stand 1. Let v1 = exiting plate speed at stand 1 and entering speed at stand 2. Let v2 = exiting plate speed at stand 2. Let vr1 = roll speed at stand 1. vr1 = πDNr = π(2 x 250)(10-3 )(20) = 31.42 m/min Let vr2 = roll speed at stand 2. vr2 = ? Forward slip s = (vf - vr)/vr svr = vf - vr (1 + s)vr = vf
• 106. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 103 At stand 1, (1 + s)vr1 = v1 (Eq. 1) At stand 2, (1 + s)vr2 = v2 (Eq. 2) By constant volume, towovo = t1w1v1 = t2w2v2 Since there is no change in width, wo = w1 = w2 Therefore, tovo = t1v1 = t2v2 1.0vo = 0.75v1 = 0.50v2 v2 = 1.5v1 (Eq. 3) Combining (Eqs. 2 and 3), (1 + s)vr2 = v2 = 1.5v1 Substituting (Eq. 1), (1 + s)vr2 = 1.5(1 + s)vr1 , thus vr2 = 1.5vr1 vr2 = 1.5(31.42) = 47.1 m/min (b) 25vo = 19v1 v1 = 25(26)/19 = 34.2 m/min (Eq. 1): (1 + s)vr1 = v1 (1 + s)(31.4) = 34.2 (1 + s) = 34.2/31.4 = 1.089 s = 0.089 (c) v1 = 34.2 m/min, previously calculated in (b) v2 = 1.5v1 = 1.5(34.2) = 51.3 m/min 19.6 A continuous hot rolling mill has eight stands. The dimensions of the starting slab are: thickness = 3.0 in, width = 15.0 in, and length = 10 ft. The final thickness is to be 0.3 in. Roll diameter at each stand = 36 in, and rotational speed at stand number 1 = 30 rev/min. It is observed that the speed of the slab entering stand 1 = 240 ft/min. Assume that no widening of the slab occurs during the rolling sequence. Percent reduction in thickness is to be equal at all stands, and it is assumed that the forward slip will be equal at each stand. Determine (a) percent reduction at each stand, (b) rotational speed of the rolls at stands 2 through 8, and (c) forward slip. (d) What is the draft at stands 1 and 8? (e) What is the length and exit speed of the final strip exiting stand 8? Solution: (a) To reduce from to = 3.0 in to tf = 0.3 in over 8 stands, 3.0(1 - x)8 = 0.3 (1 - x)8 = 0.3/3.0 = 0.10 (1 - x) = (0.10)1/8 = 0.74989 x = 1 - 0.74989 = r = 0.2501 = 25.01% at each stand. (b) Forward slip s = (vf - vr)/vr svr = vf - vr (1 + s)vr = vf At stand 1: (1 + s)vr1 = v1 , where vr1 = roll speed, v1 = exit speed of slab. At stand 2: (1 + s)vr2 = v2 , where vr2 = roll speed, v2 = exit speed of slab. Etc. At stand 8: (1 + s)vr8 = v8, where vr8 = roll speed, v8 = exit speed of slab. By constant volume, towovo = t1w1v1 = t2w2v2 = . . . = t8w8v8 Since there is no change in width, wo = w1 = w2 = . . . w8 Therefore, tovo = t1v1 = t2v2 = . . . = t8v8 to = 3.0, 3vo = 3(1 - r)v1 = 3(1 - r)2 v2 = . . . 3(1 - r)8 v8 , where r = 0.2501 as determined in part (a). Since s is a constant, vr1 : vr2 : . . . : vr8 = v1 : v2 : . . . : v8 Given that Nr1 = 30 rev/min, vr1 = πDNr1 = (2π x 18/12)(30) = 282.78 ft/min In general Nr = (30/282.78) = 0.10609vr Nr2 = 0.10609 x 282.78/(1-r) = 0.10609 x 282.78/(1-0.2501) = 40 rev/min Nr3 = 0.10609 x 282.78/(1-r)2 = 53.3 rev/min Nr4 = 0.10609 x 282.78/(1-r)3 = 71.1 rev/min Nr5 = 0.10609 x 282.78/(1-r)4 = 94.9 rev/min
• 107. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 104 Nr6 = 0.10609 x 282.78/(1-r)5 = 126.9.3 rev/min Nr7 = 0.10609 x 282.78/(1-r)6 = 168.5 rev/min Nr8 = 0.10609 x 282.78/(1-r)7 = 224.9 rev/min (c) Given vo = 240 ft/min v1 = 240/(1-r) = 240/0.74989 = 320 ft/min v2 = 320/0.74989 = 426.8 ft/min From equations for forward slip, (1 + s)vr1 = v1 (1 + s)(282.78) = 320 (1 + s) = 320/282.78 = 1.132 s = 0.132 Check with stand 2: given v2 = 426.8 ft/min from above Nr2 = 0.10609vr2 Rearranging, vr2 = Nr2/0.10609 = 9.426Nr2 = 0.426(40) = 377.04 ft/min (1 + s)(377.04) = 426.8 (1 + s) = 426.8/377.14 = 1.132 s = 0.132, as before (d) Draft at stand 1 d1 = 3.0(0.2501) = 0.7503 in Draft at stand 8 d8 = 3.0(1 - 0.2501)7 (0.2501) = 0.10006 in (e) Length of final strip Lf = L8 towoLo = t8w8L8 Given that wo = w8, toLo = t8L8 3.0(10 ft) = 0.3L8 L8 = 100 ft towovo = t8w8v8 tovo = t8v8 v8 = 240(3/0.3) = 2400 ft/min 19.7 A plate that is 250 mm wide and 25 mm thick is to be reduced in a single pass in a two-high rolling mill to a thickness of 20 mm. The roll has a radius = 500 mm, and its speed = 30 m/min. The work material has a strength coefficient = 240 MPa and a strain hardening exponent = 0.2. Determine (a) roll force, (b) roll torque, and (c) power required to accomplish this operation. Solution: (a) Draft d = 25 - 20 = 5 mm, Contact length L = (500 x 5).5 = 50 mm True strain ε = ln(25/20) = ln 1.25 = 0.223 fY = 240(0.223)0.20 /1.20 = 148.1 MPa Rolling force F = 148.1(250)(50) = 1,851,829 N (b) Torque T = 0.5(1,851,829)( 50 x 10-3 ) = 46,296 N-m (c) N = (30 m/min)/(2π x 0.500) = 9.55 rev/min = 0.159 rev/s Power P = 2π(0.159)(1,851,829)(50 x 10-3 ) = 92,591 N-m/s = 92,591 W 19.8 Solve Problem 19.7 using a roll radius = 250 mm. Solution: (a) Draft d = 25 - 20 = 5 mm, Contact length L = (250 x 5).5 = 35.35 mm True strain ε = ln(25/20) = ln 1.25 = 0.223 fY = 240(0.223)0.20 /1.20 = 148.1 MPa Rolling force F = 148.1(250)(35.35) = 1,311,095 N (b) Torque T = 0.5(1,311,095)(35.35 x 10-3 ) = 23,174 N-m (c) N = (30 m/min)/(2π x 0.250) = 19.1 rev/min = 0.318 rev/s Power P = 2π(0.318)(1,311,095)(35.35 x 10-3 ) = 92,604 N-m/s = 92,604 W
• 108. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 105 Note that the force and torque are reduced as roll radius is reduced, but that the power remains the same (within calculation error) as in the previous problem. 19.9 Solve Problem 19.7, only assume a cluster mill with working rolls of radius = 50 mm. Compare the results with the previous two problems, and note the important effect of roll radius on force, torque and power. Solution: (a) Draft d = 25 - 20 = 5 mm, Contact length L = (50 x 5).5 = 15.81 mm True strain ε = ln(25/20) = ln 1.25 = 0.223 fY = 240(0.223)0.20 /1.20 = 148.1 MPa Rolling force F = 148.1(250)(15.81) = 585,417 N (b) Torque T = 0.5(585,417)(15.81 x 10-3 ) = 4,628 N-m (c) N = (30 m/min)/(2π x 0.050) = 95.5 rev/min = 1.592 rev/s Power P = 2π(1.592)(585,417)(15.81 x 10-3 ) = 92,554 N-m/s = 92,554 W Note that this is the same power value (within calculation error) as in Problems 19.7 and 19.8. In fact, power would probably increase because of lower mechanical efficiency in the cluster type rolling mill. 19.10 A 4.50-in-thick slab that is 9 in wide and 24 in long is to be reduced in a single pass in a two-high rolling mill to a thickness of 3.87 in. The roll rotates at a speed of 5.50 rev/min and has a radius of 17.0 in. The work material has a strength coefficient = 30,000 lb/in2 and a strain hardening exponent = 0.15. Determine (a) roll force, (b) roll torque, and (c) power required to accomplish this operation. Solution: (a) Draft d = 4.50 – 3.87 = 0.63 in, Contact length L = (17.0 x 0.63)0.5 = 3.27 in True strain ε = ln(4.5/3.87) = ln 1.16 = 0.1508 fY = 30,000(0.1508)0.15 /1.15 = 19,642 lb/in2 Rolling force F = fY wL = 16,414(9.0)(3.27) = 483,000 lb (b) Torque T = 0.5FL = 0.5(483000)(3.27) = 789,700 in-lb. (c) N = 5.50 rev/min Power P = 2π(5.50)(483000)(3.27) = 54,580,500 in-lb/min HP = (54,580,500 in-lb/min)/(396,000) = 138 hp 19.11 A single-pass rolling operation reduces a 20 mm thick plate to 18 mm. The starting plate is 200 mm wide. Roll radius = 250 mm and rotational speed = 12 rev/min. The work material has a strength coefficient = 600 MPa and a strength coefficient = 0.22. Determine (a) roll force, (b) roll torque, and (c) power required for this operation. Solution: (a) Draft d = 20 - 18 = 2.0 mm, Contact length L = (250 x 2).5 = 11.18 mm = 0.0112 m True strain ε = ln(20/18) = ln 1.111 = 0.1054 fY = 600(0.1054)0.22 /1.22 = 300 MPa Rolling force F = 300(0.0112)(0.2) = 0.672 MN = 672,000 N (b) Torque T = 0.5(672,000)(0.0112) = 3,720 N-m (c) Given that N = 12 rev/min Power P = 2π(12/60)(672,000)(0.0112) = 37,697 W 19.12 A hot rolling mill has rolls of diameter = 24 in. It can exert a maximum force = 400,000 lb. The mill has a maximum horsepower = 100 hp. It is desired to reduce a 1.5 in thick plate by the maximum
• 109. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 106 possible draft in one pass. The starting plate is 10 in wide. In the heated condition, the work material has a strength coefficient = 20,000 lb/in2 and a strain hardening exponent = zero. Determine (a) maximum possible draft, (b) associated true strain, and (c) maximum speed of the rolls for the operation. Solution: (a) Assumption: maximum possible draft is determined by the force capability of the rolling mill and not by coefficient of friction between the rolls and the work. Draft d = 1.5 - tf Contact length L = (12d)0.5 fY = 20,000(ε)0 /1.0 = 20,000 lb/in2 Force F = 20,000(10) (12d)0.5 = 400,000 (the limiting force of the rolling mill) (12d)0.5 = 400,000/200,000 = 2.0 12 d = 2.02 = 4 d = 4/12 = 0.333 in (b) True strain ε = ln(1.5/tf) tf = to -d = 1.5 - 0.333 = 1.167 in ε = ln(1.5/1.167) = ln 1.285 = 0.251 (c) Given maximum possible power HP = 100 hp = 100 x 396000 (in-lb/min)/hp = 39,600,000 in- lb/min Contact length L = (12 x 0.333)0.5 = 2.0 in P = 2πN(400,000)(2.0) = 5,026,548N in-lb/min 5,026,548N = 39,600,000 N = 7.88 rev/min vr = 2πRN = 2π(12/12)(7.88) = 49.5 ft/min 19.13 Solve Problem 19.12 except that the operation is warm rolling and the strain-hardening exponent is 0.18. Assume the strength coefficient remains at 20,000 lb/in2 . Solution: (a) Assumption (same as in previous problem): maximum possible draft is determined by the force capability of the rolling mill and not by coefficient of friction between the rolls and the work. Draft d = 1.5 - tf Contact length L = (12d)0.5 ε = ln(1.5/tf) fY = 20,000(ε)0.18 /1.18 = 16,949ε.18 F = Y f (10)(12d)0.5 = 34.641 fY (d)0.5 = 400,000 (as given) fY (d)0.5 = 400,000/34.641 = 11,547 Now use trial-and-error to values of fY and d that fit this equation. Try d = 0.3 in, tf = 1.5 - 0.3 = 1.2 in ε = ln(1.5/1.2) = ln 1.25 = 0.223 fY = 16,949(0.223).18 = 13,134 lb/in2 . (d)0.5 = 11,547/13,134 = 0.8791 d = 0.773, which does not equal the initial trial value of d = 0.3 Try d = 0.5 in, tf = 1.5 - 0.5 = 1.0 in ε = ln(1.5/1.0) = ln 1.50 = 0.4055 fY = 16,949(0.4055).18 = 14,538 lb/in2 . (d)0.5 = 11,547/14,538 = 0.7942 d = 0.631, which does not equal the trial value of d = 0.5
• 110. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 107 Try d = 0.6 in, tf = 1.5 - 0.6= 0.9 in ε = ln(1.5/0.9) = 0.5108 fY = 16,949(0.5108).18 = 15,120 lb/in2 . (d)0.5 = 11,547/15,120 = 0.7637 d = 0.583, which is too much compared to d = 0.6 Try d = 0.58 in, tf = 1.5 - 0.58 = 0.92 in ε = ln(1.5/0.92) = ln 1.579 = 0.489 fY = 16,949(0.489).18 = 15,007 lb/in2 . (d)0.5 = 11,547/15,007 = 0.769 d = 0.592, which is close but still above the trial value of d = 0.55 Try d = 0.585 in, tf = 1.50 - 0.585 = 0.915 in ε = ln(1.5/0.915) = 0.494 fY = 16,949(0.494).18 = 15,036 lb/in2 . (d)0.5 = 11,547/15,036 = 0.768 d = 0.590, which is close but still above the trial value of d = 0.585. Try d = 0.588 in, tf = 1.50 - 0.588 = 0.912 in ε = ln(1.5/0.912) = 0.498 fY = 16,949(0.498).18 = 15,053 lb/in2 . (d)0.5 = 11,547/15,053 = 0.767 d = 0.588, which is almost the same as the trial value of d = 0.588. (b) True strain ε = ln(1.5/0.912) = 0.498 (c) Given maximum possible power HP = 100 hp = 100 x 396000 (in-lb/min)/hp = 39,600,000 in-lb/min Contact length L = (12 x 0.588)0.5 = 2.66 in P = 2πN(400,000)(2.66) = 6,685,000N in-lb/min 6,486,000N = 39,600,000 N = 5.92 rev/min vr = 2πRN = 2π(12/12)(5.92) = 37.2 ft/min Forging 19.14 A cylindrical part is warm upset forged in an open die. The initial diameter is 45 mm and the initial height is 40 mm. The height after forging is 25 mm. The coefficient of friction at the die-work interface is 0.20. The yield strength of the work material is 285 MPa, and its flow curve is defined by a strength coefficient of 600 MPa and a strain-hardening exponent of 0.12. Determine the force in the operation (a) just as the yield point is reached (yield at strain = 0.002), (b) at a height of 35 mm, (c) at a height of 30 mm, and (d) at a height of 25 mm. Use of a spreadsheet calculator is recommended. Solution: (a) V = πD2 L/4 = π(45)2 (40)/4 = 63,617 mm3 Given ε = 0.002, Yf = 600(0.002)0.12 = 284.6 MPa, and h = 40 - 40(0.002) = 39.92 A = V/h = 63,617/39.92 = 1594 mm2 Kf = 1 + 0.4(0.2)(45)/39.92 = 1.09 F = 1.09(284.6)(1594) = 494,400 N (b) Given h = 35, ε = ln(40/35) = ln 1.143 = 0.1335 Yf = 600(0.1335)0.12 = 471.2 MPa V = 63,617 mm3 from part (a) above. At h = 35, A = V/h = 63617/35 = 1818 mm2
• 111. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 108 Corresponding D = 48.1 mm (from A = πD2 /4) Kf = 1 + 0.4(0.2)(48.1)/35 = 1.110 F = 1.110(471.2)(1818) = 950,700 N (c) Given h = 30, ε = ln(40/30) = ln 1.333 = 0.2877 Yf = 600(0.2877)0.12 = 516.7 MPa V = 63,617 mm3 from part (a) above. At h = 30, A = V/h = 63,617/30 = 2120.6 mm2 Corresponding D = 51.96 mm (from A = πD2 /4) Kf = 1 + 0.4(0.2)(51.96)/30 = 1.138 F = 1.138(516.7)(2120.6) = 1,247,536 N (d) Given h = 25, ε = ln(40/25) = ln 1.6 = 0.4700 Yf = 600(0.470)0.12 = 548.0 MPa V = 63,617 mm3 from part (a) above. At h = 25, A = V/h = 63,617/25 = 2545 mm2 Corresponding D = 56.9 mm (from A = πD2 /4) Kf = 1 + 0.4(0.2)(56.9)/25 = 1.182 F = 1.182(548.0)(2545) = 1,649,000 N 19.15 A cylindrical workpart with D = 2.5 in and h = 2.5 in is upset forged in an open die to a height = 1.5 in. Coefficient of friction at the die-work interface = 0.10. The work material has a flow curve defined by: K = 40,000 lb/in2 and n = 0.15. Yield strength = 15,750 lb/in2 . Determine the instantaneous force in the operation (a) just as the yield point is reached (yield at strain = 0.002), (b) at height h = 2.3 in, (c) h = 2.1 in, (d) h = 1.9 in, (e) h = 1.7 in, and (f) h = 1.5 in. Use of a spreadsheet calculator is recommended. Solution: (a) V = πD2 L/4 = π(2.5)2 (2.5)/4 = 12.273 in3 Given ε = 0.002, Yf = 40,000(0.002)0.15 = 15,748 lb/in2 and h = 2.5 - 2.5(0.002) = 2.495 A = V/h = 12.273/2.495 = 4.92 in2 Kf = 1 + 0.4(0.1)(2.5)/2.495 = 1.04 F = 1.04(15,748)(4.92) = 80,579 lb (b) Given h = 2.3, ε = ln(2.5/2.3) = ln 1.087 = 0.0834 Yf = 40,000(0.0834)0.15 = 27,556 lb/in2 V = 12.273 in3 from part (a) above. At h = 2.3, A = V/h = 12.273/2.3 = 5.34 in2 Corresponding D = 2.61 (from A = πD2 /4) Kf = 1 + 0.4(0.1)(2.61)/2.3 = 1.045 F = 1.045(27,556)(5.34) = 153,822 lb (c) Given h = 2.1, ε = ln(2.5/2.1) = ln 1.191 = 0.1744 Yf = 40,000(0.1744)0.15 = 30,780 lb/in2 V = 12.273 in3 from part (a) above. At h = 2.1, A = V/h = 12.273/2.1 = 5.84 in2 Corresponding D = 2.73 (from A = πD2 /4) Kf = 1 + 0.4(0.1)(2.73)/2.1 = 1.052 F = 1.052(30,780)(5.84) = 189,236 lb (d) Given h = 1.9, ε = ln(2.5/1.9) = ln 1.316 = 0.274 Yf = 40,000(0.274)0.15 = 32,948 lb/in2 V = 12.273 in3 from part (a) above. At h = 1.9, A = V/h = 12.273/1.9 = 6.46 in2 Corresponding D = 2.87 (from A = πD2 /4)
• 112. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 109 Kf = 1 + 0.4(0.1)(2.87)/1.9 = 1.060 F = 1.060(32,948)(6.46) = 225,695 lb (e) Given h = 1.7, ε = ln(2.5/1.7) = ln 1.471 = 0.386 Yf = 40,000(0.386)0.15 = 34,673 lb/in2 V = 12.273 in3 from part (a) above. At h = 1.7, A = V/h = 12.273/1.7 = 7.22 in2 Corresponding D = 3.03 (from A = πD2 /4) Kf = 1 + 0.4(0.1)(3.03)/1.7 = 1.071 F = 1.071(34,673)(7.22) = 268,176 lb (f) Given h = 1.5, ε = ln(2.5/1.5) = ln 1.667 = 0.511 Yf = 40,000(0.511)0.15 = 36,166 lb/in2 V = 12.273 in3 from part (a) above. At h = 1.5, A = V/h = 12.273/1.5 = 8.182 in2 Corresponding D = 3.23 (from A = πD2 /4) Kf = 1 + 0.4(0.1)(3.23)/1.5 = 1.086 F = 1.086(36,166)(8.182) = 321,379 lb 19.16 A cylindrical workpart has a diameter = 2.5 in and a height = 4.0 in. It is upset forged to a height = 2.75 in. Coefficient of friction at the die-work interface = 0.10. The work material has a flow curve with strength coefficient = 25,000 lb/in2 and strain hardening exponent = 0.22. Determine the plot of force vs. work height. Use of a spreadsheet calculator is recommended. Solution: Volume of cylinder V = πD2 L/4 = π(2.5)2 (4.0)/4 = 19.635 in3 We will compute the force F at selected values of height h: h = (a) 4.0, (b) 3.75, (c) 3.5, (d) 3.25, (e) 3.0, (f) 2.75, and (g) 2.5. These values can be used to develop the plot. The shape of the plot will be similar to Figure 21.13 in the text. At h = 4.0, we assume yielding has just occurred and the height has not changed significantly. Use ε = 0.002 (the approximate yield point of metal). At ε = 0.002, Yf = 25,000(0.002)0.22 = 6,370 lb/in2 Adjusting the height for this strain, h = 4.0 - 4.0(0.002) = 3.992 A = V/h = 19.635/3.992 = 4.92 in2 Kf = 1 + 0.4(0.1)(2.5)/3.992 = 1.025 F = 1.025(6,370)(4.92) = 32,125 lb At h = 3.75, ε = ln(4.0/3.75) = ln 1.0667 = 0.0645 Yf = 25,000(0.0645)0.22 = 13,680 lb/in2 V = 19.635 in3 calculated above. At h = 3.75, A = V/h = 19.635/3.75 = 5.236 in2 Corresponding D = 2.582 (from A = πD2 /4) Kf = 1 + 0.4(0.1)(2.582)/3.75 = 1.028 F = 1.028(13,680)(5.236) = 73,601 lb At h = 3.5, ε = ln(4.0/3.5) = ln 1.143 = 0.1335 Yf = 25,000(0.1335)0.22 = 16,053 lb/in2 At h = 3.5, A = V/h = 19.635/3.5 = 5.61 in2 Corresponding D = 2.673 (from A = πD2 /4) Kf = 1 + 0.4(0.1)(2.673)/3.5 = 1.031 F = 1.031(16,053)(5.61) = 92,808 lb At h = 3.25, ε = ln(4.0/3.25) = ln 1.231 = 0.2076 Yf = 25,000(0.2076)0.22 = 17,691 lb/in2 At h = 3.25, A = V/h = 19.635/3.25 = 6.042 in2
• 114. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 111 Yf = 85(1.3863)0 = 85 MPa Force is maximum at largest area value, Af = 1963.5 mm2 D = (4 x 1963.5/π)0.5 = 50 mm Kf = 1 + 0.4(0.4)(50/12.5) = 1.64 F = 1.64(85)(1963.5) = 273,712 N 19.20 A hydraulic forging press is capable of exerting a maximum force = 1,000,000 N. A cylindrical workpart is to be cold upset forged. The starting part has diameter = 30 mm and height = 30 mm. The flow curve of the metal is defined by K = 400 MPa and n = 0.2. Determine the maximum reduction in height to which the part can be compressed with this forging press, if the coefficient of friction = 0.1. Use of a spreadsheet calculator is recommended. Solution: Volume of work V = πDo 2 ho/4 = π(30)2 (30)/4 = 21,206 mm3 . Final area Af = 21,206/hf ε = ln(30/hf) Yf = 400ε0.2 = 400(ln 30/hf)0.2 ) Kf = 1 + 0.4µ(Df/hf) = 1 + 0.4(0.1)(Df/hf) Forging force F = KfYfAf = (1 + 0.04Df/hf)( 400(ln 30/hf)0.2 )( 21,206/hf) Requires trial and error solution to find the value of hf that will match the force of 1,000,000 N. (1) Try hf = 20 mm Af = 21,206/20 = 1060.3 mm2 ε = ln(30/20) = ln 1.5 = 0.405 Yf = 400(0.405)0.2 = 333.9 MPa Df = (4 x 1060.3/π)0.5 = 36.7 mm Kf = 1 + 0.04(36.7/20) = 1.073 F = 1.073(333.9)(1060.3) = 380,050 N Too low. Try a smaller value of hf to increase F. (2) Try hf = 10 mm. Af = 21,206/10 = 2120.6 mm2 ε = ln(30/10) = ln 3.0 = 1.099 Yf = 400(1.099)0.2 = 407.6 MPa Df = (4 x 2120.6/π)0.5 = 51.96 mm Kf = 1 + 0.04(51.96/10) = 1.208 F = 1.208(407.6)(2120.6) = 1,043,998 N Slightly high. Need to try a value of hf between 10 and 20, closer to 10. (3) Try hf = 11 mm Af = 21,206/11 = 1927.8 mm2 ε = ln(30/11) = ln 2.7273 = 1.003 Yf = 400(1.003)0.2 = 400.3 MPa Df = (4 x 1927.8/π)0.5 = 49.54 mm Kf = 1 + 0.04(51.12/11) = 1.18 F = 1.18(400.3)(1927.8) = 910,653 N (4) By linear interpolation, try hf = 10 + (44/133) = 10.33 mm Af = 21,206/10.33 = 2052.8 mm2 ε = ln(30/10.33) = ln 2.9042 = 1.066 Yf = 400(1.066)0.2 = 405.16 MPa Df = (4 x 2052.8/π)0.5 = 51.12 mm Kf = 1 + 0.04(51.12/10.33) = 1.198 F = 1.198(405.16)(2052.8) = 996,364 N
• 115. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 112 (5) By further linear interpolation, try hf = 10 + (44/48)(0.33) = 10.30 Af = 21,206/10.30 = 2058.8 mm2 ε = ln(30/10.30) = ln 2.913 = 1.069 Yf = 400(1.069)0.2 = 405.38 MPa Df = (4 x 2058.8/π)0.5 = 51.2 mm Kf = 1 + 0.04(51.2/10.3) = 1.199 F = 1.199(405.38)(2058.8) = 1,000,553 N Close enough! Maximum height reduction = 30.0 - 10.3 = 19.7 mm Using a spreadsheet calculator, the author’s program (written in Excel) obtained a value of h = 19.69603 mm to achieve a force of 1,000,000 lb within one pound. 19.21 A part is designed to be hot forged in an impression die. The projected area of the part, including flash, is 16 in2 . After trimming, the part has a projected area of 10 in2 . Part geometry is complex. As heated the work material yields at 10,000 lb/in2 , and has no tendency to strain harden. At room temperature, the material yields at 25,000 lb/in2 Determine the maximum force required to perform the forging operation. Solution: Since the work material has no tendency to work harden, n = 0. From Table 19.1, choose Kf = 8.0. F = 8.0(10,000)(16) = 1,280,000 lb. 19.22 A connecting rod is designed to be hot forged in an impression die. The projected area of the part is 6,500 mm2 . The design of the die will cause flash to form during forging, so that the area, including flash, will be 9,000 mm2 . The part geometry is considered to be complex. As heated the work material yields at 75 MPa, and has no tendency to strain harden. Determine the maximum force required to perform the operation. Solution: Since the work material has no tendency to work harden, n = 0. From Table 19.1, choose Kf =8.0. F = 8.0(75)(9,000) = 5,400,000 N. Extrusion 19.23 A cylindrical billet that is 100 mm long and 50 mm in diameter is reduced by indirect (backward) extrusion to a 20 mm diameter. The die angle is 90°. The Johnson equation has a = 0.8 and b = 1.4, and the flow curve for the work metal has a strength coefficient of 800 MPa and strain hardening exponent of 0.13. Determine (a) extrusion ratio, (b) true strain (homogeneous deformation), (c) extrusion strain, (d) ram pressure, and (e) ram force. Solution: (a) rx = Ao/Af = Do 2 /Df 2 = (50)2 /(20)2 = 6.25 (b) ε = ln rx = ln 6.25 = 1.833 (c) εx = a + b ln rx = 0.8 + 1.4(1.833) = 3.366 (d) fY = 800(1.833)0.13 /1.13 = 766.0 MPa p = 766.0(3.366) = 2578 MPa (e) Ao = πDo 2 /4 = π(50)2 /4 = 1963.5 mm2 F = 2578(1963.5) = 5,062,000 N 19.24 A 3.0-in-long cylindrical billet whose diameter = 1.5 in is reduced by indirect extrusion to a diameter = 0.375 in. Die angle = 90°. In the Johnson equation, a = 0.8 and b = 1.5. In the flow curve for the work metal, K = 75,000 lb/in2 and n = 0.25. Determine (a) extrusion ratio, (b) true strain (homogeneous deformation), (c) extrusion strain, (d) ram pressure, (e) ram force, and (f) power if the ram speed = 20 in/min.
• 116. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 113 Solution: (a) rx = Ao/Af = Do 2 /Df 2 = (1.5)2 /(0.375)2 = 42 = 16.0 (b) ε = ln rx = ln 16 = 2.773 (c) εx = a + b ln rx = 0.8 + 1.5(2.773) = 4.959 (d) fY = 75,000(2.773)0.25 /1.25 = 77,423 lb/in2 p = 77,423(4.959) = 383,934 lb/in2 (e) Ao = πDo 2 /4 = π(1.5)2 /4 = 1.767 in2 F = (383,934)(1.767) = 678,411 lb. (f) P = 678,411(20) = 13,568,228 in-lb/min HP = 13,568,228/396,000 = 34.26 hp 19.25 A billet that is 75 mm long with diameter = 35 mm is direct extruded to a diameter of 20 mm. The extrusion die has a die angle = 75°. For the work metal, K = 600 MPa and n = 0.25. In the Johnson extrusion strain equation, a = 0.8 and b = 1.4. Determine (a) extrusion ratio, (b) true strain (homogeneous deformation), (c) extrusion strain, and (d) ram pressure and force at L = 70, 60, 50, 40, 30, 20, and 10 mm. Use of a spreadsheet calculator is recommended for part (d). Solution: (a) rx = Ao/Af = Do 2 /Df 2 = (35)2 /(20)2 = 3.0625 (b) ε = ln rx = ln 3.0625 = 1.119 (c) εx = a + b ln rx = 0.8 + 1.4(1.119) = 2.367 (d) fY = 600(1.119)0.25 /1.25 = 493.7 MPa Ao = π(35)2 /4 = 962.1 mm2 It is appropriate to determine the volume of metal contained in the cone of the die at the start of the extrusion operation, to assess whether metal has been forced through the die opening by the time the billet has been reduced from L = 75 mm to L = 70 mm. For a cone-shaped die with angle = 75°, the height h of the frustum is formed by metal being compressed into the die opening: The two radii are: R1 = 0.5Do = 17.5 mm and R2 = 0.5Df = 10 mm, and h = (R1 - R2)/tan 75 = 7.5/tan 75 = 2.01 mm Frustum volume V = 0.333πh(R1 2 + R1R2 + R2 2 ) = 0.333π(2.01)(17.52 + 10 x 17.5 + 102 ) = 1223.4 mm3 . Compare this with the volume of the portion of the cylindrical billet between L = 75 mm and L = 70 mm. V = πDo 2 h/4 = 0.25π(35)2 (75 - 70) = 4810.6 mm3 Since this volume is greater than the volume of the frustum, this means that the metal has extruded through the die opening by the time the ram has moved forward by 5 mm. L = 70 mm: pressure p = 493.7(2.367 + 2 x 70/35) = 3143.4 MPa Force F = 3143.4(962.1) = 3,024, 321 N L = 60 mm: pressure p = 493.7(2.367 + 2 x 60/35) = 2861.3 MPa Force F = 2861.3(962.1) = 2,752,890 N L = 50 mm: pressure p = 493.7(2.367 + 2 x 50/35) = 2579.2 MPa Force F = 2579.2(962.1) = 2,481,458 N L = 40 mm: pressure p = 493.7(2.367 + 2 x 40/35) = 2297.1 MPa Force F = 2297.1(962.1) = 2,210,027 N L = 30 mm: pressure p = 493.7(2.367 + 2 x 30/35) = 2014.9 MPa Force F = 2014.9(962.1) = 1,938,595 N L = 20 mm: pressure p = 493.7(2.367 + 2 x 20/35) = 1732.8 MPa Force F = 1732.8(962.1) = 1,667,164 N L = 10 mm: pressure p = 493.7(2.367 + 2 x 10/35) = 1450.7 MPa Force F = 1450.7(962.1) = 1,395,732 N
• 117. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 114 19.26 A 2.0-in-long billet with diameter = 1.25 in is direct extruded to a diameter of 0.50 in. The extrusion die angle = 90°. For the work metal, K = 45,000 lb/in2 , and n = 0.20. In the Johnson extrusion strain equation, a = 0.8 and b = 1.5. Determine (a) extrusion ratio, (b) true strain (homogeneous deformation), (c) extrusion strain, and (d) ram pressure at L = 2.0, 1.5, 1.0, 0.5 and zero in. Use of a spreadsheet calculator is recommended for part (d). Solution: (a) rx = Ao/Af = Do 2 /Df 2 = (1.25)2 /(0.5)2 = 6.25 (b) ε = ln rx = ln 6.25 = 1.8326 (c) εx = a + b ln rx = 0.8 + 1.5(1.8326) = 3.549 (d) fY = 45,000(1.8326)0.20 /1.20 = 42,330 lb/in2 Ao = π(1.25)2 /4 = 1.227 in2 Unlike the previous problem, the die angle α = 90°, so metal is forced through the die opening as soon as the billet starts to move forward in the chamber. L = 2.0 in: pressure p = 42,330(3.549 + 2 x 2.0/1.25) = 285,677 lb/in2 Force F = 285,677(1.227) = 350,579 lb L = 1.5 in: pressure p = 42,330(3.549 + 2 x 1.5/1.25) = 251,813 lb/in2 Force F = 251,813(1.227) = 309,022 lb L = 1.0 in: pressure p = 42,330(3.549 + 2 x 1.0/1.25) = 217,950 lb/in2 Force F = 217,950(1.227) = 267,465 lb L = 0.5 in: pressure p = 42,330(3.549 + 2 x 0.5/1.25) = 184,086 lb/in2 Force F = 184,086(1.227) = 225,908 lb L = 0.0 in: pressure p = 42,330(3.549 + 2 x 0.0/1.25) = 150,229 lb/in2 Force F = 150,229(1.227) = 184,351 lb These last values for L = 0 are not possible because of the increase in pressure and force due to the butt remaining in the extruder container at the end of the operation. 19.27 A direct extrusion operation is performed on a cylindrical billet with an initial diameter of 2.0 in and an initial length of 4.0 in. The die angle = 60° and orifice diameter is 0.50 in. In the Johnson extrusion strain equation, a = 0.8 and b = 1.5. The operation is carried out hot and the hot metal yields at 13,000 lb/in2 and does not strain harden when hot. (a) What is the extrusion ratio? (b) Determine the ram position at the point when the metal has been compressed into the cone of the die and starts to extrude through the die opening. (c) What is the ram pressure corresponding to this position? (d) Also determine the length of the final part if the ram stops its forward movement at the start of the die cone. Solution: (a) rx = Ao/Af = Do 2 /Df 2 = (2.0)2 /(0.5)2 = 16.0 (b) The portion of the billet that is compressed into the die cone forms a frustum with R1 = 0.5Do = 1.0 in and R2 = 0.5Df = 0.25 in. The height of the frustum h = (R1 - R2)/tan 65 = (1.0 - 0.25)/tan 60 = 0.433 in. The volume of the frustum is V = 0.333πh(R1 2 + R1R2 + R2 2 ) = 0.333π(0.433)(1.02 + 1.0 x 0.25 + 0.252 ) = 0.595 in3 The billet has advanced a certain distance by the time this frustum is completely filled and extrusion through the die opening is therefore initiated. The volume of billet compressed forward to fill the frustum is given by: V = πR1 2 (Lo - L1) = π(1.0)2 (Lo - L1) Setting this equal to the volume of the frustum, we have π(Lo - L1) = 0.595 in3 (Lo - L1) = 0.595/π = 0.189 in L1 = 4.0 - 0.189 = 3.811 in (c) ε = ln rx = ln 16 = 2.7726
• 118. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 115 εx = a + b ln rx = 0.8 + 1.5(2.7726) = 4.959 fY = 13,000(2.7726)0 /1.0 = 13,000 lb/in2 p = 13,000(4.959 + 2 x 3.811/2.0) = 114,000 lb/in2 (d) Length of extruded portion of billet = 3.811 in. With a reduction rx = 16, the final part length, excluding the cone shaped butt remaining in the die is L = 3.811(16) = 60.97 in. 19.28 An indirect extrusion process starts with an aluminum billet with diameter = 2.0 in and length = 3.0 in. Final cross section after extrusion is a square with 1.0 in on a side. The die angle = 90°. The operation is performed cold and the strength coefficient of the metal K = 26,000 lb/in2 and strain- hardening exponent n = 0.20. In the Johnson extrusion strain equation, a = 0.8 and b = 1.2. (a) Compute the extrusion ratio, true strain, and extrusion strain. (b) What is the shape factor of the product? (c) If the butt left in the container at the end of the stroke is 0.5 in thick, what is the length of the extruded section? (d) Determine the ram pressure in the process. Solution: (a) rx = Ao/Af Ao = πDo 2 /4 = π(2)2 /4 = 3.142 in2 Af = 1.0 x 1.0 = 1.0 in2 rx = 3.142/1.0 = 3.142 ε = ln 3.142 = 1.145 εx = 0.8 + 1.3(1.145) = 2.174 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, A = 1.0 in2 . The radius of the circle is R = (1.0/π)0.5 = 0.5642 in, Cc = 2π(0.5642) = 3.545 in The perimeter of the extruded cross section Cx = 4(1.0) = 4.0 in Kx = 0.98 + 0.02(4.0/3.545)2.25 = 1.006 (c) Given that the butt thickness = 0.5 in Original volume V = (3.0)(π x 22 /4) = 9.426 in3 The final volume consists of two sections: (1) butt, and (2) extrudate. The butt volume V1 = (0.5)(π22 /4) = 1.571 in3 . The extrudate has a cross-sectional area Af = 1.0 in2 . Its volume V2 = LAf = 9.426 - 1.571 = 7.855 in3 . Thus, length L = 7.855/1.0 = 7.855 in (d) fY = 26,000(1.145)0.2 /1.2 = 22,261 lb/in3 p = 1.006(22,261)(2.174) = 48,698 lb/in2 19.29 An L-shaped structural section is direct extruded from an aluminum billet in which Lo = 500 mm and Do = 100 mm. Dimensions of the cross section are given in Figure P19.29. Die angle = 90°. Determine (a) extrusion ratio, (b) shape factor, and (c) length of the extruded section if the butt remaining in the container at the end of the ram stroke is 25 mm. Solution: (a) rx = Ao/Af Ao = π(100)2 /4 = 7854 mm2 Af = 2(12 x 50) = 1200 mm2 rx = 7854/1200= 6.545 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, A = 1200 mm2 . The radius of the circle is R = (1200/π)0.5 = 19.54 mm, Cc = 2π(19.54) = 122.8 mm. The perimeter of the extruded cross section Cx = 62 + 50 + 12 + 38 + 50 + 12 = 224 mm Kx = 0.98 + 0.02(224/122.8)2.25 = 1.057 (c) Total original volume V = 0.25π(100)2 (500) = 3,926,991 mm3
• 119. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 116 The final volume consists of two sections: (1) butt, and (2) extrudate. The butt volume V1 = 0.25π(100)2 (25) = 196,350 mm3 . The extrudate has a cross-sectional area Af = 1200 mm2 . Its volume V2 = LAf = 3,926,991 - 196,350 = 3,730,641 mm3 . Thus, length L = 3,730,641/1200 = 3108.9 mm = 3.109 m 19.30 The flow curve parameters for the aluminum alloy of Problem 19.29 are: K = 240 MPa and n = 0.16. If the die angle in this operation = 90°, and the corresponding Johnson strain equation has constants a = 0.8 and b = 1.5, compute the maximum force required to drive the ram forward at the start of extrusion. Solution: From Problem 19.29, rx = 5.068 ε = ln 5.068= 1.623 εx = 0.8 + 1.5(1.623) = 3.234 fY = 240(1.623)0.16 /1.16 = 223.6 MPa Maximum ram force occurs at beginning of stroke when length is maximum at L = 250 mm p = Kx fY (εx + 2L/Do) = 1.057(223.6)( 3.234 + 2(250)/88) = 2107.2 MPa F = pAo = 2107.2 (6082.1) = 12,816,267 N 19.31 A cup-shaped part is backward extruded from an aluminum slug that is 50 mm in diameter. The final dimensions of the cup are: OD = 50 mm, ID = 40 mm, height = 100 mm, and thickness of base = 5 mm. Determine (a) extrusion ratio, (b) shape factor, and (c) height of starting slug required to achieve the final dimensions. (d) If the metal has flow curve parameters K = 400 MPa and n = 0.25, and the constants in the Johnson extrusion strain equation are: a = 0.8 and b = 1.5, determine the extrusion force. Solution: (a) rx = Ao/Af Ao = 0.25π(50)2 = 1963.75 mm2 Af = 0.25π(502 - 402 ) = 706.86 mm2 rx = 1963.75/706.86 = 2.778 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, A = 706.86 mm2 . The radius of the circle is R = (706.86/π)0.5 = 15 mm, Cc = 2π(15) = 94.25 mm. The perimeter of the extruded cross section Cx = π(50 + 40) = 90π = 282.74 mm. Kx = 0.98 + 0.02(282.74/94.25)2.25 = 1.217 (c) Volume of final cup consists of two geometric elements: (1) base and (2) ring. (1) Base t = 5 mm and D = 50 mm. V1 = 0.25π(50)2 (5) = 9817.5 mm3 (2) Ring OD = 50 mm, ID = 40 mm, and h = 95 mm. V2 = 0.25π(502 - 402 )(95) = 0.25π(2500 - 1600)(95) = 67,151.5 mm3 Total V = V1 + V2 = 9817.5 + 67,151.5 = 76,969 mm3 Volume of starting slug must be equal to this value V = 76,969 mm3 V = 0.25π(50)2 (h) = 1963.5h = 76,969 mm3 h = 39.2 mm (d) ε = ln 2.778 = 1.0218 εx = 0.8 + 1.5(1.0218) = 2.33 fY = 400(1.0218)0.25 /1.25 = 321.73 MPa p = Kx fY εx = 1.217(321.73)(2.33) = 912.3 MPa Ao = 0.25π(40)2 = 1256.6 mm2 F = 912.3(1256.6) = 1,146,430 N 19.32 Determine the shape factor for each of the extrusion die orifice shapes in Figure P19.32.
• 120. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 117 Solution: (a) Ax = 20 x 60 = 1200 mm, Cx = 2(20 + 60) = 160 mm Ao = πR2 = 1200 R2 = 1200/π = 381.97, R = 19.544 mm, Cc = 2πR = 2π(19.544) = 122.8 mm Kx = 0.98 + 0.02(160/122.8)2.25 = 1.016 (b) Ax = πRo 2 - πRi 2 = π(252 - 22.52 ) = 373.06 mm2 Cx = πDo + πDi = π(50 + 45) = 298.45 mm R2 = 373.06/π = 118.75, R = 10.897 mm, Cc = 2πR = 2π(10.897) = 68.47 mm Kx = 0.98 + 0.02(298.45/68.47)2.25 = 1.53 (c) Ax = 2(5)(30) + 5(60 - 10) = 300 + 250 = 550 mm2 Cx = 30 + 60 + 30 + 5 + 25 + 50 + 25 + 5 = 230 mm Ao = πR2 = 550, R2 = 550/π = 175.07, R = 13.23 mm Cc = 2πR = 2π(13.23) = 83.14 mm Kx = 0.98 + 0.02(230/83.14)2.25 = 1.177 (d) Ax = 5(55)(5) + 5(85 - 5x5) = 1675 mm2 Cx = 2 x 55 + 16 x 25 + 8 x 15 + 10 x 5 = 680 mm Ao = πR2 = 1675, R2 = 1675/π = 533.17, R = 23.09 mm Cc = 2πR = 2π(23.09) = 145.08 mm Kx = 0.98 + 0.02(680/145.08)2.25 = 1.626 19.33 A direct extrusion operation produces the cross section shown in Figure P19.32(a) from a brass billet whose diameter = 125 mm and length = 350 mm. The flow curve parameters of the brass are K = 700 MPa and n = 0.35. In the Johnson strain equation, a = 0.7 and b = 1.4. Determine (a) the extrusion ratio, (b) the shape factor, (c) the force required to drive the ram forward during extrusion at the point in the process when the billet length remaining in the container = 300 mm, and (d) the length of the extruded section at the end of the operation if the volume of the butt left in the container is 600,000 mm3 . Solution: (a) rx = Ao/Af Ao = π(125)2 /4 = 12,272 mm2 Af = Ax = 20(60) = 1200 mm2 rx = 12272/1200 = 10.23 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, Af = 1200 mm2 . The radius of the circle is R = (1200/π)0.5 = 19.544 mm, Cc = 2π(19.544) = 122.8 mm. The perimeter of the extruded cross section Cx = 2(20 + 60) = 160 mm Kx = 0.98 + 0.02(160/122.8)2.25 = 1.016 (c) ε = ln 10.23 = 2.325 εx = 0.7 + 1.4(2.325) = 3.955 fY = 700(2.325)0.35 /1.35 = 696.6 MPa p = Kx fY εx = 1.016(696.6)(3.955 + 2(300)/125) = 6196.3 MPa F = pAo = 6196.3(12,272) = 76,295,200 N (d) Total original volume V = π(125)2 (350)/4 = 4,295,200 mm3 The final volume consists of two sections: (1) butt, and (2) extrudate. The butt volume as given V1 = 600,000 mm3 . The extrudate has a cross-sectional area Af = 1200 mm2 . Its volume V2 = LAf = 4,295,200 – 600,000 = 3,695,200 mm3 . Thus, length L = 3,695,200/1200 = 3079.3 mm = 3.079 m
• 121. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 118 19.34 In a direct extrusion operation the cross section shown in Figure P19.32(b) is produced from a copper billet whose diameter = 100 mm and length = 500 mm. In the flow curve for copper, the strength coefficient = 300 MPa and strain hardening exponent = 0.50. In the Johnson strain equation, a = 0.8 and b = 1.5. Determine (a) the extrusion ratio, (b) the shape factor, (c) the force required to drive the ram forward during extrusion at the point in the process when the billet length remaining in the container = 450 mm, and (d) the length of the extruded section at the end of the operation if the volume of the butt left in the container is 350,000 mm3 . Solution: (a) rx = Ao/Af Ao = π(100)2 /4 = 7854 mm2 Af = Ax = π(50)2 /4 - π(45)2 /4 = 1963.5 – 1590.4 = 373.1 mm2 rx = 7854/373.1 = 21.05 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, Ax = 373.1 mm2 . The radius of the circle is R = (373.1/π)0.5 = 10.9 mm, Cc = 2π(10.9) = 68.5 mm. The perimeter of the extruded cross section Cx = π(50) + π(45) = 298.5 mm Kx = 0.98 + 0.02(298.5/68.5)2.25 = 1.53 (c) ε = ln 21.05= 3.047 εx = 0.8 + 1.5(3.047) = 5.37 fY = 300(3.047)0.50 /1.50 = 349.1 MPa p = Kx fY εx = 1.53(349.1)(5.37 + 2(450)/100) = 7675.3 MPa F = pAo = 7675.3(7854) = 60,282,179 N (d) Total original volume V = π(100)2 (500)/4 = 3,926,991 mm3 The final volume consists of two sections: (1) butt, and (2) extrudate. The butt volume as given V1 = 350,000 mm3 . The extrudate has a cross-sectional area Af = 373.1 mm2 . Its volume V2 = LAf = 3,926,991 – 350,000 = 3,576,991 mm3 . Thus, length L = 3,576,991/373.1 = 9,587.2 mm = 9.587 m 19.35 A direct extrusion operation produces the cross section shown in Figure P19.32(c) from an aluminum billet whose diameter = 150 mm and length = 500 mm. The flow curve parameters for the aluminum are K = 240 MPa and n = 0.16. In the Johnson strain equation, a = 0.8 and b = 1.2. Determine (a) the extrusion ratio, (b) the shape factor, (c) the force required to drive the ram forward during extrusion at the point in the process when the billet length remaining in the container = 400 mm, and (d) the length of the extruded section at the end of the operation if the volume of the butt left in the container is 600,000 mm3 . Solution: (a) rx = Ao/Af Ao = π(150)2 /4 = 17,671.5 mm2 Af = Ax = 60(5) + 2(25)(5) = 300 + 250 = 550 mm2 rx = 17,671.5/550 = 32.1 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, Ax = 550 mm2 . Cx = 30 + 60 + 30 + 5 + 25 + 50 + 25 + 5 = 230 mm Ao = πR2 = 550, R2 = 550/π = 175.07, R = 13.23 mm Cc = 2πR = 2π(13.23) = 83.14 mm Kx = 0.98 + 0.02(230/83.14)2.25 = 1.177 (c) ε = ln 32.1= 3.47 εx = 0.8 + 1.2(3.47) = 4.96
• 122. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 119 fY = 240(3.47)0.16 /1.16 = 252.5 MPa p = Kx fY εx = 1.177(252.5)(4.96 + 2(400)/150) = 3059.1 MPa F = pAo = 3059.1(17,671.5) = 54,058,912 N (d) Total original volume V = π(150)2 (500)/4 = 8,835,750 mm3 The final volume consists of two sections: (1) butt, and (2) extrudate. The butt volume as given V1 = 600,000 mm3 . The extrudate has a cross-sectional area Af = 550 mm2 . Its volume V2 = LAf = 8,835,750 – 600,000 = 8,235,750 mm3 . Thus, length L = 8,835,750/550 = 14,974 mm = 14.974 m 19.36 A direct extrusion operation produces the cross section shown in Figure P19.32(d) from an aluminum billet whose diameter = 150 mm and length = 900 mm. The flow curve parameters for the aluminum are K = 240 MPa and n = 0.16. In the Johnson strain equation, a = 0.8 and b = 1.5. Determine (a) the extrusion ratio, (b) the shape factor, (c) the force required to drive the ram forward during extrusion at the point in the process when the billet length remaining in the container = 850 mm, and (d) the length of the extruded section at the end of the operation if the volume of the butt left in the container is 600,000 mm3 . Solution: (a) rx = Ao/Af Ao = π(150)2 /4 = 17,671.5 mm2 Af = Ax = 5(55)(5) + 5(85 – 5(5)) = 1675 mm2 rx = 17,671.5/1675 = 10.55 (b) To determine the die shape factor we need to determine the perimeter of a circle whose area is equal to that of the extruded cross section, Ax = 1675 mm2 . Cx = 2 x 55 + 16 x 25 + 8 x 15 + 10 x 5 = 680 mm Ao = πR2 = 1675, R2 = 1675/π = 533.17, R = 23.09 mm Cc = 2πR = 2π(23.09) = 145.08 mm Kx = 0.98 + 0.02(680/145.08)2.25 = 1.626 (c) ε = ln 10.55= 2.36 εx = 0.8 + 1.5(2.36) = 4.33 fY = 240(2.36)0.16 /1.16 = 237.4 MPa p = Kx fY εx = 1.626(237.4)(4.33 + 2(850)/150) = 6046.2 MPa F = pAo = 6046.2(17,671.5) = 106,846,146 N (d) Total original volume V = π(150)2 (900)/4 = 15,904,313 mm3 The final volume consists of two sections: (1) butt, and (2) extrudate. The butt volume as given V1 = 600,000 mm3 . The extrudate has a cross-sectional area Af = 1675 mm2 . Its volume V2 = LAf = 15,904,313 – 600,000 = 15,304,313 mm3 . Thus, length L = 15,304,313/1675 = 9,137 mm = 9.137 m Drawing 19.37 A spool of wire has a starting diameter of 2.5 mm. It is drawn through a die with an opening that is to 2.1 mm. The entrance angel of the die is 18° degrees. Coefficient of friction at the work-die interface is 0.08. The work metal has a strength coefficient of 450 MPa and a strain hardening coefficient of 0.26. The drawing is performed at room temperature. Determine (a) area reduction, (b) draw stress, and (c) draw force required for the operation. Solution: (a) r = (Ao - Af)/Ao Ao = 0.25π(2.50)2 = 4.91 mm2
• 123. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 120 Af = 0.25π(2.1)2 = 3.46 mm2 r = (4.91 – 3.46)/4.91 = 0.294 (b) Draw stress σd: ε = ln(4.91/3.46) = ln 1.417 = 0.349 fY = 450(0.349)0.26 /1.26 = 271.6 MPa φ = 0.88 + 0.12(D/Lc) D = 0.5(2.5 + 2.1) = 2.30 Lc = 0.5(2.5 - 2.1)/sin 18 = 0.647 φ = 0.88 + 0.12(2.30/0.647) = 1.31 σd = fY (1 + µ/tan α)φ(ln Ao/Af) = 271.6(1 + 0.08/tan 18)(1.31)(0.349) = 154.2 MPa (c) Draw force F: F = Af σd = 3.46(154.2) = 534.0 N 19.38 Rod stock that has an initial diameter of 0.50 in is drawn through a draw die with an entrance angle of 13°. The final diameter of the rod is = 0.375 in. The metal has a strength coefficient of 40,000 lb/in2 and a strain hardening exponent of 0.20. Coefficient of friction at the work-die interface = 0.1. Determine (a) area reduction, (b) draw force for the operation, and (c) horsepower to perform the operation if the exit velocity of the stock = 2 ft/sec. Solution: (a) r = (Ao - Af)/Ao Ao = 0.25π(0.50)2 = 0.1964 in2 Af = 0.25π(0.35)2 = 0.1104 in2 r = (0.1964 - 0.1104)/0.1964 = 0.4375 (b) Draw force F: ε = ln(0.1964/0.1104) = ln 1.778 = 0.5754 fY = 40,000(0.5754)0.20 /1.20 = 29,845 lb/in2 φ = 0.88 + 0.12(D/Lc) D = 0.5(.50 + 0.375) = 0.438 Lc = 0.5(0.50 - 0.375)/sin 13 = 0.2778 φ = 0.88 + 0.12(0.438/0.2778) = 1.069 F = Af fY (1 + µ/tan α)φ(ln Ao/Af) F = 0.1104(29,845)(1 + 0.1/tan 13)(1.069)(0.5754) = 2907 lb (c) P = 2907(2 ft/sec x 60) = 348,800 ft/lb/min HP = 348800/33,000 = 10.57 hp 19.39 Bar stock of initial diameter = 90 mm is drawn with a draft = 15 mm. The draw die has an entrance angle = 18°, and the coefficient of friction at the work-die interface = 0.08. The metal behaves as a perfectly plastic material with yield stress = 105 MPa. Determine (a) area reduction, (b) draw stress, (c) draw force required for the operation, and (d) power to perform the operation if exit velocity = 1.0 m/min. Solution: (a) r = (Ao - Af)/Ao Ao = 0.25π(90)2 = 6361.7 mm2 Df = Do - d = 90 - 15 = 75 mm, Af = 0.25π(75)2 = 4417.9 mm2 r = (6361.7 - 4417.9)/6361.7 = 0.3056 (b) Draw stress σd: ε = ln(6361.7 /4417.9) = ln 1.440 = 0.3646
• 124. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 121 fY = k = 105 MPa φ = 0.88 + 0.12(D/Lc) D = 0.5(90 + 75) = 82.5 mm Lc = 0.5(90 - 75)/sin 18 = 24.3 mm φ = 0.88 + 0.12(82.5/24.3) = 1.288 σd = fY (1 + µ/tan α)φ(ln Ao/Af) = 105(1 + 0.08/tan 18)(1.288)(0.3646) = 61.45 MPa (c) F = Af σd = 4417.9 (61.45) = 271,475 N (d) P = 271,475(1 m/min) = 271,475 N-m/min = 4524.6 N-m/s = 4524.6 W 19.40 Wire stock of initial diameter = 0.125 in is drawn through two dies each providing a 0.20 area reduction. The starting metal has a strength coefficient = 40,000 lb/in2 and a strain hardening exponent = 0.15. Each die has an entrance angle of 12°, and the coefficient of friction at the work-die interface is estimated to be 0.10. The motors driving the capstans at the die exits can each deliver 1.50 hp at 90% efficiency. Determine the maximum possible speed of the wire as it exits the second die. Solution: First draw: Do = 0.125 in, Ao = 0.25π(0.125)2 = 0.012273 in2 009819 in2 ε = ln(0.012273/0.009819) = ln 1.250 = 0.2231 r = (Ao - Af)/Ao, Af = Ao(1 - r) = 0.012773(1 - 0.2) = 0. fY = 40,000(0.2231)0.15 /1.15 = 27,775 lb/in2 φ = 0.88 + 0.12(D/Lc) Df = 0.125(1 - r)0.5 = 0.125(0.8).5 = 0.1118 in D = 0.5(.125 + 0.1118) = 0.1184 Lc = 0.5(0.125 - 0.1118)/sin 12 = 0.03173 φ = 0.88 + 0.12(0.1184/0.03173) = 1.33 F = Af fY (1 + µ/tan α)φ(ln Ao/Af) F = 0.09819(27,775)(1 + 0.1/tan 12)(1.33)(0.2231) = 119 lb 1.5 hp at 90% efficiency = 1.5 x 0.90(33,000 ft-lb/min)/60 = 742.5 ft-lb/sec P = Fv = 119v = 742.5 v = 742.5/119 = 6.24 ft/sec Second draw: Do = 0.1118 in, Ao = 0.25π(0.1118)2 = 0.009819 in2 r = (Ao - Af)/Ao, Af = Ao(1 - r) = 0.009819(1 - 0.2) = 0.007855 in2 ε = ln(0.009819/0.007855) = ln 1.250 = 0.2231 Total strain experienced by the work metal is the sum of the strains from the first and second draws: ε = ε1 + ε2 = 0.2231 + 0.2231 = 0.4462 fY = 40,000(0.4462)0.15 /1.15 = 30,818 lb/in2 φ = 0.88 + 0.12(D/Lc) Df = 0.1118(1 - r)0.5 = 0.1118(.8).5 = 0.100 in D = 0.5(0.1118 + 0.100) = 0.1059 Lc = 0.5(0.1118 - 0.100)/sin 12 = 0.0269 φ = 0.88 + 0.12(0.1059/0.0269) = 1.35 F = Af fY (1 + µ/tan α)φ(ln Ao/Af) F = 0.007855(30,818)(1 + 0.1/tan 12)(1.35)(0.4462) = 214 lb. 1.5 hp at 90% efficiency = 742.5 ft-lb/sec as before in the first draw. P = Fv = 214v = 742.5 v = 742.5/214 = 3.47 ft/sec
• 125. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 122 Note: The calculations indicate that the second draw die is the limiting step in the drawing sequence. The first operation would have to be operated at well below its maximum possible speed; or the second draw die could be powered by a higher horsepower motor; or the reductions to achieve the two stages could be reallocated to achieve a higher reduction in the first drawing operation.
• 130. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 123 Answer. (b) and (d). Problems Cutting Operations 20.1 A power shears is used to cut soft cold-rolled steel that is 4.75 mm thick. At what clearance should the shears be set to yield an optimum cut? Solution: From Table 20.1, Ac = 0.060. Thus, c = Act = 0.060(4.75) = 0.285 mm 20.2 A blanking operation is to be performed on 2.0 mm thick cold-rolled steel (half hard). The part is circular with diameter = 75.0 mm. Determine the appropriate punch and die sizes for this operation. Solution: From Table 20.1, Ac = 0.075. Thus, c = 0.075(2.0) = 0.15 mm. Punch diameter = Db - 2c = 75.0 - 2(0.15) = 74.70 mm. Die diameter = Db = 75.0 mm. 20.3 A compound die will be used to blank and punch a large washer out of 6061ST aluminum alloy sheet stock 3.50 mm thick. The outside diameter of the washer is 50.0 mm and the inside diameter is 15.0 mm. Determine (a) the punch and die sizes for the blanking operation, and (b) the punch and die sizes for the punching operation. Solution: From Table 20.1, Ac = 0.060. Thus, c = 0.060(3.50) = 0.210 mm (a) Blanking punch diameter = Db - 2c = 50 - 2(0.21) = 49.58 mm Blanking die diameter = Db = 50.00 mm (b) Punching punch diameter = Dh = 15.00 mm Punching die diameter = Dh + 2c = 30 + 2(0.210) = 15.42 mm 20.4 A blanking die is to be designed to blank the part outline shown in Figure P20.4. The material is 4 mm thick stainless steel (half hard). Determine the dimensions of the blanking punch and the die opening. Solution: From Table 20.1, Ac = 0.075. Thus, c = 0.075(4.0) = 0.30 mm Blanking die: dimensions are the same as for the part in Figure P20.4. Blanking punch: 85 mm length dimension = 85 - 2(0.3) = 84.4 mm 50 mm width dimension = 50 - 2(0.3) = 49.4 mm Top and bottom 25 mm extension widths = 25 - 2(0.3) = 24.4 mm The 25 mm inset dimension remains the same. 20.5 Determine the blanking force required in Problem 20.2, if the shear strength of the steel = 325 MPa and the tensile strength is 450 MPa. Solution: F = StL t = 2.0 mm from Problem 20.2. L = πD = 75π = 235.65 mm F = 325(2.0)(235.65) = 153,200 N 20.6 Determine the minimum tonnage press to perform the blanking and punching operation in Problem 20.3. The aluminum sheet metal has a tensile strength = 310 MPa, a strength coefficient of 350 MPa, and a strain-hardening exponent of 0.12. (a) Assume that blanking and punching occur simultaneously. (b) Assume the punches are staggered so that punching occurs first, then blanking. Solution: (a) F = 0.7(TS)tL t =3.5 mm from Problem 20.3. L = 50π + 15π = 65π = 204.2 mm F = 0.7(310)(3.5)(235.6) = 155,100 N = 155,1000/(4.4482*2000) tons = 17.4 tons => 18 ton press
• 131. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 124 (b) Longest length will determine the minimum tonnage press required. Punching length of cut, L= 15π, blanking length of cut, L=50π = 157.1 mm (use blanking) F = 0.7(310)(3.5)(157.1) = 119,300 N = 119,3000/(4.4482*2000) tons = 13.4 tons => 14 ton press 20.7 Determine the tonnage requirement for the blanking operation in Problem 20.4, given that the stainless steel has a yield strength = 500 MPa, a shear strength = 600 MPa, and a tensile strength = 700 MPa. Solution: F = StL t = 4 mm from Problem 20.4. L = 85 + 50 + 25 + 25 + 35 + 25 + 25 + 50 = 320 mm F = 600(4.0)(320) = 768,000 N. This is about 86.3 tons 20.8 The foreman in the pressworking section comes to you with the problem of a blanking operation that is producing parts with excessive burrs. (a) What are the possible reasons for the burrs, and (b) what can be done to correct the condition? Solution: (a) Reasons for excessive burrs: (1) clearance between punch and die is too large for the material and stock thickness; and (2) punch and die cutting edges are worn (rounded) which has the same effect as excessive clearance. (b) To correct the problem: (1) Check the punch and die cutting edges to see if they are worn. If they are, regrind the faces to sharpen the cutting edges. (2) If the die is not worn, measure the punch and die clearance to see if it equals the recommended value. If not, die maker must rebuild the punch and die. Bending 20.9 A bending operation is to be performed on 5.00 mm thick cold-rolled steel. The part drawing is given in Figure P20.9. Determine the blank size required. Solution: From drawing, α’ = 40°, R = 8.50 mm α = 180 - α’ = 140°. Ab = 2π(α/360)(R + Kbat) R/t = (8.5)/(5.00) = 1.7, which is less than 2.0; therefore, Kba = 0.333 Ab = 2π(140/360)(8.5 + 0.333 x 5.0) = 24.84 mm Dimensions of starting blank: w = 35 mm, L = 58 + 24.84 + 46.5 = 129.34 mm 20.10 Solve Problem 20.9 except that the bend radius R = 11.35 mm. Solution: From drawing, α’ = 40°, R = 11.35 mm α = 180 - α’ = 140°. Ab = 2π(α/360)(R + Kbat) R/t = (11.35)/(5.00) = 2.270; therefore, Kba = 0.5 Ab = 2π(140/360)(11.35 + 0.5 x 5.00) = 34.21 mm Dimensions of starting blank: w = 35 mm, L = 58 + 34.21 + 46.5 = 138.71 mm 20.11 An L-shaped part is to be bent in a V-bending operation on a press brake from a flat blank 4.0 in by 1.5 in that is 5/32 in thick. The bend of 90° is to be made in the middle of the 4-in length. (a) Determine the dimensions of the two equal sides that will result after the bend, if the bend radius = 3/16 in. For convenience, these sides should be measured to the beginning of the bend radius. (b) Also, determine the length of the part's neutral axis after the bend. (c) Where should the machine operator set the stop on the press brake relative to the starting length of the part? Solution: (a) R/t = (3/16)/(5/32) = 1.2. Therefore, Kba = 0.33 Ab = 2π(90/360)(0.1875 + 0.33 x 0.15625) = 0.3756 in Dimensions (lengths) of each end = 0.5(4.0 - 0.3756) = 1.8122 in
• 132. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 125 (b) Since the metal stretches during bending, its length will be greater after the bend than before. Its length before bending = 4.000 in. The stretched length of the bend along the neutral axis will be: Bent length = 2π(90/360)(0.1875 + 0.5 x 0.15625) = 0.4173 in Therefore, the length of the neutral axis of the part will be 2(1.8122) + 0.4173 = 4.0417 in However, if stretching occurs along the neutral axis of the bend, then thinning of the stretched metal will also occur, and this will affect the preceding calculated value of the length of the bent section. The amount of thinning will be inversely proportional to the amount of stretching because volume must remain constant, before and after bending. The sheet thickness after bending (assuming uniform stretching and thinning) = (0.3756/0.4173)(0.15625) = 0.1406 in. Now let us recalculate the length of the bent section with this new value of t. The bend radius will remain the same (R = 3/16 = 0.1875 in) because it is located at the inside of the bend. Length of neutral axis along the bend = 2π(90/360)(0.1875 + 0.5 x 0.1406) = 0.4049 in. The new final length of the neutral axis is L = 2(1.8122) + 0.4049 = 4.0293 in. The amount of stretching is less than previously determined, and so is the amount of thinning. An iterative procedure must be used to arrive at the final values of stretching and thinning. Recalculate the thickness of the stretched sheet as (0.3756/0.4049)(0.15625) = 0.1449 in, and recalculating the length of the bent section based on this value, we have the following: Length of neutral axis along the bend = 2π(90/360)(0.1875 + 0.5 x 0.1449) = 0.4084 in The new final length of the neutral axis is L = 2(1.8122) + 0.4084 = 4.0328 in. One more iteration: The thickness of the stretched sheet is (0.3756/0.4084)(0.15625) = 0.1437 in, and recalculating the length of the bent section based on this value, we have 2π(90/360)(0.1875 + 0.5 x 0.1437) = 0.4074 in. The new final length of the neutral axis is L = 2(1.8122) + 0.4074 = 4.0318 in. Close enough and only about 0.01 in different from our previous value of 4.0417 in. (c) The operator should set the stop so that the tip of the V-punch contacts the starting blank at a distance = 2.000 in from the end. 20.12 A bending operation is to be performed on 4.0 mm thick cold-rolled steel sheet that is 25 mm wide and 100 mm long. The sheet is bent along the 25 mm direction, so that the bend is 25 mm long. The resulting sheet metal part has an acute angle of 30° and a bend radius of 6 mm. Determine (a) the bend allowance and (b) the length of the neutral axis of the part after the bend. (Hint: the length of the neutral axis before the bend = 100.0 mm). Solution: (a) Given that α’ = 30°, R = 6.0 mm, and t = 4.0 mm α = 180 - α’ = 150°. Ab = 2π(α/360)(R + Kbat) R/t = 6/4 = 1.5, which is less than 2.0; therefore, Kba = 0.333 Ab = 2π(150/360)(6.0 + 0.333 x 4.0) = 19.195 mm (b) Due to stretching, the neutral axis of the final part will be greater than 100.0 mm. The amount of stretching will be the difference between the bend allowance and the length of the bent section, which is computed as 2π(150/360)(6.0 + 0.5 x 4.0) = 20.944. The difference = 20.944 – 19.195 = 1.75 mm Thus, the final length of the neutral axis will be L = 100 + 1.75 = 101.75 mm However, if stretching occurs along the neutral axis of the bend, then thinning of the stretched metal will also occur, and this will affect the preceding calculated value of the length of the bent section. The amount of thinning will be inversely proportional to the amount of stretching because volume must remain constant, before and after bending. The sheet thickness after bending (assuming uniform stretching and thinning) = (19.195/20.944)(4.0) = 3.67 mm. Now let us recalculate the length of the bent section with this new value of t.
• 133. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 126 The bend radius will remain the same (R = 6.0 mm) because it is located at the inside of the bend. Length of neutral axis along the bend = 2π(150/360)(6.0 + 0.5 x 3.67) = 20.512 mm. Now the difference between the length of the bent section and the bend allowance = 20.512 – 19.195 = 1.317 mm. The new final length of the neutral axis is L = 100 + 1.32 = 101.32 mm The amount of stretching is less than previously determined, and so is the amount of thinning. An iterative procedure must be used to arrive at the final values of stretching and thinning. Recalculate the thickness of the stretched sheet as (19.195/20.512)(4.0) = 3.74 mm, and recalculating the length of the bent section based on this value, we have the following: Length of neutral axis along the bend = 2π(150/360)(6.0 + 0.5 x 3.74) = 20.608 mm The new difference between the length of the bent section and the bend allowance = 20.608 – 19.195 = 1.413 mm, and the new final length of the neutral axis is L = 100 + 1.41 = 101.41 mm One more iteration: The thickness of the stretched sheet is (19.195/20.608)(4.0) = 3.73 mm, and recalculating the length of the bent section based on this value, we have 2π(150/360)(6.0 + 0.5 x 3.73) = 20.585 mm. The new before and after difference = 20.585 – 19.195 = 1.39 mm, and the new final length of the neutral axis is L = 100 + 1.39 = 101.39 mm 20.13 Determine the bending force required in Problem 20.9 if the bend is to be performed in a V-die with a die opening dimension of 40 mm. The material has a tensile strength of 600 MPa and a shear strength of 430 MPa. Solution: For V-bending, Kbf = 1.33. F = Kbf(TS)wt2 /D = 1.33(600)(35)(5.0)2 /40 = 17,460 N 20.14 Solve Problem 20.13 except that the operation is performed using a wiping die with die opening dimension = 28 mm. Solution: For edge-bending in a wiping die, Kbf = 0.33. F = Kbf(TS)wt2 /D = 0.33(600)(35)(5.0)2 /28 = 6,188 N 20.15 Determine the bending force required in Problem 20.11 if the bend is to be performed in a V-die with a die opening width dimension = 1.25 in. The material has a tensile strength = 70,000 lb/in2 . Solution: For V-bending, Kbf = 1.33. F = Kbf(TS)wt2 /D = 1.33(70,000)(1.5)(5/32)2 /1.25 = 2728 lb. 20.16 Solve Problem 20.15 except that the operation is performed using a wiping die with die opening dimension = 0.75 in. Solution: For edge-bending in a wiping die, Kbf = 0.33. F = Kbf(TS)wt2 /D = 0.33(70,000)(1.5)(5/32)2 /0.75 = 1128 lb. 20.17 A sheet-metal part 3.0 mm thick and 20.0 mm long is bent to an included angle = 60° and a bend radius = 7.5 mm in a V-die. The metal has a yield strength = 220 MPa and a tensile strength = 340 MPa. Compute the required force to bend the part, given that the die opening dimension = 15 mm. Solution: For V-bending, Kbf = 1.33. F = Kbf(TS)wt2 /D = 1.33(340)(20)(3)2 /15 = 5426 N Drawing Operations 20.18 Derive an expression for the reduction r in drawing as a function of drawing ratio DR. Solution: Reduction r = (Db - Dp)/Db Drawing ratio DR = Db/Dp r = Db/Db - Dp/Db = 1 - Dp/Db = 1 - 1/DR
• 134. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 127 20.19 A cup is to be drawn in a deep drawing operation. The height of the cup is 75 mm and its inside diameter = 100 mm. The sheet-metal thickness = 2 mm. If the blank diameter = 225 mm, determine (a) drawing ratio, (b) reduction, and (c) thickness-to-diameter ratio. (d) Does the operation seem feasible? Solution: (a) DR = Db/Dp = 225/100 = 2.25 (b) r = (Db - Dp)/Db = (225 - 100)/225 = 0.555 = 55.5% (c) t/Db = 2/225 = 0.0089 = 0.89% (d) Feasibility? No! DR is too large (greater than 2.0), r is too large (greater than 50%), and t/D is too small (less than 1%). 20.20 Solve Problem 20.19 except that the starting blank size diameter = 175 mm. Solution: (a) DR = Db/Dp = 175/100 = 1.75 (b) r = (Db - Dp)/Db = (175 - 100)/175 = 0.429 = 42.9% (c) t/Db = 2/175 = 0.0114 = 1.14% (d) Feasibility? DR < 2.0, r < 50%, and t/D > 1%. However, the operation is not feasible because the 175 mm diameter blank size does not provide sufficient metal to draw a 75 mm cup height. The actual cup height possible with a 175 mm diameter blank can be determined by comparing surface areas (one side only for convenience) between the cup and the starting blank. Blank area = πD2 /4 = π(175)2 /4 = 24,053 mm2 . To compute the cup surface area, let us divide the cup into two sections: (1) walls, and (2) base, assuming the corner radius on the punch has a negligible effect in our calculations and there is no earing of the cup. Thus, Cup area = πDph + πDp 2 /4 = 100πh + π(100)2 /4 = 100πh + 2500π = 314.16h + 7854. Set surface area of cup = surface are of starting blank: 314.16h + 7854= 24,053 314.16h = 16,199 h = 51.56 mm. This is less than the specified 75 mm height. 20.21 A deep drawing operation is performed in which the inside of the cylindrical cup has a diameter of 4.25 in and a height = 2.65 in. The stock thickness = 3/16 in, and the starting blank diameter = 7.7 in. Punch and die radii = 5/32 in. The metal has a tensile strength = 65,000 lb/in2 , a yield strength = 32,000 lb/in2 , and a shear strength of 40,000 lb/in2 . Determine (a) drawing ratio, (b) reduction, (c) drawing force, and (d) blankholder force. Solution: (a) DR = 7.7/4.25 = 1.81 (b) r = (Db – Dp)/Db = (7.7 – 4.25)/7.7 = 3.45/7.70 = 0.448 = 44.8% (c) F = πDpt(TS)(Db/Dp - 0.7) = π(4.25)(0.1875)(65,000)(7.7/4.25 - 0.7) = 180,900 lb. (d) Fh = 0.015Yπ(Db 2 - (Dp + 2.2t + 2Rd)2 ) Fh = 0.015(32,000)π(7.72 - (4.25 + 2.2 x 0.1875 + 2 x 0.15625)2 ) = 0.015(32,000)π(7.72 - 4.9752 ) Fh = 52,100 lb 20.22 Solve Problem 20.21 except that the stock thickness t = 1/8 in. Solution: (a) DR = 7.7/4.25 = 1.81 (same as previous problem) (b) t/Db = 0.125/7.7 = 0.01623 = 1.623% (c) F = πDpt(TS)(D/Dp - 0.7) = π(4.25)(0.125)(65,000)(7.7/4.25 - 0.7) = 120,600 lb. (d) Fh = 0.015Yπ(D2 - (Dp + 2.2t + 2Rd)2 ) Fh = 0.015(32,000)π(7.72 - (4.25 + 2.2 x 0.125 + 2 x 0.15625)2 ) = 0.015(32,000)π(7.72 - 4.83752 ) Fh = 54,100 lb
• 137. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 130 Solution: (1) Ears are caused by sheet metal that has directional properties. The material is anisotropic. One remedy is to anneal the metal to reduce the directionality of the properties. (2) Wrinkles are caused by compressive buckling of the flange as it is drawn inward to form the cup. There are several possible remedies: (a) increase the t/D ratio by using a thicker gage sheet metal. This may not be possible since a design change is required. (b) Increase the blankholder pressure against the work during drawing. (3) Tearing occurs due to high tensile stresses in the walls of the cup near the base. A remedy would be to provide a large punch radius. Tearing can also occur due to a die corner radius that is too small. 20.30 A cup-shaped part is to be drawn without a blankholder from sheet metal whose thickness = 0.25 in. The inside diameter of the cup = 2.5 in, its height = 1.5 in, and the corner radius at the base = 0.375 in. (a) What is the minimum starting blank diameter that can be used, according to Eq. (20.14)? (b) Does this blank diameter provide sufficient material to complete the cup? Solution: (a) According to Eq. (22.14), Db - Dp < 5t Db < 5t + Dp = 5(0.25) + 2.5 = 3.75 in (b) Because the sheet metal is rather thick, let us use volume rather than area to determine whether there is sufficient metal in a 3.75 in blank diameter. The drawn cup consists of three sections: (1) cup walls, (2) toroid at base, and (3) base. V1 = (1.5 - 0.375)π[(2.5 + 2 x 0.25)2 ] - (2.5)2 )/4 = 1.125π(2.75)/4 = 2.430 in3 V2 = (cross-section of quarter toroid) x (circle made by sweep of centroid) Cross-section of quarter toroid = 0.25π[(0.375 + 0.25)2 - (0.375)2 ] = 0.1964 in2 Circle made by centroid sweep has diameter = (2.5 - 2 x 0.25) + 2(0.375 + 0.25/2)sin 45 = 2.457 in V2 = 2.457π(0.1964) = 1.516 in3 V3 = (2.5 - 2 x 0.375)2 π(0.25)/4 = 0.601 in3 Total V = V1 + V2 + V3 = 2.430 + 1.516 + 0.601 = 4.547 in3 Volume of blank = πDb 2 t/4 = π(0.25)Db 2 /4 = 0.1963Db 2 Setting blank volume = cup volume: 0.1963Db 2 = 4.547 Db 2 = 4.547/0.1963 = 23.16 Db = 4.81 in. The diameter of 3.75 in computed in (a) does not provide sufficient metal to complete the drawing. Other Operations 20.31 A 20-in-long sheet-metal workpiece is stretched in a stretch forming operation to the dimensions shown in Figure P20.31. The thickness of the beginning stock is 3/16 in and the width is 8.5 in. The metal has a flow curve defined by a strength coefficient of 75,000 lb/in2 and a strain hardening exponent of 0.20. The yield strength of the material is 30,000 lb/in2 . (a) Find the stretching force F required near the beginning of the operation when yielding first occurs. Determine (b) true strain experienced by the metal, (c) stretching force F, and (d) die force Fdie at the very end when the part is formed as indicated in Figure P20.31(b). Solution: (a) Use ε = 0.002 as start of yielding. F = LtYf Yf = 75,000(0.002)0.20 = 21,600 lb/in2 F = (8.5)(0.1875)(21,600) = 34,500 lb. (b) After stretching, the length of the piece is increased from 20.0 in to 2(102 + 52 )0.5 = 22.361 in ε = ln(22.361/20) = ln 1.118 = 0.1116 (c) At the final length of 22.361 in, the thickness of the sheet metal has been reduced to maintain constant volume, assuming width L = 8.5 in remains the same during stretching.
• 138. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 131 tf = 0.1875(20/22.361) = 0.168 in Yf = 75,000(0.1116)0.20 = 48,400 lb/in2 F = 8.5(0.168)(48,400) = 69,000 lb. (d) Fdie = 2F sin A A = tan-1 (5/10) = 26.57° Fdie = 2(69,000) sin 26.57 = 61,700 lb. 20.32 Determine the starting disk diameter required to spin the part in Figure P20.32 using a conventional spinning operation. The starting thickness = 2.4 mm. Solution: From part drawing, radius = 25 + (100 - 25)/sin 30 = 25 + 75/0.5 = 175 mm Starting diameter D = 2(175) = 350 mm 20.33 If the part illustrated in Figure P20.32 were made by shear spinning, determine (a) the wall thickness along the cone-shaped portion, and (b) the spinning reduction r. Solution: (a) tf = t sin α = (2.4)sin 30 = 2.4(0.5) = 1.2 mm (b) r = (t - tf)/t = (2.4 – 1.2)/2.4 = 0.50 = 50% 20.34 Determine the shear strain that is experienced by the material that is shear spun in Problem 20.33. Solution: Based on sidewise displacement of metal through a shear angle of 30°, Shear strain γ = cot 30 = 1.732. 20.35 A 75 mm diameter tube is bent into a rather complex shape with a series of simple tube bending operations. The wall thickness on the tube = 4.75 mm. The tubes will be used to deliver fluids in a chemical plant. In one of the bends where the bend radius is 125 mm, the walls of the tube are flattening badly. What can be done to correct the condition? Solution: Possible solutions: (1) Use a mandrel to prevent collapsing of tube wall. (2) Request the designer to increase the bend radius to 3D = 225 mm. (3) Pack sand into the tube. The sand will act as an internal flexible mandrel to support the tube wall.
• 142. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 134 21.12 For which one of the following values of chip thickness before the cut to would you expect the specific energy in machining to be the greatest: (a) 0.010 inch, (b) 0.025 inch, (c) 0.12 mm, or (d) 0.50 mm? Answer. (c). 21.13 Which of the following cutting conditions has the strongest effect on cutting temperature: (a) feed or (b) speed? Answer. (b). Problems Chip Formation and Forces in Machining 21.1 In an orthogonal cutting operation, the tool has a rake angle = 15°. The chip thickness before the cut = 0.30 mm and the cut yields a deformed chip thickness = 0.65 mm. Calculate (a) the shear plane angle and (b) the shear strain for the operation. Solution: (a) r = to/tc = 0.30/0.65 = 0.4615 φ = tan-1 (0.4615 cos 15/(1 - 0.4615 sin 15)) = tan-1 (0.5062) = 26.85° (b) Shear strain γ = cot 26.85 + tan (26.85 - 15) = 1.975 + 0.210 = 2.185 21.2 In Problem 21.1, suppose the rake angle were changed to 0°. Assuming that the friction angle remains the same, determine (a) the shear plane angle, (b) the chip thickness, and (c) the shear strain for the operation. Solution: From Problem 21.1, α = 15° and φ = 26.85°. Using the Merchant Equation, Eq. (21.16): φ = 45 + α/2 - β/2; rearranging, β = 2(45) + α - 2φ β = 2(45) + α - 2(φ) = 90 + 15 – 2(26.85) = 51.3° Now, with α = 0 and β remaining the same at 51.3°, φ = 45 + 0/2 – 51.3/2 = 19.35° (b) Chip thickness at α = 0: tc = to/tan φ = 0.30/tan 19.35 = 0.854 mm (c) Shear strain γ = cot 19.35 + tan (19.35 - 0) = 2.848 + 0.351 = 3.199 21.3 In an orthogonal cutting operation, the 0.250 in wide tool has a rake angle of 5°. The lathe is set so the chip thickness before the cut is 0.010 in. After the cut, the deformed chip thickness is measured to be 0.027 in. Calculate (a) the shear plane angle and (b) the shear strain for the operation. Solution: (a) r = to/tc = 0.010/0.027 = 0.3701 φ = tan-1 (0.3701 cos 5/(1 - 0.3701 sin 5)) = tan-1 (0.3813) = 20.9° (b) Shear strain γ = cot 20.9 + tan (20.9 – 5) = 2.623 + 0.284 = 2.907 21.4 In a turning operation, spindle speed is set to provide a cutting speed of 1.8 m/s. The feed and depth of cut of cut are 0.30 mm and 2.6 mm, respectively. The tool rake angle is 8°. After the cut, the deformed chip thickness is measured to be 0.49 mm. Determine (a) shear plane angle, (b) shear strain, and (c) material removal rate. Use the orthogonal cutting model as an approximation of the turning process. Solution: (a) r = to/tc = 0.30/0.49 = 0.612 φ = tan-1 (0.612 cos 8/(1 – 0.612 sin 8)) = tan-1 (0.6628) = 33.6° (b) γ = cot 33.6 + tan (33.6 - 8) = 1.509 + 0.478 = 1.987 (c) RMR = (1.8 m/s x 103 mm/m)(0.3)(2.6) = 1404 mm3 /s
• 143. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 135 21.5 The cutting force and thrust force in an orthogonal cutting operation are 1470 N and 1589 N, respectively. The rake angle = 5°, the width of the cut = 5.0 mm, the chip thickness before the cut = 0.6, and the chip thickness ratio = 0.38. Determine (a) the shear strength of the work material and (b) the coefficient of friction in the operation. Solution: (a) φ = tan-1 (0.38 cos 5/(1 - 0.38 sin 5)) = tan-1 (0.3916) = 21.38° Fs = 1470 cos 21.38 – 1589 sin 21.38 = 789.3 N As = (0.6)(5.0)/sin 21.38 = 3.0/.3646 = 8.23 mm2 S = 789.3/8.23 = 95.9 N/mm2 = 95.9 MPa (b) φ = 45 + α/2 - β/2; rearranging, β = 2(45) + α - 2φ β = 2(45) + α - 2(φ) = 90 + 5 – 2(21.38) = 52.24° µ = tan 52.24 = 1.291 21.6 The cutting force and thrust force have been measured in an orthogonal cutting operation to be 300 lb and 291 lb, respectively. The rake angle = 10°, width of cut = 0.200 in, chip thickness before the cut = 0.015, and chip thickness ratio = 0.4. Determine (a) the shear strength of the work material and (b) the coefficient of friction in the operation. Solution: φ = tan-1 (0.4 cos 10/(1 - 0.4 sin 10)) = tan-1 (0.4233) = 22.94° Fs = 300 cos 22.94 - 291sin 22.94 = 162.9 lb. As = (0.015)(0.2)/sin 22.94 = 0.0077 in2 S = 162.9/0.0077 = 21,167 lb/in2 β = 2(45) + α - 2(φ) = 90 + 10 - 2(22.94) = 54.1° µ = tan 54.1 = 1.38 21.7 An orthogonal cutting operation is performed using a rake angle of 15°, chip thickness before the cut = 0.012 in and width of cut = 0.100 in. The chip thickness ratio is measured after the cut to be 0.55. Determine (a) the chip thickness after the cut, (b) shear angle, (c) friction angle, (d) coefficient of friction, and (e) shear strain. Solution: (a) r = to/tc, tc = to/r = 0.012/0.55 = 0.022 in (b) φ = tan-1 (0.55 cos 15/(1 - 0.55 sin 15)) = tan-1 (0.6194) = 31.8° (c) β = 2(45) + α - 2(φ) = 90 + 15 - 2(31.8) = 41.5° (d) µ = tan 41.5 = 0.88 (e) γ = cot 31.8 + tan(31.8 - 15) = 1.615 + 0.301 = 1.92 21.8 The orthogonal cutting operation described in previous Problem 21.7 involves a work material whose shear strength is 40,000 lb/in2 . Based on your answers to the previous problem, compute (a) the shear force, (b) cutting force, (c) thrust force, and (d) friction force. Solution: (a) As = (0.012)(0.10)/sin 31.8 = 0.00228 in2 . Fs = AsS = 0.00228(40,000) = 91.2 lb (b) Fc = 91.2 cos (41.5 - 15)/cos (31.8 + 41.5 -15) = 155 lb (c) Ft = 91.2 sin (41.5 - 15)/cos (31.8 + 41.5 -15) = 77.2 lb (d) F = 155 sin 15 - 77.2 cos 15 = 115 lb 21.9 In an orthogonal cutting operation, the rake angle = -5°, chip thickness before the cut = 0.2 mm and width of cut = 4.0 mm. The chip ratio = 0.4. Determine (a) the chip thickness after the cut, (b) shear angle, (c) friction angle, (d) coefficient of friction, and (e) shear strain. Solution: (a) r = to/tc, tc = to/r = 0.2/.4 = 0.5 mm
• 144. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 136 (b) φ = tan-1 (0.4 cos(–5)/(1 - 0.4 sin(–5))) = tan-1 (0.3851) = 21.1° (c) β = 2(45) + α - 2(φ) = 90 + (-5) - 2(21.8) = 42.9° (d) µ = tan 42.9 = 0.93 (e) γ = cot 31.8 + tan(31.8 - 15) = 2.597 + 0.489 = 3.09 21.10 The shear strength of a certain work material = 50,000 lb/in2 . An orthogonal cutting operation is performed using a tool with a rake angle = 20° at the following cutting conditions: cutting speed = 100 ft/min, chip thickness before the cut = 0.015 in, and width of cut = 0.150 in. The resulting chip thickness ratio = 0.50. Determine (a) the shear plane angle, (b) shear force, (c) cutting force and thrust force, and (d) friction force. Solution: (a) φ = tan-1 (0.5 cos 20/(1 - 0.5 sin 20)) = tan-1 (0.5668) = 29.5° (b) As = (0.015)(0.15)/sin 29.5 = 0.00456 in2 . Fs = AsS = 0.00456(50,000) = 228 lb (c) β = 2(45) + α - 2(φ) = 90 + 20 - 2(29.5) = 50.9° Fc = 228 cos (50.9 - 20)/cos (29.5 + 50.9 -20) = 397 lb Ft = 228 sin (50.9 - 20)/cos (29.5 + 50.9 -20) = 238 lb (d) F = 397 sin 20 + 238 cos 20 = 359 lb 21.11 Consider the data in Problem 21.10 except that rake angle is a variable, and its effect on the forces in parts (b), (c), and (d) is to be evaluated. (a) Using a spreadsheet calculator, compute the values of shear force, cutting force, thrust force, and friction force as a function of rake angle over a range of rake angles between the high value of 20° in Problem 21.10 and a low value of -10°. Use intervals of 5° between these limits. The chip thickness ratio decreases as rake angle is reduced and can be approximated by the following relationship: r = 0.38 + 0.006α, where r = chip thickness and α = rake angle. (b) What observations can be made from the computed results? Solution: (a) The author’s spreadsheet calculations (using Excel) returned the following results: α r Fs (lb) Fc (lb) Ft (lb) F (lb) 20 0.5 228 397 238 359 15 0.47 245 435 309 411 10 0.44 265 480 399 476 5 0.41 288 531 515 559 0 0.38 317 592 667 667 -5 0.35 351 665 870 809 -10 0.32 393 754 1150 1001 (b) Observations: (1) All forces increase as rake angle decreases. (2) The change in forces with rake angle increases at an accelerating rate as rake angle is reduced. (3) Thrust force is less than cutting force at high rake angles (e.g., 20°) but increases at a faster rate than cutting force so that its value is greater at low and negative rake angles. (4) Chip thickness ratio decreases with decreasing rake angle, as indicated by the given relationship r = 0.38 + 0.006α. 21.12 Solve previous Problem 21.10 except that the rake angle has been changed to -5° and the resulting chip thickness ratio = 0.35. Solution: (a) φ = tan-1 (0.35 cos(–5)/(1 - 0.35 sin(-5))) = tan-1 (0.3384) = 18.7° (b) As = (0.015)(0.15)/sin 18.7 = 0.00702 in2 . Fs = AsS = 0.00702(50,000) = 351 lb
• 145. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 137 (c) β = 2(45) + α - 2(φ) = 90 + (-5) - 2(18.7) = 47.6° Fc = 351 cos(47.6 - (-5))/cos(18.7 + 47.6 - (-5)) = 665 lb Ft = 351 sin(47.6 - (-5))/cos(18.7 + 47.6 - (-5)) = 870 lb (d) F = 665 sin (-5) + 870 cos (-5) = 809 lb 21.13 A carbon steel bar with 7.64 in diameter has a tensile strength of 65,000 lb/in2 and a shear strength of 45,000 lb/in2 . The diameter is reduced using a turning operation at a cutting speed of 400 ft/min. The feed is 0.011 in/rev and the depth of cut is 0.120 in. The rake angle on the tool in the direction of chip flow is 13°. The cutting conditions result in a chip ratio of 0.52. Using the orthogonal model as an approximation of turning, determine (a) the shear plane angle, (b) shear force, (c) cutting force and feed force, and (d) coefficient of friction between the tool and chip. Solution: (a) φ = tan-1 (0.52 cos 13/(1 - 0.52 sin 13)) = tan-1 (0.5738) = 29.8° (b) As = tow/sin φ = (0.011)(0.12)/sin 29.8 = 0.00265 in2 . Fs = AsS = 0.00587(40,000) = 119.4 lb (c) β = 2(45) + α - 2(φ) = 90 + 10 - 2(29.8) = 43.3° Fc = Fscos (β – α)/cos (φ + β – α) Fc = 264.1 cos (43.3 - 13)/cos (29.8 + 43.3 - 13) = 207 lb Ft = Fssin (β – α)/cos (φ + β – α) Ft = 264.1 sin (43.3 - 13)/cos (29.8 + 43.3 - 13) = 121 lb (d) μ = tan β = tan 43.3 = 0.942 21.14 Low carbon steel having a tensile strength of 300 MPa and a shear strength of 220 MPa is cut in a turning operation with a cutting speed of 3.0 m/s. The feed is 0.20 mm/rev and the depth of cut is 3.0 mm. The rake angle of the tool is 5° in the direction of chip flow. The resulting chip ratio is 0.45. Using the orthogonal model as an approximation of turning, determine (a) the shear plane angle, (b) shear force, (c) cutting force and feed force. Solution: (a) φ = tan-1 (0.45 cos 5/(1 - 0.45 sin 5)) = tan-1 (0.4666) = 25.0° (b) As = tow/sin φ = (0.2)(3.0)/sin 25.0 = 1.42 mm2 . Fs = AsS = 1.42(220) = 312 N (c) β = 2(45) + α - 2(φ) = 90 + 5 - 2(25.0) = 45.0° Fc = Fscos (β – α)/cos (φ + β – α) Fc = 312 cos(45 - 5)/cos(25.0 + 45.0 - 5) = 566 N Ft = Fssin(β – α)/cos(φ + β – α) Ft = 312 sin(45 - 5)/cos(25.0 + 45.0 - 5) = 474 N 21.15 A turning operation is made with a rake angle of 10°, a feed of 0.010 in/rev and a depth of cut = 0.100 in. The shear strength of the work material is known to be 50,000 lb/in2 , and the chip thickness ratio is measured after the cut to be 0.40. Determine the cutting force and the feed force. Use the orthogonal cutting model as an approximation of the turning process. Solution: φ = tan-1 (0.4 cos 10/(1 - 0.4 sin 10)) = tan-1 (0.4233) = 22.9° As = (0.010)(0.10)/sin 22.9 = 0.00257 in2 Fs = AsS = 0.00256(50,000) = 128 lb β = 2(45) + α - 2(φ) = 90 + 10 - 2(22.9) = 54.1° Fc = 128 cos (54.1 - 10)/cos (22.9 + 54.1 - 10) = 236 lb Ft = 128 sin (54.1 - 10)/cos (22.9 + 54.1 - 10) = 229 lb 21.16 Show how Eq. (21.3) is derived from the definition of chip ratio, Eq. (21.2), and Figure 21.5(b). Solution: Begin with the definition of the chip ratio, Eq. (21.2): r = to/tc = sin φ/cos (φ - α)
• 148. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 140 At efficiency E = 87%, available horsepower = 0.87(20) = 17.4 hp Since required horsepower exceeds available horsepower, the job cannot be accomplished on the 20 hp lathe, at least not at the specified cutting speed of 375 ft/min. 21.23 Suppose the cutting speed in Problems 21.7 and 21.8 is 200 ft/min. From your answers to those problems, find (a) the horsepower consumed in the operation, (b) metal removal rate in in3 /min, (c) unit horsepower (hp-min/in3 ), and (d) the specific energy (in-lb/in3 ). Solution: (a) From Problem 21.8, Fc = 155 lb. HPc = 155(200)/33,000 = 0.94 hp (b) RMR = vfd = (200 x 12)(0.012)(0.100) = 2.88 in3 /min (c) HPu = 0.94/2.88 = 0.326 hp/(in3 /min) (d) U = 155(200)/2.88 = 10,764 ft-lb/in3 = 129,167 in-lb/in3 21.24 For Problem 21.12, the lathe has a mechanical efficiency = 0.83. Determine (a) the horsepower consumed by the turning operation; (b) horsepower that must be generated by the lathe; (c) unit horsepower and specific energy for the work material in this operation. Solution: (a) From Problem 21.12, Fc = 207 lb. HPc = Fcv/33,000 = 207(400)/33,000 = 2.51 hp (b) HPg = HPc/E = 2.51/0.83 = 3.02 hp (c) RMR = 12 vfd = (400 x 12)(0.011)(0.120) = 6.336 in3 /min HPu = HPc/RMR = 2.51/6.336 = 0.396 hp/(in3 /min) U = Fcv/RMR = 207(400 x 12)/6.336 = 157,000 in-lb/in3 21.25 In a turning operation on low carbon steel (175 BHN), cutting speed = 400 ft/min, feed = 0.010 in/rev, and depth of cut = 0.075 in. The lathe has a mechanical efficiency = 0.85. Based on the unit horsepower values in Table 21.2, determine (a) the horsepower consumed by the turning operation and (b) the horsepower that must be generated by the lathe. Solution: (a) From Table 21.2, HPu = 0.6 hp/(in3 /min) for low carbon steel. HPc = HPu x RMR RMR = vfd = 400 x 12(.010)(0.075) = 3.6 in3 /min HPc = 0.6(3.6) = 2.16 hp (b) HPg = 2.16/0.85 = 2.54 hp 21.26 Solve Problem 21.25 except that the feed = 0.0075 in/rev and the work material is stainless steel (Brinell Hardness = 240 HB). Solution: (a) From Table 21.2, HPu = 1.0 hp/(in3 /min) for stainless steel. Since feed is lower than 0.010 in/rev in the table, a correction factor must be applied from Figure 21.14. For f = 0.0075 in/rev = to, correction factor = 1.1. HPc = HPu x RMR RMR = 400 x 12(0.0075)(0.12) = 4.32 in3 /min HPc = 1.1(1.0)(4.32) = 4.75 hp (b) HPg = 5.01/0.83 = 5.73 hp 21.27 A turning operation is carried out on aluminum (100 BHN). Cutting speed = 5.6 m/s, feed = 0.25 mm/rev, and depth of cut = 2.0 mm. The lathe has a mechanical efficiency = 0.85. Based on the specific energy values in Table 21.2, determine (a) the cutting power and (b) gross power in the turning operation, in Watts. Solution: (a) From Table 21.2, U = 0.7 N-m/mm3 for aluminum. RMR = vfd = 5.6(103 )(.25)(2.0) = 2.8(103 ) mm3 /s.
• 149. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 141 Pc = U RMR = 0.7(2.8)(103 ) = 1.96(103 ) N-m/s = 1960 W (b) Gross power Pg = 1960/0.85 = 2306 W 21.28 Solve Problem 21.27 but with the following changes: cutting speed = 1.3 m/s, feed = 0.75 mm/rev, and depth = 4.0 mm. Note that although the power used in this operation is only about 10% greater than in the previous problem, the metal removal rate is about 40% greater. Solution: (a) From Table 21.2, U = 0.7 N-m/mm3 for aluminum. Since feed is greater than 0.25 mm/rev in the table, a correction factor must be applied from Figure 21.14. For f = 0.75 mm/rev = to, correction factor = 0.80. RMR = vfd = 1.3(103 )(.75)(4.0) = 3.9(103 ) mm3 /s. Pc = U RMR = 0.8(0.7)(3.9)(103 ) = 2.184(103 ) N-m/s = 2184 W (b) Gross power Pg = 2184/0.85 = 2569 W 21.29 A turning operation is performed on an engine lathe using a tool with zero rake angle in the direction of chip flow. The work material is an alloy steel with hardness = 325 Brinell hardness. The feed is 0.015 in/rev, depth of cut is 0.125 in and cutting speed is 300 ft/min. After the cut, the chip thickness ratio is measured to be 0.45. (a) Using the appropriate value of specific energy from Table 21.2, compute the horsepower at the drive motor, if the lathe has an efficiency = 85%. (b) Based on horsepower, compute your best estimate of the cutting force for this turning operation. Use the orthogonal cutting model as an approximation of the turning process. Solution: (a) From Table 21.2, U = Pu = 520,000 in-lb/in3 for alloy steel of the specified hardness. Since feed is greater than 0.010 in/rev in the table, a correction factor must be applied from Figure 21.14. For f = 0.015 in/rev = to, correction factor = 0.95. Thus, U = 520,000(0.95) = 494,000 in-lb/in3 = 41,167 ft-lb/in3 . RMR = 300 x 12(.015)(0.125) = 6.75 in3 /min Pc = U RMR = 41,167(6.75) = 277,875 ft-lb/min HPc = 277,875/33,000 = 8.42 hp HPg = 8.42/0.85 = 9.9 hp (b) HPc = vFc/33,000. Rearranging, Fc = 33,000 (HPc/v) = 33,000(8.42/300) = 926 lb. Check: Use unit horsepower from Table 21.2 rather than specific energy. HPu = 1.3 hp/(in3 /min). Applying the correction factor correction factor = 0.95, HPu = 1.235 hp/(in3 /min). RMR = 300 x 12(.015)(0.125) = 6.75 in3 /min, same as before HPc = 1.235(6.75) = 8.34 hp HPg = 8.34/0.85 = 9.8 hp (b) Fc = 33,000 (8.3/300) = 913 lb. 21.30 A lathe performs a turning operation on a workpiece of 6.0 in diameter. The shear strength of the work is 40,000 lb/in2 and the tensile strength is 60,000 lb/in2 . The rake angle of the tool is 6°. The cutting speed = 700 ft/min, feed = 0.015 in/rev, and depth = 0.090 in. The chip thickness after the cut is 0.025 in. Determine (a) the horsepower required in the operation, (b) unit horsepower for this material under these conditions, and (c) unit horsepower as it would be listed in Table 21.2 for a to of 0.010 in. Use the orthogonal cutting model as an approximation of the turning process. Solution: (a) Must find Fc and v to determine HP. r = 0.015/0.025 = 0.6 φ = tan-1 (0.6 cos 6/(1 - 0.6 sin 6)) = tan-1 (0.6366) = 32.5° β = 2(45) + α - 2(φ) = 90 + 6 -2(32.5) = 31.0° As = tow/sin φ = (0.015)(0.09)/sin 32.5 = 0.00251 in2 Fs = SAs = 40,000(0.00251) = 101 lb. Fc = Fs cos (β – α)/cos (φ + β – α)
• 150. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 142 Fc = 101 cos(31 - 6)/cos(32.5 + 31.0 – 6) = 170 lb. HPc = Fcv/33,000 = 170(700)/33,000 = 3.61 hp. (b) RMR = 700 x 12(0.0075)(0.075) = 11.3 in3 /min HPu = HPc /RMR = 3.61/11.3 = 0.319 hp/(in3 /min) (c) Correction factor = 0.85 from Fig. 21.14 to account for the fact that f = 0.015 in/rev instead of 0.010 in/rev. Taking this correction factor into account, HPu = 0.375/0.85 = 0.441 hp/(in3 /min) as it would appear in Table 21.2 for a feed (to) = 0.010 in/rev. 21.31 In a turning operation on an aluminum alloy workpiece, the feed = 0.020 in/rev, and depth of cut = 0.250 in. The motor horsepower of the lathe is 20 hp and it has a mechanical efficiency = 92%. The unit horsepower value = 0.25 hp/(in3 /min) for this aluminum grade. What is the maximum cutting speed that can be used on this job? Solution: From Table 21.3, HPu = 0.25 hp/(in3 /min) for aluminum. Since feed is greater than 0.010 in/rev in the table, a correction factor must be applied from Figure 21.14. For f = 0.020 in/rev = to, correction factor = 0.9. HPc = HPu x RMR, HPg = HPc/E RMR = vfd = 12v(.020)(0.250) = 0.06 v in3 /min HPc = 0.9(0.25)(0.06 v) = 0.0135 v hp HPg = 0.0135 v /0.92 = 0.014674 v = 20 hp v = 20/0.014674 = 1363 ft/min Cutting Temperature 21.32 Orthogonal cutting is performed on a metal whose mass specific heat = 1.0 J/g-C, density = 2.9 g/cm3 , and thermal diffusivity = 0.8 cm2 /s. The cutting speed is 4.5 m/s, uncut chip thickness is 0.25 mm, and width of cut is 2.2 mm. The cutting force is measured at 1170 N. Using Cook's equation, determine the cutting temperature if the ambient temperature = 22°C. Solution: ρC = (2.9 g/cm3 )(1.0 J/g-°C) = 2.90 J/cm3 -°C = (2.90x10-3 ) J/mm3 -°C K = 0.8 cm2 /s = 80 mm2 /s U = Fcv/RMR = 1170 N x 4.5 m/s/(4500 mm/s x 0.25 mm x 2.2 mm) = 2.127 N-m/mm3 T = 0.4U/(ρC) x (vto/K)0.333 T = 22 + (0.4 x 2.127 N-m/mm3 /(2.90x10-3 ) J/mm3 -C) [4500 mm/s x 0.25 mm/80 mm2 /s]0.333 T = 22 + (0.2934 x 103 C)(14.06).333 = 22 + 293.4(2.41) = 22° + 707° = 729°C 21.33 Consider a turning operation performed on steel whose hardness = 225 HB at a speed = 3.0 m/s, feed = 0.25 mm, and depth = 4.0 mm. Using values of thermal properties found in the tables and definitions of Section 4.1 and the appropriate specific energy value from Table 21.2, compute an estimate of cutting temperature using the Cook equation. Assume ambient temperature = 20°C. Solution: From Table 21.2, U = 2.2 N-m/mm3 = 2.2 J/mm3 From Table 4.1, ρ = 7.87 g/cm3 = 7.87(10-3 ) g/mm3 From Table 4.1, C = 0.11 Cal/g-°C. From note “a” at the bottom of the table, 1 cal = 4.186 J. Thus, C = 0.11(4.186) = 0.460 J/ g-°C ρC = (7.87 g/cm3 )(0.46 J/g-°C) = 3.62(10-3 ) J/mm3 -°C From Table 4.2, thermal conductivity k = 0.046 J/s-mm-°C From Eq. (4.3), thermal diffusivity K = k/ρC K = 0.046 J/s-mm-°C /[(7.87 x 10-3 g/mm3 )(0.46 J/g-°C)] = 12.7 mm2 /s Using Cook’s equation, to = f = 0.25 mm T = (0.4(2.2)/3.62(10-3 ))[3(103 )(0.25)/12.7]0.333 = 0.2428(103 )(59.06)0.333 = 242.8(3.89) = 944.4 C° Final temperature, taking ambient temperature in account T = 20 + 944 = 964°C
• 151. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 143 21.34 An orthogonal cutting operation is performed on a certain metal whose volumetric specific heat = 110 in-lb/in3 -F, and thermal diffusivity = 0.140 in2 /sec. The cutting speed = 350 ft/min, chip thickness before the cut = 0.008 in, and width of cut = 0.100 in. The cutting force is measured at 200 lb. Using Cook's equation, determine the cutting temperature if the ambient temperature = 70°F. Solution: v = 350 ft/min x 12 in/ft/60 sec/min = 70 in/sec. U = Fcv/vtow = 200(70)/(70 x 0.008 x 0.100) = 250,000 in-lb/in3 . T = 70 + (0.4U/ρC)(vto/K)0.333 = T = 70 + (0.4 x 250,000/110)[70 x 0.008/0.14]0.333 = 70 + (909)(4)0.333 = 70 + 1436 = 1506°F 21.35 It is desired to estimate the cutting temperature for a certain alloy steel whose hardness = 240 Brinell. Use the appropriate value of specific energy from Table 21.2 and compute the cutting temperature by means of the Cook equation for a turning operation in which the cutting speed is 500 ft/min, feed is 0.005 in/rev, and depth of cut is 0.070 in. The work material has a volumetric specific heat of 210 in lb/in3 -F and a thermal diffusivity of 0.16 in2 /sec. Assume ambient temperature = 88°F. Solution: From Table 21.2, U for alloy steel (310 BHN) = 320,000 in-lb/in3 . Since f = 0.005 in/rev, correction factor = 1.25. Therefore U = 320,000(1.25) = 400,000 in-lb/in3 . v = 500 ft/min x 12 in/ft/60 sec/min = 100 in/sec. T = Ta + (0.4U/ρC)(vto/K)0.333 = 88 + (0.4 x 400,000/210)(100 x 0.005/0.16)0.333 = 88 + (762)(3.125)0.333 = 88 + 1113 = 1201°F 21.36 An orthogonal machining operation removes metal at 1.8 in3 /min. The cutting force in the process = 300 lb. The work material has a thermal diffusivity = 0.18 in2 /sec and a volumetric specific heat = 124 in-lb/in3 -F. If the feed f = to = 0.010 in and width of cut = 0.100 in, use the Cook formula to compute the cutting temperature in the operation given that ambient temperature = 70°F. Solution: RMR = vtow, v = RMR/tow = 1.8/(0.01 x 0.100) = 1800 in/min = 30 in/sec U = Fcv/vtow = 300(30)/(30 x 0.010 x 0.100) = 300,000 in-lb/in3 . T = 70 + (0.4U/ρC)(vto/K)0.333 = 70 + (0.4 x 300,000/124)(30 x 0.010/0.18)0.333 = 70 + (968)(1.667)0.333 = 70 + 1147 = 1217°F 21.37 A turning operation uses a cutting speed = 200 m/min, feed = 0.25 mm/rev, and depth of cut = 4.00 mm. The thermal diffusivity of the work material = 20 mm2 /s and the volumetric specific heat = 3.5 (10-3 ) J/mm3 -C. If the temperature increase above ambient temperature (20°F) is measured by a tool-chip thermocouple to be 700°C, determine the specific energy for the work material in this operation. Solution: Rearranging the Cook equation, U = T(ρC/0.4)(K/vto)0.333 U = (700 – 20)(3.5 x 10-3 /0.4)(20/{(200/60)(103 )(0.25)})0.333 U = 680(8.75 x 10-3 )(0.024)0.333 = 5.95(0.2888) = 1.72 N-m/mm3 21.38 During a turning operation, a tool-chip thermocouple was used to measure cutting temperature. The following temperature data were collected during the cuts at three different cutting speeds (feed and depth were held constant): (1) v = 100 m/min, T = 505°C, (2) v = 130 m/min, T = 552°C, (3) v = 160 m/min, T = 592°C. Determine an equation for temperature as a function of cutting speed that is in the form of the Trigger equation, Eq. (21.23). Solution: Trigger equation T = Kvm Choose points (1) and (3) and solve simultaneous equations using T = Kvm as the model. (1) 505 = K(100)m and (3) 592 = K(160)m (1) ln 505 = ln K + m ln 100 and (3) ln 592 = ln K + m ln 160
• 152. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 144 Combining (1) and (3): ln 505 - m ln 100 = ln 592 - m ln 160 6.2246 – 4.6052 m = 6.3835 – 5.0752 m 0.47 m = 0.1589 m = 0.338 (1) K = 505/1000.338 = 505/4.744 = 106.44 (2) K = 592/1600.338 = 592/5.561 = 106.45 Use K = 106.45 Check equation with data point (2): T = 106.45(130)0.338 = 551.87°C (pretty close to the given value of 552°C).
• 159. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 02-07-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 At Di = 24 in, N=v/πD, v = NπD = (40 rev/min)(π24/12) = 251 ft/min RMR = vfd = (251 x 12)(0.015)(0.18) = 8.14 in3 /min 22.9 Solve Problem 22.8 except that the machine tool controls operate at a constant cutting speed by continuously adjusting rotational speed for the position of the tool relative to the axis of rotation. The rotational speed at the beginning of the cut = 40 rev/min, and is continuously increased thereafter to maintain a constant cutting speed. Solution: (a) Total metal removed VMR = 0.25πd(Do 2 - Di 2 ) = 0.25π(0.180)(38.02 – 24.02 ) = 122.7 in3 RMR is constant throughout cutting if v is constant. N=v/πD; v = NπD = (40 rev/min)(π38/12) = 398 ft/min RMR = vfd = (398 x 12)(0.015)(0.18) = 12.89 in3 /min Tm = VMR/RMR = 122.7/12.89 = 9.52 min Drilling 22.10 A drilling operation is to be performed with a 12.7 mm diameter twist drill in a steel workpart. The hole is a blind hole at a depth of 60 mm and the point angle is 118°. The cutting speed is 25 m/min and the feed is 0.30 mm/rev. Determine (a) the cutting time to complete the drilling operation, and (b) metal removal rate during the operation, after the drill bit reaches full diameter. Solution: (a) N = v/πD = 25(103 ) / (12.7π) = 626.6 rev/min fr = Nf = 626.6(0.30) = 188 mm/min A = 0.5D tan (90 – θ/2) = 0.5(12.7)tan(90 – 118/2) = 3.82 mm Tm = (d + A)/fr = (60 + 3.82)/188 = 0.339 min (b) RMR = 0.25πD2 fr = 0.25π(12.7)2 (188) = 23,800 mm3 /min 22.11 A two-spindle drill simultaneously drills a ½ in hole and a ¾ in hole through a workpiece that is 1.0 inch thick. Both drills are twist drills with point angles of 118°. Cutting speed for the material is 230 ft/min. The rotational speed of each spindle can be set individually. The feed rate for both holes must be set to the same value because the 2 spindles lower at the same rate. The feed rate is set so the total metal removal rate does not exceed 1.50 in3 /min. Determine (a) the maximum feed rate (in/min) that can be used, (b) the individual feeds (in/rev) that result for each hole, and (c) the time required to drill the holes. Solution: (a) Total RMR = 1.50 = 0.25πD1 2 fr + 0.25πD2 2 fr = 0.25π( D1 2 + D2 2 )fr 1.50 = 0.25π( 0.52 + 0.752 )fr = 0.638fr fr = 1.50/0.638 = 2.35 in/min (b) For 1/2 in hole, N = v/πD = 230/(0.50π/12) = 1757 For 3/4 in hole, N = v/πD = 230/(0.75π/12) = 1171 f = fr/N. For 1/2 hole, f = 2.35/1757 = 0.0013 in/rev For 3/4 hole, f = 2.35/1171 = 0.0020 in/rev (c) Must use maximum Allowance for the 2 drills. For 1/2 in hole, A = 0.5D tan (90 – θ/2) = 0.5(0.50) tan(90 – 118/2) = 0.150 in For 3/4 in hole, A = 0.5D tan (90 – θ/2) = 0.5(0.75) tan (90 – 118/2) = 0.225 in Tm= (t + A)/fr = (1.00 + 0.225)/2.35 = 0.522 min = 31.2 seconds 22.12 A NC drill press is to perform a series of through-hole drilling operations on a 1.75 in thick aluminum plate that is a component in a heat exchanger. Each hole is 3/4 in diameter. There are 100 holes in all, arranged in a 10 by 10 matrix pattern, and the distance between adjacent hole centers (along the square) = 1.5 in. The cutting speed = 300 ft/min, the penetration feed (z-direction) = 0.015 in/rev, and the traverse rate between holes (x-y plane) = 15.0 in/min. Assume that x-y moves are made at a distance of 0.50 in above the work surface, and that this distance must be included in
• 160. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 02-07-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 the penetration feed rate for each hole. Also, the rate at which the drill is retracted from each hole is twice the penetration feed rate. The drill has a point angle = 100°. Determine the time required from the beginning of the first hole to the completion of the last hole, assuming the most efficient drilling sequence will be used to accomplish the job. Solution: Time to drill each hole: N = 300 x 12/0.75π = 1527.7 rev/min fr = 1527.7(0.015) = 22.916 in/min Distance per hole = 0.5 + A + 1.75 A = 0.5(0.75) tan(90 – 100/2) = 0.315 in Tm = (0.5 + 0.315 + 1.75)/22.916 = 0.112 min Time to retract drill from hole = 0.112/2 = 0.056 min All moves between holes are at a distance = 1.5 in using a back and forth path between rows of holes. Time to move between holes = 1.5/15 = 0.1 min. With 100 holes, the number of moves between holes = 99. Total cycle time to drill 100 holes = 100(0.112 + 0.056) + 99(0.1) = 26.7 min 22.13 A gundrilling operation is used to drill a 9/64-in diameter hole to a certain depth. It takes 4.5 minutes to perform the drilling operation using high pressure fluid delivery of coolant to the drill point. The current spindle speed = 4000 rev/min, and feed = 0.0017 in/rev. In order to improve the surface finish in the hole, it has been decided to increase the speed by 20% and decrease the feed by 25%. How long will it take to perform the operation at the new cutting conditions? Solution: fr = Nf = 4000 rev/min (0.0017 in/rev) = 6.8 in/min Hole depth d = 4.5 min (6.8 in/min) = 30.6 in New speed v = 4000(1 + 0.20) = 4800 rev/min New feed f = 0.0017(1- 0.25) = 0.001275 in/min New feed rate fr = 4800(0.001275) = 6.12 in/min New drilling time Tm = 30.6/6.12 in/min = 5.0 min Milling 22.14 A peripheral milling operation is performed on the top surface of a rectangular workpart which is 400 mm long by 60 mm wide. The milling cutter, which is 80 mm in diameter and has five teeth, overhangs the width of the part on both sides. Cutting speed = 70 m/min, chip load = 0.25 mm/tooth, and depth of cut = 5.0 mm. Determine (a) the actual machining time to make one pass across the surface and (b) the maximum material removal rate during the cut. Solution: (a) N = v/πD = 70,000 mm/80π = 279 rev/min fr = Nntf = 279(5)(0.25) = 348 mm/min A = (d(D-d))0.5 = (5(80-5))0.5 = 19.4 mm Tm = (400 + 19.4)/348 = 1.20 min (b) RMR = wdfr = 60(5)(348) = 104,400 mm3 /min 22.15 A face milling operation is used to machine 6.0 mm from the top surface of a rectangular piece of aluminum 300 mm long by 125 mm wide in a single pass. The cutter follows a path that is centered over the workpiece. It has four teeth and is 150 mm in diameter. Cutting speed = 2.8 m/s, and chip load = 0.27 mm/tooth. Determine (a) the actual machining time to make the pass across the surface and (b) the maximum metal removal rate during cutting. Solution: (a) N = v/πD = (2800 mm/s)/150π = 5.94 rev/s fr = Nntf = 5.94(4)(0.27) = 6.42 mm/s
• 165. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 02-07-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 13 least one of the following conditions: (1) large volumes of metal removed from large parts, (2) multiple cutting operations requiring many different tools, and (3) complex shapes and hard materials (as in the die and mold industry).
• 170. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 (1) C = 125(20.4)0.3894 = 404.46 (2) C = 165(10.0)0.3894 = 404.46 C = 404.46 23.2 Solve Problem 23.1 except that the tool life criterion is 0.50 mm of flank land wear rather than 0.75 mm. Solution: (a) and (b) Student exercises. For part (a), at v1 = 125 m/min, T1 = 13.0 min using criterion FW = 0.50 mm, and at v2 = 165 m/min, T2 = 5.6 min using criterion FW = 0.50 mm. In part (b), values of C and n may vary due to variations in the plots. The values should be approximately the same as those obtained in part (c) below. (c) Two equations: (1) 125(13.0)n = C, and (2) 165(5.6)n = C (1) and (2) 125(13.0)n = 165(5.6)n ln 125 + n ln 13.0 = ln 165 + n ln 5.6 4.8283 + 2.5649 n = 5.1059 + 1.7228 n 0.8421 n = 0.2776 n = 0.3296 (1) C = 125(13.0)0.3894 = 291.14 (2) C = 165(5.6)0.3894 = 291.15 C = 291.15 23.3 A series of turning tests were conducted using a cemented carbide tool, and flank wear data were collected. The feed was 0.010 in/rev and the depth was 0.125 in. At a speed of 350 ft/min, flank wear = 0.005 in at 1 min, 0.008 in at 5 min, 0.012 in at 11 min, 0.0.015 in at 15 min, 0.021 in at 20 min, and 0.040 in at 25 min. At a speed of 450 ft/min, flank wear = 0.007 in at 1 min, 0.017 in at 5 min, 0.027 in at 9 min, 0.033 in at 11 min, and 0.040 in at 13 min. The last value in each case is when final tool failure occurred. (a) On a single piece of linear graph paper, plot flank wear as a function of time. Using 0.020 in of flank wear as the criterion of tool failure, determine the tool lives for the two cutting speeds. (b) On a piece of natural log-log paper, plot your results determined in the previous part. From the plot, determine the values of n and C in the Taylor Tool Life Equation. (c) As a comparison, calculate the values of n and C in the Taylor equation solving simultaneous equations. Are the resulting n and C values the same? Solution: (a) Flank Wear vs Time 0.000 0.005 0.010 0.015 0.020 0.025 0.030 0.035 0.040 0.045 0 5 10 15 20 25 30 Time (min) FlankWear(in) Flank v = 350 ft/min Flank v = 450 ft/min Using the graph, at 350 ft/min the tool last about 6.2 min; at 450 ft/min, it lasts 19.0 min. (b) The points are graphed in Excel and the line connecting the two points is extended to the axis.
• 171. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 Taylor Tool Life 10 100 1000 1 10 100 Tool Life (min) CuttingSpeed(ft/min) C is read from the Y-intercept and is approximately 680 ft/min. The slope, n, can be determined by taking the ln of the x and y coordinates of any 2 points and determining ΔY/ΔX. It is positive because the Taylor tool life equation is derived assuming the slope is negative. Using the points (1,680) and (19,350) the slope is about 0.226. (c) Depending on the values of tool life read from the flank wear graph, the values of n and C will vary. Two equations: (1) 350(19.0)n = C, and (2) 450(6.2)n = C (1) and (2) 350(19.0)n = 450(6.2)n ln 350 + n ln 19.0 = ln 450 + n ln 6.2 5.8579 + 2.9444 n = 6.1092 + 1.8245 n 1.1199 n = 0.2513 n = 0.224 (1) C = 350(19.0)0.224 = 677 (2) C = 450(6.2)0.224 = 677 C = 677 23.4 Solve problem 23.3 except the tool life wear criterion is 0.015 in of flank wear. What cutting speed should be used to get 20 minutes of tool life? Solution: Reading the time of tool failure on the Flank Wear vs Time plot yields the following data points. Note the values of n and C will change based on the estimates for time of failure. v1 = 350 ft/min, T1 = 15 min and v2 = 450 ft/min, T2 = 4.2 min Two equations: (1) 350(15.0)n = C, and (2) 450(4.2)n = C (1) and (2) 350(15.0)n = 450(4.2)n ln 350 + n ln 15.0 = ln 450 + n ln 4.2 5.8579 + 2.7081 n = 6.1092 + 1.4351 n 1.2730 n = 0.2513 n = 0.197 (1) C = 350(15.0)0.197 = 597 (2) C = 450(4.2)0.197 = 597 C = 597 To achieve 20 min of tool life: v = C/Tn = 597/200.197 = 597/1.8065 = 330 ft/min
• 172. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 23.5 Tool life tests on a lathe have resulted in the following data: (1) at a cutting speed of 375 ft/min, the tool life was 5.5 min; (2) at a cutting speed of 275 ft/min, the tool life was 53 min. (a) Determine the parameters n and C in the Taylor tool life equation. (b) Based on the n and C values, what is the likely tool material used in this operation? (c) Using your equation, compute the tool life that corresponds to a cutting speed of 300 ft/min. (d) Compute the cutting speed that corresponds to a tool life T = 10 min. Solution: (a) VTn = C; Two equations: (1) 375(5.5)n = C and (2) 275(53)n = C 375(5.5)n = 275(53)n 375/275 = (53/5.5)n 1.364 = (9.636)n ln 1.364 = n ln 9.636 0.3102 = 2.2655 n n = 0.137 C = 375(5.5)0.137 = 375(1.2629) C = 474 Check: C = 275(53)0.137 = 275(1.7221) = 474 (b) Comparing these values of n and C with those in Table 23.2, the likely tool material is high speed steel. (c) At v = 300 ft/min, T = (C/v)1/n = (474/300)1/0.137 = (1.579)7.305 = 28.1 min (d) For T = 10 min, v = C/Tn = 474/100.137 = 474/1.371 = 346 ft/min 23.6 Tool life tests in turning yield the following data: (1) when cutting speed is 100 m/min, tool life is 10 min; (2) when cutting speed is 75 m/min, tool life is 30 min. (a) Determine the n and C values in the Taylor tool life equation. Based on your equation, compute (b) the tool life for a speed of 110 m/min, and (c) the speed corresponding to a tool life of 15 min. Solution: (a) Two equations: (1) 120(7)n = C and (2) 80(28)n = C. 120(7)n = 80(28)n ln 120 + n ln 7 = ln 80 + n ln 28 4.7875 + 1.9459 n = 4.3820 + 3.3322 n 4.7875 - 4.3820 = (3.3322 – 1.9459) n 0.4055 = 1.3863 n n = 0.2925 C = 120(7)0.2925 = 120(1.7668) C = 212.0 Check: C = 80(28)0.2925 = 80(2.6503) = 212.0 (b) 110 T0.2925 = 212.0 T0.2925 = 212.0/110 = 1.927 T = 1.9271/0.2925 = 1.9273.419 = 9.42 min (c) v (15)0.2925 = 212.0 v = 212.0/(15)0.2925 = 212.0/2.2080 = 96.0 m/min 23.7 Turning tests have resulted in 1-min tool life at a cutting speed = 4.0 m/s and a 20-min tool life at a speed = 2.0 m/s. (a) Find the n and C values in the Taylor tool life equation. (b) Project how long the tool would last at a speed of 1.0 m/s. Solution: (a) For data (1) T = 1.0 min, then C = 4.0 m/s = 240 m/min For data (2) v = 2 m/s = 120 m/min 120(20)n = 240 20n = 240/120 = 2.0 n ln 20 = ln 2.0 2.9957 n = 0.6931 n = 0.2314 (b) At v = 1.0 m/s = 60 m/min 60(T)0.2314 = 240
• 173. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 (T)0.2314 = 240/60 = 4.0 T = (4.0)1/0.2314 = (4)4.3215 = 400 min 23.8 A 15.0-in-by-2.0-in-workpart is machined in a face milling operation using a 2.5 in diameter fly cutter with a single carbide insert. The machine is set for a feed of 0.010 in/tooth and a depth of 0.20 in. If a cutting speed of 400 ft/min is used, the tool lasts for 3 pieces. If a cutting speed of 200 ft/min is used, the tool lasts for 12 parts. Determine the Taylor tool life equation. Solution: N1 =v/πD = 400(12)/2.5π = 611 rev/min fr = Nfnt = 611(0.010)(1) = 6.11 in/min From Eq. (22.18) in the previous chapter, A = 0.5(2.5 – (2.52 – 2.02 )0.5 ) = 0.5 in Tm = (L+A)/fr = (15 + 0.5))/6.11 = 2.537 min T1 = 3Tm = 3(2.537) = 7.61 min when v1 = 400 ft/min N2 = 200(12)/2.5π = 306 rev/min fr = Nfnt = 306(0.010)(1) = 3.06 in/min Tm = (15 + 0.5))/3.06 = 5.065 min T2 = 12Tm = 12(5.065) = 60.78 min when v2 = 200 ft/min n = ln (v1/v2)/ln(T2/T1) = ln (400/200)/ln (60.78/7.61) = 0.3336 C = vTn = 400(7.61 )0.3336 = 787.2 23.9 In a production turning operation, the workpart is 125 mm in diameter and 300 mm long. A feed of 0.225 mm/rev is used in the operation. If cutting speed = 3.0 m/s, the tool must be changed every 5 workparts; but if cutting speed = 2.0 m/s, the tool can be used to produce 25 pieces between tool changes. Determine the Taylor tool life equation for this job. Solution: (1) Tm = π(125 mm)(0.3 m)/(3.0 m/s)(0.225 mm) = 174.53 s = 2.909 min T = 5(2.909) = 14.54 min (2) Tm = π(125 mm)(0.3 m)/(2.0 m/s)(0.225 mm) = 261.80s = 4.363 min T = 25(4.363) = 109.08 min (1) v = 3 m/s = 180 m/min (2) v = 2 m/s = 120 m/min (1) 180(14.54)n = C (2) 120(109.08)n = C 180(14.54)n = 120(109.08)n ln 180 + n ln(14.54) = ln 120 + n ln(109.08) 5.1929 + 2.677 n = 4.7875 + 4.692 n 5.1929 - 4.7875 = (4.692 - 2.677) n 0.4054 = 2.0151 n n = 0.2012 C = 180 (14.54)0.2012 C = 308.43 23.10 For the tool life plot of Figure 23.5, show that the middle data point (v = 130 m/min, T = 12 min) is consistent with the Taylor equation determined in Example Problem 23.1. Solution: Taylor equation calculated in Example 23.1 is: vT0.223 = 229. Consistency would be demonstrated by using the values from the middle data point (T = 12 min at v = 130 ft/min) in the equation and obtaining the same value of C as above (C = 229). 130(12)0.223 = 130(1.7404) = 226.3 This represents a difference of less than 1.2%, which is close enough and well within expected random variation in typical tool life data. 23.11 In the tool wear plots of Figure 23.4, complete failure of the cutting tool is indicated by the end of each wear curve. Using complete failure as the criterion of tool life instead of 0.50 mm flank wear, the resulting data are: (1) v = 160 m/min, T = 5.75 min; (2) v = 130 m/min, T = 14.25 min; and (3) v
• 174. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 9 = 100 m/min, T = 47 min. Determine the parameters n and C in the Taylor tool life equation for this data. Solution: Let us use the two extreme data points to calculate the values of n and C, then check the resulting equation against the middle data point. (1) 160(5.75)n = C and (3) 100(47)n = C 160(5.75)n = 100(47)n ln 160 + n ln 5.75 = ln 100 + n ln 47 5.0752 + 1.7492 n = 4.6052 + 3.8501 n 0.4700 = 2.1009 n n = 0.224 (1) C = 160(5.75)0.224 = 236.7 (3) C = 100(47)0.224 = 236.9 use average: C = 236.8 Check against data set (2): 130(14.25)0.224 = 235.7. This represents a difference of less than 0.5%, which would be considered good agreement for experimental data. Better results on determining the Taylor equation would be obtained by using regression analysis on all three data sets to smooth the variations in the tool life data. Note that the n value is very close to the value obtained in Example 23.1 (n = 0.224 here vs. n = 0.223 in Example 23.1), and that the C value is higher here (C = 236.8 here vs. C = 229 in Example 23.1). The higher C value here reflects the higher wear level used to define tool life (complete failure of cutting edge here vs. a flank wear level of 0.50 mm in Example 23.1). 23.12 The Taylor equation for a certain set of test conditions is vT.25 = 1000, where the U.S. customary units are used: ft/min for v and min for T. Convert this equation to the equivalent Taylor equation in the International System of units (metric), where v is in m/sec and T is in seconds. Validate the metric equation using a tool life = 16 min. That is, compute the corresponding cutting speeds in ft/min and m/sec using the two equations. Solution: vT0.25 = 1000(Tref)0.25 C = 1000 ft/min for a 1.0 min tool life; ft/min converts to m/s as (1000 ft/min)(0.3048m/ft)(1 min/60 s) = 5.08 m/s Tref = 1 min = 60 s. (Tref)0.25 = (60)0.25 = 2.78316 The converted value of C = 5.08(2.78316) = 14.14 The converted equation is: vT0.25 = 14.14, where v = m/s and T = s. Check both equations at T = 16 min = 960 s. USCU: v = 1000/160.25 = 1000/2 = 500 ft/min SI: v = 14.14/9600.25 = 14.14/5.566 = 2.54 m/s Check: (500 ft/min)( 0.3048m/ft)(1 min/60 s) = 2.54 m/s Q.E.D. 23.13 A series of turning tests are performed to determine the parameters n, m, and K in the expanded version of the Taylor equation, Eq. (23.4). The following data were obtained during the tests: (1) cutting speed = 1.9 m/s, feed = 0.22 mm/rev, tool life = 10 min; (2) cutting speed = 1.3 m/s, feed = 0.22 mm/rev, tool life = 47 min; and (3) cutting speed = 1.9 m/s, feed = 0.32 mm/rev, tool life = 8 min. (a) Determine n, m, and K. (b) Using your equation, compute the tool life when the cutting speed is 1.5 m/s and the feed is 0.28 mm/rev. Solution: Three equations to be solved simultaneously: (1) (1.9 x 60)(10)n (0.22)m = K (2) (1.3 x 60)(47)n (0.22)m = K (3) (1.9 x 60)(8)n (0.32)m = K (1) and (2): ln 114 + n ln 10 + m ln 0.22 = ln 78 + n ln 47 + m ln 0.22 ln 114 + n ln 10 = ln 78 + n ln 47
• 175. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 10 4.7362 + 2.3026 n = 4.3567 + 3.8501 n 0.3795 = 1.548 n n = 0.245 (1) and (3): ln 114 + 0.245 ln 10 + m ln 0.22 = ln 114 + 0.245 ln 8 + m ln 0.32 0.5646 + m (-1.5141) = 0.5099 + m (-1.1394) -0.3747 m = -0.0547 m = 0.146 (1) K = 114(10)0..245 (0.22)0.146 =114(1.7588)(0.8016) = K = 160.7 (b) v = 1.5 m/s, f = 0.28 mm/rev (1.5 x 60)(T)0.245 (0.28)0.146 = 160.7 90(T)0.245 (0.8304) = 160.7 (T)0.245 = 2.151 T = 2.1511/0.245 = 22.7 min 23.14 Eq. (23.4) in the text relates tool life to speed and feed. In a series of turning tests conducted to determine the parameters n, m, and K, the following data were collected: (1) v = 400 ft/min, f = 0.010 in/rev, T = 10 min; (2) v = 300 ft/min, f = 0.010 in/rev, T = 35 min; and (3) v = 400 ft/min, f = 0.015 in/rev, T = 8 min. Determine n, m, and K. What is the physical interpretation of the constant K? Solution: Three equations to be solved simultaneously: (1) 400(10)n (0.010)m = K (2) 300(35)n (0.010)m = K (3) 400(8)n (0.015)m = K (1) and (2): ln 400 + n ln 10 + m ln 0.010 = ln 300 + n ln 35 + m ln 0.010 ln 400 + n ln 10 = ln 300 + n ln 35 5.9915 + 2.3026 n = 5.7038 + 3.5553 n 0.2877 = 1.2527 n n = 0.2297 (1) and (3): ln 400 + n ln 10 + m ln 0.010 = ln 400 + n ln 8 + m ln 0.015 n ln 10 + m ln 0.010 = n ln 8 + m ln 0.015 0.2297(2.3026) + m (-4.6052) = 0.2297(2.0794) + m (-4.1997) 0.2297(2.3026 - 2.0794) = m(-4.1997 + 4.6052) 0.05127 = 0.4055 m m = 0.1264 (1) K = 400(10)0.2297 (0.010)0.1264 = 400(1.6971)(0.5587) = 379.3 (2) K = 300(35)0.2297 (0.010)0.1264 = 300(2.2629)(0.5587) = 379.3 (3) K = 400(8)0.2297 (0.015)0.1264 = 400(1.6123)(0.5881) = 379.3 K = 379.3 The constant K represents the cutting speed (ft/min) for a 1.0 minute tool life at a feed rate of 1.0 in/rev. This feed is of course an extrapolation and not a real possible feed value. 23.15 The n and C values in Table 23.2 are based on a feed rate of 0.25 mm/rev and a depth of cut = 2.5 mm. Determine how many cubic mm of steel would be removed for each of the following tool materials, if a 10-min tool life were required in each case: (a) plain carbon steel, (b) high speed steel, (c) cemented carbide, and (d) ceramic. Use of a spreadsheet calculator is recommended. Solution: (a) Plain carbon steel: n = 0.10, C = 20 m/min v = 20/100.1 = 20/1.259 = 15.886 m/min RMR = 15.886(103 )(0.25)(2.50) = 9.9288(103 ) m3 /min For 10 min, metal removed = 10(9.9288)(103 ) = 99.288(103 ) mm3 (b) HSS: n = 0.125, C = 70 m/min v = 70/100.125 = 70/1.333 = 52.513 m/min RMR = 52.513(103 )(0.25)(2.50) = 32.821(103 ) mm3 /min
• 176. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 11 For 10 min, metal removed = 10(32.821(103 )) = 328.21(103 ) mm3 (c) Cemented carbide: n = 0.25, C = 500 m/min v = 500/100.25 = 500/1.778 = 281.215 m/min RMR = 281.215(103 )(0.25)(2.50) = 175.759(103 ) mm3 /min For 10 min, metal removed = 10(175.759(103 )) = 1,757.59(103 )) mm3 (d) Ceramic: n = 0.60, C = 3000 m/min v = 3000/100.6 = 3000/3.981 = 753.58 m/min RMR = 753.58 (103 )(0.25)(2.50) = 470.987(103 ) mm3 /min For 10 min, metal removed = 10(470.987 (103 )) = 4,709.87(103 ) mm3 23.16 A drilling operation is performed in which 0.5 in diameter holes are drilled through cast iron plates that are 1.0 in thick. Sample holes have been drilled to determine the tool life at two cutting speeds. At 80 surface ft/min, the tool lasted for exactly 50 holes. At 120 surface ft/min, the tool lasted for exactly 5 holes. The feed of the drill was 0.003 in/rev. (Ignore effects of drill entrance and exit from the hole. Consider the depth of cut to be exactly 1.00 in, corresponding to the plate thickness.) Determine the values of n and C in the Taylor tool life equation for the above sample data, where cutting speed v is expressed in ft/min, and tool life T is expressed in min. Solution: (1) v = 80 ft/min, N = (80)/(0.5π/12) = 611 rev/min feed rate fr = (0.003)(611) = 1.833 in/min time per hole Tm = 1.0 in/(1.833 in/min) = 0.545 min for 50 holes, T = 50(0.545 min) = 27.25 min Formulating the data as vTn = C, we have: 80(27.25)n = C (2) v = 120 ft/min, N = (120)/(.5π/12) = 917 rev/min feed rate fr = (0.003)(917) = 2.75 in/min time per hole Tm = 1.0 in/(2.75 in/min) = 0.364 min for 5 holes, T = 5(0.364 min) = 1.82 min Formulating the data as vTn = C, we have: 120(1.82)n = C Setting (1) = (2): 80(27.25)n = 120(1.82)n ln 80 + n ln 27.25 = ln 120 + n ln 1.82 4.382 + 3.3051 n = 4.7875 + 0.5978 n 2.7073 n = 0.4055 n = 0.15 C = 80(27.25)0.15 = 80(1.6417) = 131.34 C = 120(1.82)0.15 = 120(1.094) = 131.29 C = 131.32 23.17 The outside diameter of a cylinder made of titanium alloy is to be turned. The starting diameter is 400 mm and the length is 1100 mm. The feed is 0.35 mm/rev and the depth of cut is 2.5 mm. The cut will be made with a cemented carbide cutting tool whose Taylor tool life parameters are: n = 0.24 and C = 450. Units for the Taylor equation are min for tool life and m/min for cutting speed. Compute the cutting speed that will allow the tool life to be just equal to the cutting time for this part. Solution: In this problem we want Tm = T, where Tm = machining time per piece and T = tool life. Both of these times must be expressed in terms of cutting speed. Tm = πDL/fv and T = (C/v)1/n Tm = π(400)(1100)(10-6 )/0.35(10-3 )v = 3949/v = 3949 (v)-1 T = (450/v)1/.24 = (450/v)4.1667 = 4504.1667 (v)-4.1667 = 1135(108 )(v)-4.1667 Setting Tm = T: 3949 v-1 = 1135(108 )(v)-4.1667 v3.1667 = 0.2874(108 ) v = {0.2874(108 )}1/3.1667 = {0.2874(108 )}0.3158 = 226.6 m/min Check: Tm = 3949 (226.6)-1 = 17.4 min
• 177. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 12 T = (450/226.6)1/.24 = (450/226.6)4.1667 = 17.4 min 23.18 The outside diameter of a roll for a steel rolling mill is to be turned. In the final pass, the starting diameter = 26.25 in and the length = 48.0 in. The cutting conditions will be: feed = 0.0125 in/rev, and depth of cut = 0.125 in. A cemented carbide cutting tool is to be used and the parameters of the Taylor tool life equation for this setup are: n = 0.25 and C = 1300. Units for the Taylor equation are min for tool life and ft/min for cutting speed. It is desirable to operate at a cutting speed so that the tool will not need to be changed during the cut. Determine the cutting speed that will make the tool life equal to the time required to complete the turning operation. Solution: In this problem we want Tm = T, where Tm = machining time per piece and T = tool life. Both of these times must be expressed in terms of cutting speed. Tm = πDL/12fv and T = (C/v)1/n Tm = π(26.25)(48.0)/12(0.0125)v = 26,389.38/v = 26,389.38(v)-1 T = (1300/v)1/.25 = (1300/v)4.0 = 13004.0 (v)-4.0 = 2.8561(1012 )(v)-4.0 Setting Tm = T: 26,389.38(v)-1 = 2.8561(1012 )(v)-4.0 v3.0 = 1.08229(108 ) v = {1.08229(108 )}1/3 = {1.08229(108 )}0.3333 = 476.56 ft/min Check: Tm = 26,389.38 (476.56)-1 = 55.375 min T = (1300/476.56)1/.25 = (1300/476.56)4.0 = 55.375 min 23.19 The workpart in a turning operation is 88 mm in diameter and 400 mm long. A feed of 0.25 mm/rev is used in the operation. If cutting speed = 3.5 m/s, the tool must be changed every 3 workparts; but if cutting speed = 2.5 m/s, the tool can be used to produce 20 pieces between tool changes. Determine the cutting speed that will allow the tool to be used for 50 parts between tool changes. Solution: (1) v = 3.5 m/s = 210 m/min Tm = π(0.088 m)(0.4 m)/(210 m/min)(0.00025 m) = 2.106 min T = 3(2.106) = 6.32 min (2) v = 2.5 m/s = 150 m/min Tm = π(0.088 m)(0.4 m)/(150 m/min)(0.00025 mm) = 2.949 min T = 20(2.949) = 58.98 min (1) 210(6.32)n = C (2) 150(58.98)n = C 210(6.32)n = 150(58.98)n ln 210 + n ln(6.32) = ln 150 + n ln(58.98) 5.347 + 1.844 n = 5.011 + 4.077 n 5.347 – 5.011 = (4.077 – 1.844) n 0.336 = 2.233 n n = 0.150 C = 210 (6.32)0.150 C = 277.15 Check: 150(58.98)0.150 = 277.03 ) Close enough. use C = 277.1 Set T = 50 Tm vT0.15 = 277.1, T0.15 = 277.1/v, T = (277.1/v)1/0.15 = (277.1/v)6.646 = 1.711415(10)16 /v6.646 Tm = π(0.088)(0.4)/0.00025 v = 442.34/v 1.711415(10)16 /v6.646 = 50(442.34/v) = 22116.8/v 1.711415(10)16 /v5.646 = 22116.8 v5.646 = 1.711415(10)16 /22116.8= 7.738075(10)11 = 773,807,500,000 v = (773,807,500,000)1/5.646 = (773,807,500,000)0.177122 = 127.57 m/min Check: Tm = 442.34/127.57 = 3.468 min, 50 Tm = 173.4 min T = (277.1/127.57)6.646 = (2.172)6.646 = 173.3 min (Close enough!)
• 178. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 13 23.20 In a production turning operation, the steel workpart has a 4.5 in diameter and is 17.5 in long. A feed of 0.012 in/rev is used in the operation. If cutting speed = 400 ft/min, the tool must be changed every four workparts; but if cutting speed = 275 ft/min, the tool can be used to produce 15 pieces between tool changes. A new order for 25 pieces has been received but the dimensions of the workpart have been changed. The new diameter is 3.5 in, and the new length is 15.0 in. The work material and tooling remain the same, and the feed and depth are also unchanged, so the Taylor tool life equation determined for the previous workparts is valid for the new parts. Determine the cutting speed that will allow one cutting tool to be used for the new order. Solution: (1) v = 400 ft/min Tm = π(4.5 in)(17.5 in)/(400 x 12 in/min)(0.012 in) = 4.295 min T = 4(4.295) = 17.18 min (2) v = 275 ft/min Tm = π(4.5 in)(17.5 in)/(275 x 12 in/min)(0.012 in) = 6.247 min T = 15(6.247) = 93.71 min (1) 400(17.18)n = C (2) 275(93.71)n = C 400(17.18)n = 275(93.71)n ln 400 + n ln(17.18) = ln 275 + n ln(93.71) 5.991 + 2.844 n = 5.617 + 4.540 n 5.991 - 5.617 = (4.540 - 2.844) n 0.374 = 1.696 n n = 0.2205 C = 400 (17.18)0.2205 C = 748.87 (ft/min) Check: 275(93.71)0.2205 = 748.43, use C = 748.65 Set T = 25 Tm vT0.2205 = 748.65, T0.2205 = 748.65/v, T = (748.65/v)1/0.2205 = (748.65/v)4.535 T = 10.8184(10)12 /v4.535 For the new part dimensions, Tm = π(3.5 in)(15 in)/(12v in/min)(0.012 in) = 1145.37/v 10.8184(10)12 /v4.535 = 25(1145.37/v) = 28634.25/v 10.8184(10)12 /v3.535 = 28634.25 v3.535 = 10.8184(10)12 /28634.25= 377,813,096.3 v = (377,813,096.3)1/3.535 = (377,813,096.3)0.2829 = 267.025 ft/min Check: Tm = 1145.37/267.025 = 4.289 min, 25 Tm = 107.23 min T = (748.65/267.025)4.535 = (2.804)4.535 = 107.23 min 23.21 The outside diameter of a cylinder made of a steel alloy is to be turned. The starting diameter is 300 mm and the length is 625 mm. The feed is 0.35 mm/rev and the depth of cut is 2.5 mm. The cut will be made with a cemented carbide cutting tool whose Taylor tool life parameters are: n = 0.24 and C = 450. Units for the Taylor equation are min for tool life and m/min for cutting speed. Compute the cutting speed that will allow the tool life to be just equal to the cutting time for three of these parts. Solution: In this problem we want 3Tm = T, where Tm = machining time per piece and T = tool life. Both of these times must be expressed in terms of cutting speed. Tm = πDL/fv and T = (C/v)1/n Tm = π(300)(625)(10-6 )/0.35(10-3 )v = 1683/v = 1683 (v)-1 3Tm = 3(1683 (v)-1 ) = 5049(v)-1 T = (450/v)1/.24 = (450/v)4.1667 = 4504.1667 (v)-4.1667 = 1135(108 )(v)-4.1667 Setting 3Tm = T: 5049v-1 = 1135(108 )(v)-4.1667 v3.1667 = 0.2248(108 ) v = {0.2248(108 )}1/3.1667 = {0.2248(108 )}0.3158 = 209.747 m/min
• 180. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 15 (c) Composite is a nonmetallic and would use group K (red). Precise machining would require a high hardness (lower number). (d) Steel would indicate the P (blue) group. Rough milling would indicate a higher toughness and thus a high number. 23.25 A turning operation is performed on a steel shaft with diameter = 5.0 in and length = 32 in. A slot or keyway has been milled along its entire length. The turning operation reduces the shaft diameter. For each of the following tool materials, indicate whether it is a reasonable candidate to use in the operation: (a) plain carbon steel, (b) high-speed steel, (c) cemented carbide, (d) ceramic, and (e) sintered polycrystalline diamond. For each material that is not a good candidate, give the reason why it is not. Solution: The lengthwise slot results in an interrupted cut, so toughness is important in the tool material. (a) Plain carbon steel: not economical because of low cutting speeds. (b) HSS: this is a reasonable candidate; it has good toughness for the interrupted cut. (c) Cemented carbide: this is a reasonable candidate; it must be a steel cutting grade with high toughness (high cobalt content). (d) Ceramic: this is not a good candidate because of its low toughness; it is likely to fracture during interrupted cutting. (e) Sintered polycrystalline diamond: SPD is not suitable for cutting steel. Cutting Fluids 23.26 In a milling operation with no coolant, a cutting speed of 500 ft/min is used. The current cutting conditions (dry) yield Taylor tool life equation parameters of n = 0.25 and C = 1300 (ft/min). When a coolant is used in the operation, the cutting speed can be increased by 20% and still maintain the same tool life. Assuming n does not change with the addition of coolant, what is the resulting change in the value of C? Solution: Find the present tool life T vTn = C; T = (C/v)(1/n) T = (1300/500)(1/.25) = 2.604.0 = 45.7 min After coolant, the new cutting speed would be 500(1+.20) = 600 If the tool life stays the same, C = vTn = 600(45.7).25 = 1560 % increase in C = (1560-1500)/1500 = 20% Note: When viewing the log-log plot of the Taylor tool life curve, it is a straight line. Since n, the slope, is not affected by the coolant, the coolant effectively raises the line on the graph. Raising the curve so that it increases the value of v by a certain percentage will increase C by the same percentage. This is true independent of the values of n and C. 23.27 In a turning operation using high-speed steel tooling, cutting speed = 110 m/min. The Taylor tool life equation has parameters n = 0.140 and C = 150 (m/min) when the operation is conducted dry. When a coolant is used in the operation, the value of C is increased by 15%. Determine the percent increase in tool life that results if the cutting speed is maintained at 110 m/min. Solution: Dry: 110(T)0.14 = 150 T = (150/110)1/.14 = (1.364)7.143 = 9.18 min With coolant: 110(T)0.14 = 150(1 + 15%) = 150(1.15) = 172.5 T = (172.5/110)1/.14 = (1.568)7.143 = 24.85 min Increase = (24.85 – 9.18)/9.18 = 1.71 = 171%
• 181. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 08-18-08 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 16 23.28 A production turning operation on a steel workpiece normally operates at a cutting speed of 125 ft/min using high-speed steel tooling with no cutting fluid. The appropriate n and C values in the Taylor equation are given in Table 23.2 in the text. It has been found that the use of a coolant type cutting fluid will allow an increase of 25 ft/min in the speed without any effect on tool life. If it can be assumed that the effect of the cutting fluid is simply to increase the constant C by 25, what would be the increase in tool life if the original cutting speed of 125 ft/min were used in the operation? Solution: From Table 23.2, n = 0.125 and C = 200 for dry cutting. With cutting fluid, C = 200 + 25 = 225. Dry: at v = 125 ft/min, T = (200/125)1/.125 = (1.6)8 = 42.95 min With cutting fluid: at v = 125 ft/min, T = (225/125)1/.125 = (1.8)8 = 110.2 min Increase = (110.2 - 42.95) = 67.25 min = 156.6% 23.29 A high speed steel 6.0 mm twist drill is being used in a production drilling operation on mild steel. A cutting oil is applied by the operator by brushing the lubricant onto the drill point and flutes prior to each hole. The cutting conditions are: speed = 25 m/min, and feed = 0.10 mm/rev, and hole depth = 40 mm. The foreman says that the "speed and feed are right out of the handbook" for this work material. Nevertheless, he says, "the chips are clogging in the flutes, resulting in friction heat, and the drill bit is failing prematurely due to overheating." What's the problem? What do you recommend to solve it? Solution: There are several problems here. First, the depth-to-diameter ratio is 1.75:0.25 = 7:1, which is greater than the 4:1 which is usually recommended. As a consequence the chips produced in the hole are having difficulty exiting, thus causing overheating of the drill. Second, the manual method of applying the cutting oil may not be particularly effective. Third, with overheating as a problem, the cutting oil may not be removing heat from the operation effectively. Recommendation: The 7:1 depth-to-diameter ratio is a given, a requirement of the drilling operation, and we assume it cannot be changed. The twist drill might be operated in a peck-drilling mode to solve the chip clogging problem. Peck-drilling means drilling for a distance approximately equal to one drill diameter, then retract the drill, then drill some more, etc. A twist drill with a fluid hole could be used to more effectively deliver the cutting fluid to the drill point to help extract the chips. Finally, an emulsified oil might be tried in the operation, one with good lubricating qualities, as a substitute for the cutting oil. Since overheating is a problem, it makes sense to try a coolant.